Embed Size (px)
WORKS OF PROF. M. A. HOWEPUBLISHED BY
JOHN WILEY & SONS, Inc.
A short Text-book on Masonry Construction, in-cluding Descriptions of the Materials Used, theirPreparation and Arrangement in Structures. 8vo,ix +160 pages. 115 figures. Cloth, $1.50 net.
A short Text-book on Ordinary Foundations,including a brief Description of the MethodsUsed for Difficurt Foundations. 8vo, vii + 110pages. 56 figures. Cloth, $1.25 net.
Influence Diagrams for the Determination of
Maximum Moments in Trusses and Beams
8vo, vii+65 pages, 42 figures. Cloth, $1.25 net.
The Design of Simple Roof=trusses in Wood andSteel.
With an Introduction to the Elements of GraphicStatics. Third edition, revised and enlarged.8vo, vi+173 pages, 124 figures and 3 foldingplates. Cloth, $1.80 net.
Retaining-walls for Earth.
Including the theory of Earth-pressure as Devel-oped from the Ellipse of Stress. With a ShortTreatise on Foundations. Illustrated with Ex-amples from Practice. Sixth edition, revisedand enlarged. 12mo, xv +194 pages, 110 figures.Cloth, $1.25 net.
A Treatise on Arches.
Designed for the use of Engineers and Studentsin Technical Schools. Second edition, revisedand enlarged. 8vo, xxv +369 pages, 74 figures.Cloth, $4.00 net.
Symmetrical Masonry Arches.
Including Natural Stone, Plain concrete and Rein-forced concrete arches, for the use of TechnicalSchools, Engineers and Computers .in DesigningArches according to the Elastic Theory. Secondedition, revised and enlarged. 8vo, xxiv -r245pages. Profusely illustrated with figures in thetext and folding plates. Cloth, $2.50 net.
MASONRYA Short Text-Book on Masonry Construction, Including
Descriptions of the Materials Used, their Prepa-
ration and Arrangement in Structures
MALVERD A. , C. E.
Professor of Civil Engineering, Rose Polytechnic Institute; Member American Societyof Civil Engineers, American Society for Testing Materials, Society for
the Promotion of Engineering Education, Fellow AmericanAssociation for the Advancement of Science
JOHN WILEY & SONS, INC.
LONDON: CHAPMAN & HALL, LIMITED
Copyright, 1915, by
MALVERD A. HOWE
PUBLISHERS PRINTING COMPANY207-217 West Twenty-fifth Street, New York
PREFACETHE following pages have been written to furnish a
concise treatment of masonry construction for use as a
text in courses of instruction which do not provide suf-
ficient time for the study of a more comprehensive
treatise. The matter as presented, however, may serve as
a skeleton for an extended course of study by making use
of the references at the end of the book which suggest
supplementary reading. The references are arranged in the
order in which the subject matter is considered in the text.
Modern methods are described and modern tools and
machinery are illustrated.
Reinforced concrete masonry has not been considered, as
there are numerous books which treat this subject both in
an elementary and in a thorough manner.
The specifications in Part III give the best modern
methods of selecting materials and their use in structures.
M. A. H.
PART I. THE MATERIALS
NATURAL BUILDING STONES
PAGENatural Building Stone -
Geological Classification of Rocks 1
Chemical Classification of Rocks 2
Classification of Rocks According to Their Physical Structure ... 2
Rocks Used for Building Stone . . . . . . . , . ... 2
Durability of Rocks . .- ... . . . 2
Artificial Methods of Determining the Durability of Rocks .... 3
The Absorption Test of Building Stones 3
The Crushing Strength of Building Stones 4
Freezing Tests of Building Stones . 5
Chemical Tests of Building Stones .6Microscopic Tests of Building Stones .6Determination of the Specific Gravity of Building Stones ..... 6
Minerals Which Are Injurious .7Granite ......... 7
Granular Limestone 9
Compact Limestone 9
Average Physical Properties of Building Stones ........ 11
Fire-Resisting Property of Stone 12
Quarrying '-....' . . . 12
Joints in Relation to Quarrying . . . . . . . . ^ . . .12Quarrying by Hand Tools . 13
Quarrying by Machinery 14
The Use of Explosives in Quarrying 14
Tools Used in Preparing Building Stones . . . ... . . . 20
Power Tools for Finishing Stone . . . . . . '. .-
.- . . . 24
Classification of Building Stones According to the Finish of the Surface . 28
Squared Stones 29
Cut Stones ... 30
ARTIFICIAL BUILDING MATERIALS
Building Brick 33
Manufacture of Building Brick ..... ...... 33
Drying Brick ...... 34
Burning Brick 36
Modern Methods of Burning Brick 37
Fuel Used in Burning Brick 41
Annealing or Cooling Brick 41
Classification of Brick 41
Essential Requirements for Good Building Brick 43
Ornamental Face Brick 45
Sizes of Brick 45
Sand Lime Brick 45
Cement Bricks - 46
Hollow Terra-Cotta 46
Plaster Blocks 48
Fat or Quick Lime 48
Burning Lime 50
Natural Cement 50
Portland Cement 51
Iron-Ore Cement 52
Magnesia Cement . ... 52
Puzzolan Cement .52Manufacture of Portland Cement ...... . . . . .53Sand 53
Testing Sand. ... . . . . . . . .< . . . , . . .54Gravel 54
Voids in Sand and Gravel 56
Mortar . . ..
. . . .56Lime Mortar 1
Natural Cement Mortar 57
Portland Cement Mortar ... 57
Lime Paste Used with Cement Mortar . . . ... : . <. 57
Water-Tight Mortar . . ;58
Colored Cement Mortar . 58
Pointing Mortar 58
PART II. MASONRY
Masonry .......... ^ ...'..... 59
Classification of Stone Masonry 61
Ashlar Masonry . . . . . . . . . . . . ... . . 61
Dressing Joint Surfaces for Ashlar 62
Backing and Filling for Ashlar . . . . .63Bond 64
Relative Dimensions of Stones . 66
Setting Stone . . -. . . . . . . . . | . . . . . .66Pointing .70Joint Mortar 71
Pointing Mortar . .... .... . . .... ... .71Squared-Stone Masonry 71
Backing and Filling for Squared-Stone Masonry 72
Bond, Mortar, Sizes of Stones, etc., for Squared-Stone Masonry ... 72
Stope-Wall Masonry . . . . . . . 73
Stone Paving . ... f ........*.... 73
Specifications for Stone Paving .... . . .
. . . . .73Riprap 73
Strength of Stone Masonry . . . . . 73
Measurement of Stone Masonry 74
Water-proofing Stone Masonry . . . . / . . . ;,='*, . . 75
Cleaning Stone Masonry . 75
BRICK AND HOLLOW-TILE MASONRY
Brick Masonry "......... 76
Joints for Brick-work .............. 77
Mortar for Brick-work 77
Pointing Joints of Brick-work . . . . . . . . . . . . . 77
Bond in Brick-work . . . . . .... 78
Crushing Strength of Brick-work ........ . _. . . 81
Lintels Supporting Brick Masonry 82
Efflorescence . . . . . _. .."*.. ..... 82
Measuring Brick-work , 83
Waterproofing Brick Masonry 83
Cleaning Brick Masonry 83
Hollow-Tile Masonry 84
Reinforced Concrete ... .... . . . . . . . . 87
Reinforcing Concrete for Shrinkage, etc 87
Constituents of Concrete 88
Proportions of Materials for Concrete 88
Mixing Concrete 89
Machines for Mixing Concrete 90
Concrete Building Blocks 91
Architectural Concrete 93
Surface Finish for Concrete Blocks 95
Monolithic and Mass Concrete 95
Depositing Concrete in Mass Construction 96
Mixing and Depositing Concrete by Compressed Air 98
Mixing and Depositing Grout by Compressed Air 100
Mixing and Depositing Concrete in Freezing Weather 101
Depositing Concrete Under Water 102
Finishing the Surface of Concrete 104
Bush-Hammer Surface Finish 105
Spaded Finish for Concrete Surfaces 105
Brushed Concrete Surfaces 105
Plaster Coats , 106
Sand-Blasted Surfaces ; . . ...... . . ... .107
Pebble Finish 107
Special Surface Finish for Concrete 107
Cement-Gun Surface Finish . .- 109
Forms for Mass Concrete ^. 110
Wetting and Oiling Forms Ill
Rubble Concrete . . . . . . . .... 112
Waterproofing Concrete 113
Tests of the Absorptive and Permeable Properties of Portland Cement
Mortars and Concretes 114
Waterproofing with Asphalt and Coal Tar . .118
Joining Old and New Concrete . . . 119
Effect of Alkali and Sea-water on Concrete 119
Physical Properties of Concrete 120
Fire-Resisting Property of Concrete 120
PART III. SPECIFICATIONS
RAILROAD MASONRY, BRICK CEMENT, ETC.
PAGEClassification of Railroad Masonry . . 121
Definitions ... . . .,
. . ..... . ... . 122
Specifications for Stone Masonry . . . ... . . . . . . 127
Specifications for Plain Concrete . . . 133
Specifications for Building Brick . . . . .... . . . .138
Specifications for Lime . . . 141
Specifications for Sand 143
Specifications for Cement . ... ... 144
Periodicals ;- 150
Books . . 153
MASONRYPART I. THE MATERIALS
NATURAL BUILDING STONES
Natural Building Stone is obtained from rock which has
been formed by natural processes. Its use for a particular
purpose depends upon its chemical and physical properties.
Rocks may be classified according to their geological posi-
tion, their chemical composition, or their physical structure.
Geological Classification of Rocks. The three geolog-
ical divisions of rocks are igneous, sedimentary, and
Igneous rocks are those which have been formed by"cooling from fusion," the melted rock having come up
through fissures in the earth's rocky crust. When the
melted rock has solidified on the surface, it is designated as
extrusive or volcanic. Lava is an example. When for
some reason the solidification takes place below the surface
the rock is designated as intrusive or plutonic. Granite is
Sedimentary or stratified rocks are those which have, in
general, been laid down under water by mechanical, organic,,
or chemical agents. This division also includes those rocks
which have been formed through the action of winds. The
shales and sandstones (water deposits) are examples of rocks
having mechanical origin; gypsum, rock salt, and some lime-
stones are examples of rocks having chemical origin formed
from solution; and numerous limestones and coal are ex-
amples of organic origin.
Metamorphic rocks have been formed from original
2 & * c*J ifA&ONRY
igneous or sedimentary rocks chiefly through the action of
heat, pressure, and water. Crystalline limestones are meta-
Chemical Classification of Rocks. Chemically, rocks are
divided into argillaceous, calcareous, and siliceous.
Argillaceous rocks are those in which alumina gives the
characteristic properties, slate being an example.Calcareous rocks or limestones are those which are prin-
cipally composed of carbonate of lime.
Siliceous rocks are those in which silica is the principal
constituent. Granite, quartzite (a siliceous sandstone), and
buhrstone (a cellular siliceous rock used for millstones) are
examples.Classification of Rocks According to Their Physical Struc-
ture. Rocks are classified according to their physical
structure as stratified and unstratified. A large number of
the limestones and sandstones are examples of the stratified
rocks, and basalt, granite, and lava examples of the un-
Rocks Used for Building Stone. The principal rocks
used for building purposes are granite, limestone, and sand-
stone. Trap-rock is used but little, owing to the difficulty
with which it is quarried and cut.
The selection of stone for a particular structure depends
upon a number of things which differ in different parts of
the country. The durability of the stone, if exposed to the*
weather, is of prime importance. For footings of heavystructures it must have the proper strength, and for build-
ings, etc., the question of color may be an important factor
governing the selection. The cost of quarrying, cutting, and
transporting will, of course, govern the choice between two
kinds of stone which are otherwise satisfactory.
Durability of Rocks. The durability of a rock depends
upon the closeness of its texture and the absence of any-
thing in its make-up which is liable to oxidation. Anyrock which is sufficiently porous to admit air or water will
degrade more or less to the depth of penetration of the air
NATURAL BUILDING STONES 6
or water. This is due partly to chemical action, and, in
cold climates, to alternate freezing and thawing.
Coarse-grained rocks are injured by alternate heating and
cooling in the daily passage of the sun. Rock which has been
protected by a layer of earth, and which shows the marks
of glacial action, will disintegrate on the surface when ex-
posed to the air, due to changes of temperature probably.
There is but one way, which is conclusive, to determine
the durability of a building stone in a particular locality,
and that is to examine it where it has been used in said
locality. It does not follow if a stone is durable in one
locality that it will be equally durable in another. This is
well illustrated by the almost perfect condition of the obel-
isks in Egypt, and the disintegration of Cleopatra's Needle
after it was transported, in 1880, to New York City.
In general, stones which absorb but little water, and those
having smooth surfaces exposed to the weather, are more
durable than those which absorb considerable water or have
rough surfaces exposed. There are a few exceptions to this
Artificial Methods of Determining the Durability of
Rocks. While not conclusive, artificial methods of deter-
mining the durability of rocks are, more or less, in general
use. These methods comprise the determination of the
amount of water the rock will absorb, the crushing strength,
the resistance to the action of frost, the solubility in acids,
a microscopical examination, and the determination of the
The Absorption Test of Building Stones. To determine
the amount of water which a stone will absorb in a given
period of time, a small piece is dried for twenty-four hours
at a temperature not lower than 212 F. The specimenis then weighed and placed in clean water for at least
twenty-four hours; then it is removed from the water, its
surface wiped fairly dry, and is again weighed. The differ-
ence between the wet and dry weights divided by the dry
weight is the percentage of absorption. As this test is com-
parative, the specimens should be of about the same size and
shape, and the time intervals the same for all specimens. Asair imprisoned in the stone will prevent the entrance of water,
the coefficient of absorption will be materially increased if
the dry specimen is placed under the receiver of an air pump,and the air exhausted. Complete saturation of a specimen
may be determined by repeated weighings while it is in the
The percentage of absorption should not exceed about
3 per cent. There are a few exceptions to this, however,where the percentage of absorption is as high as 6 per cent,
and the stones very durable.
The Crushing Strength of Building Stones. This is of
prime importance only for very heavy structures, but it is
an approximate guide to the durability of the stone, the
stronger stones being more durable than the weaker
To obtain the crushing strength of a stone, a specimenin the form of a cube is cut from the stone and crushed in
a testing machine designed for compressive tests. A record
is made when the first crack appears and when the specimenfails. For the best results, the specimens should be sawed
approximately to shape and then ground to the proper size.
The faces of the specimen should be planes, and the opposite
faces should be parallel. Steel plates without any beddingbetween them and the specimen should be used to transmit
the load. These conditions are difficult to obtain, so that
it is more or less customary to bed the specimens in plaster
of Paris, a piece of oiled paper being placed between the
plaster and the specimen.The use of cubical specimens is quite satisfactory when
only comparative strengths are wanted. The strengths ob-
tained from cubical specimens are in excess of the normal
strengths as obtained from prisms which are one and one-half
the least lateral dimension in height. Stratified stones are
usually tested with the stratifications horizontal.
For all ordinary structures, the building stones in common
NATURAL BUILDING STONES 5
use are very much stronger than necessary to carry the
Freezing Tests of Building Stones. Two methods are
followed for this test. In one, the stone is saturated with
water, frozen and thawed; and in the other, the action of
frost is artificially obtained by the action of Glauber's salts.
There appears to be no standard course of procedure in
either method. For the natural-freezing method, Baushingerused the practical process,
"consisting in the exposure of the
material twenty-five times to frost in the open air, the
(crushing) strength, before and after the test, serving as a
guide to the resisting power." (Van Nostrand's Engineering
Magazine, Vol. XXXIV, 1886, p. 44.)
For the natural method, the specimens may be two-inch
cubes. One set of specimens is thoroughly dried and tested
in compression. The other set is thoroughly dried and placed
in water for twelve hours, and then frozen. Cold-storage
plants are so common now that the specimens can be suffi-
ciently frozen in twelve hours. The soaking and freezing
are repeated from ten to twenty-five times, and then the
specimens are thoroughly dried and tested in compression.
The same soaking and freezing routine is followed if the
loss of weight is wanted. Usually, the loss of weight is verysmall.
The artificial-freezing test, or the sulphate of soda test,
is made in several ways. The following method is recom-
mended by Johnson (The Materials of Construction). Thesolution in which the specimens are immersed is a boiling
solution of the sulphate of soda, commonly known as
Glauber's salts. "The specimens should be heated before
immersion in the boiling liquid, or they should be immersed
before the liquid has come to the boiling temperature. Thetime of immersion need not be over thirty minutes, after
which the specimens should be freely suspended in the openair for twenty-four hours. They are then sprayed from a
wash-bottle and again immersed and boiled, this process
being repeated for any desired number of times, generally
from seven to ten. The specimens should be small, about
one-inch cubes being a suitable size, as the weighings have
to be done with great care on delicate balances to secure
reliable results. The specimens must be carefully dried
for twenty-four hours, at a temperature above boiling,
before the first weighing and after the long soaking in fresh
water subsequent to the tests."
The artificial test is much more severe on stone than the
natural test. Both tests are comparative and of little value.
A description of methods with discussion is given in a paperentitled "The Relative Effects of Frost, and the Sulphateof Soda Efflorescence Tests on Building Stones," by Lea
Mel. Luquer, Transactions of the American Society of Civil
Engineers, Vol. XXXIII, 1895, p. 235.
Chemical Tests of Building Stones. These appear to
have little value unless made for the determination of con-
stituents which may stain the stone, or in connection with
Microscopic Tests of Building Stones. This test, whenmade by an expert, is probably the most valuable of anyof those mentioned. The structural arrangement, the identi-
fication of its constituent parts, and the character of the
cementing material of the specimen are determined by this
Determination of the Specific Gravity of Building Stones.
The weight of building stone is of importance in all struc-
tures subjected to overturning forces and the pressure of
water, the heavier stones being better suited to resist such
A small specimen is thoroughly dried and weighed, then
saturated with water, and weighed again in the manner
described for the absorption test. The saturated specimenis then weighed in water. Letting W represent the dry
weight, W8 the saturated weight, and Ww the weight in
water, then the specific gravity, dry, equals Wl (Wa Ww),
and the specific gravity, wet, equals Wj'
(W8 Ww). The
weight per cubic foot is found by multiplying the weight
NATURAL BUILDING STONES 7
of a cubic foot of water (62.4 pounds, approximately) bythe specific gravity.
Minerals Which Are Injurious. Some minerals are in-
jurious under all conditions, while others are only injurious
when distributed in a particular manner.
Chert, or flint, forms the so-called glass seams in lime-
stone. It is very much harder than the surrounding stone
and, consequently, interferes with the cutting, and is muchmore resistant to the weather, forming ridges on weathered
stone. A glass seam which extends completely through the
stone does not affect its strength, but very often a seam
which appears on the surface only extends into the stone
a short distance, and beyond this point there may be an
open seam. Therefore, for durability, all stone with glass
seams should be rejected.
Mica occurs in granites, sandstones, and marbles, but
usually it is not harmful, especially if uniformly distributed
throughout the rock. In stratified rocks, it is harmful if
it is segregated along the planes of stratification. It is also
harmful in some of the crystalline limestones where it mayoccur as scattered grains or in bands. The scattered grains
do not do much harm, but bands injure the polish of marbles,
and also affect the durability of the stone, as the mica bands
do not weather well.
Pyrite and other iron sulphides, in small quantities, as
specks here and there in stone, do not do much harm. Asthe quantity increases, the exposure to the weather causes
pits, and, in many cases, the stone is stained. Stones which
contain iron as ferrous carbonate also stain.
Granite. As commonly used, the term granite includes
all igneous rocks and gneiss (gneiss has mica and other con-
stituents more or less in layers). According to Ries and
Watson, granite is an even granular, crystalline, plutonic,
igneous rock composed of quartz and alkalic feldspar (commonfeldspar), with usually mica, hornblende, or pyroxene.The quartz (oxygen and silica) is usually grayish white,
glassy, and without any appearance of cleavage. The feld-
spar (silica, alumina, and potash) is whitish or flesh-colored,
and is distinguished from the quartz by its cleavage surfaces
which reflect light brilliantly. The mica (silica, alumina,
potash +) is generally in small flat scales, either black,
brownish black, or silvery. The combined silica in the
quartz, feldspar, and mica constitutes over fifty per cent
of the rock.
The specific gravity of granite ranges from 2.5 to 2.8,
which corresponds to weights per cubic foot of 156 to 175
pounds.The crushing strength of granite is very variable, even for
stones from the same region. The range may be taken as
13,000 to 26,000 pounds per square inch, although some
granites have considerably less strength, and some a strength
as high as 43,000 pounds per square inch.
The modulus of rupture of granite, used as a beam over
an opening, for example, is about 1,800 pounds per squareinch. This is an average value.
Young's modulus of elasticity varies from 4,500,000 to
9,800,000 pounds per square inch in compression. This is
a very uncertain property, as it does not vary directly
with the compressive load. The loads corresponding to the
above values lie between 100 and 1,000 pounds per squareinch.
The coefficient of expansion for each degree Fahrenheit
ranges from .00000324 to .00000461.
The absorption of water by granite seldom exceeds one
Granites make very excellent building stones, and can be
used for all purposes from the bottom stones in a heavy
footing to the carved statuary of a building. The material
is one of the hardest to work, but modern methods have
done away with many difficulties which formerly existed.
The usual color of granite is gray, but pink and red granites
are more or less common.Limestone is stratified rock of sedimentary origin, and is
the general name for all of the massive varieties of calcite
NATURAL BUILDING STONES 9
(lime, carbon-dioxide +) which occur in extensive beds.
The principal constituent is carbonate of lime.
Granular Limestone, often called crystalline limestone, is
of metamorphic origin, and is composed of crystalline grains.
The coarser-grained stones are used in the construction of
marble buildings and the finer-grained stones for statuary.
The colors have a wide range; some of the more commoncolors are white, gray, black, red, pink, green, and yellow.
Compact Limestone breaks with a smooth, dull surface,
and does not show a distinct granular structure. When it
can be polished, some of it is very beautiful and is used as
marble. The famous oolitic limestones of Indiana belong
to the compact limestones.
The specific gravity of limestone ranges from 2.52 to 2.69,
corresponding to weights of 157 to 168 pounds per cubic
The crushing strength of limestone is very variable. The
greatest strength obtains for some stone when tested on
edge, and for others when tested on the bed. When specific
data are not obtainable, 10,000 pounds per square inch maybe considered a fair average value for the crushing strength.
The modulus of rupture varies from 300 to 2,700 pounds
per square inch.
Young's modulus of elasticity in compression ranges from
3,600,000 to 13,600,000 pounds per square inch, and, as is
the case for all stones, the values are true only for certain
The coefficient of expansion, for each degree Fahrenheit,
varies from .00000058 to .00000634.
The absorption of water may be less than one per cent or
over twelve per cent. The hard limestones usually absorb
less than two per cent of water, but many stones, widelyused and of excellent durability, have coefficients exceedingfour per cent.
Limestone is used for nearly all purposes in construction
where stone is suitable. The marbles are used for exterior
walls, interior finish, and for decorative purposes.
Sandstones and quartzites are generally composed of
grains cf quartz cemented together by some substance.
The quartz grains may be coarse or fine, and the cementingmaterial may be clay, calcium carbonate, iron oxide, or silica.
The cementing material affects the strength and color of
the stone. The buff and yellow colors are due to limonite
(brown hematite), the red and reddish brown colors are due
to hematite (specular iron ore), and the bluish gray andblack colors are due to clay or carbonaceous matter.
Sandstones always show a bedded structure. The layers
are sometimes horizontal, and sometimes tipped.
The specific gravity varies from 2.34 to 2.649, correspondingto weights of 146 to 165 pounds per cubic foot.
The crushing strength, as in the case of limestones, is very
variable, ranging from 4,300 to 19,000 pounds per square inch.
The modulus of rupture has a range of 700 to 2,300 pounds
per square inch.
Young's modulus of elasticity for compression varies from
1,100,000 to 7,700,000 pounds per square inch, and, as stated
for other stones, the values are only true for certain com-
, pressive stresses.
The coefficient of expansion, for each degree Fahrenheit,
has a wide range, varying from .00000177 to .00000686.
The absorption coefficients have a range from less than
one per cent, for quartzite, to over ten per cent, for the
In general, the harder sandstones and quartzite makedurable building stones. In all cases, however, the stones
should be laid on their natural beds, and not on edge.
Slates are metamorphic rocks formed, usually, from clay
or shale, and sometimes from fine-grained igneous rocks.
They are used for roofing, stair treads, tubs, sinks, black-
boards, etc. Locally, they are used for basement walls in
The colors are red, green, purple, and black. Some of the
slates are unfading, and others are not. The only con-
clusive way to determine the unfading property is to com-
NATURAL BUILDING STONES 11
pare newly quarried slate with that which has been exposed
to the weather for several years.
The specific gravity of slate varies from 2.7 to 2.9, corre-
sponding to weights of 169 to 181 pounds per cubic foot.
The crushing strength, when tested normal to the cleavage
planes, varies from 19,900 to 29,400 pounds per square inch,
and when tested on edge, from 14,200 to 31,600 pounds per
square inch, the specimens being cubes in both cases.
(Tests of Metals, etc., 1902.)
The modulus of rupture, for the states upon which the
above compression values are based, varies from 700 to
10,000 pounds per square inch.
Young's modulus of elasticity in compression, tests madeon edge, averages about 14,000,000 pounds per square inch.
The coefficient of expansion is between .0000050 and
.0000060, for each degree Fahrenheit.
The absorption of water is less than one-half of one per cent.
Average Physical Properties of Building Stones. Theseveral properties of stones given above at once show, bytheir range, that average values may be unsafe for some
particular stone about which little is known. Stone from
a new quarry should always be tested to the extent of
showing that the stone is suitable for the purpose for which
it is to be used.
The following table is given by Rudolph P. Miller, in the
American Civil Engineer's Pocket Book, Mansfield Merri-
AVERAGE DATA FOR BUILDING STONES OF GOOD QUALITY
Kind of Stone
Fire-Resisting Property of Stone. In general, sandstone
is not seriously injured by the heat of a burning building,
except it may be stained by smoke.
Limestone is uninjured in strength for temperatures whichdo not exceed about 900 F. The stone seldom cracks, but
reduces to a powder under the application of water.
Granite appears to be a very poor fire-resistant, as it
The rapid change of temperature, due to throwing cold
water on the heated stones, generally injures the faces of
all building stones.
Quarrying. All building stones, as a rule, are cut from
rough blocks of stone which are separated from large masses
of rock by quarrying. The particular method used in ob-
taining these rough blocks depends upon a number of con-
ditions, such as the kind of rock, the amount required, the
capital available, etc. For example, if a relatively small
amount of stone is required, it is cheaper to use hand tools
instead of power tools in quarrying, while for large quantities
of stone the use of power tools is more economical.
The use of explosives is common in some localities, but
where the stone is to be used for any purpose other than for
rip-rap, broken stone, etc., it is better not to employ ex-
Joints in Relation to Quarrying. All rocks which are hard
and firm are broken up into masses by joints. These mayrun in almost any direction, but usually they divide the
rock into masses which are more or less regular in shape.
Joints in bedded rocks are generally in two systems runningat right angles, and normal to the bedding planes.
In igneous rocks, there are usually two sets of joints,
one horizontal and the other vertical, with sometimes an
odd set running in a diagonal direction. The horizontal
joints in granite are usually parallel to the surface of
the rock (see Figs. 1 and 13). Basalt and lava are often
divided by joints into vertical prismatic forms of columnar
NATURAL BUILDING STONES 13
The existence of joints greatly facilitates the quarryingof building stones, but they do not improve the quality of
the stone, as all joint surfaces are more or less subjected to
the action of deteriorating agencies.
Quarrying by Hand Tools. Hand tools, such as the crow-
bar, pick, drill hammer, wedge, and plug and feathers, are used
FIG. 1. "Wood and Water," or Wedging Up. Note Horizontal Joints.
in getting out all kinds of building stone (see Figs. 2, 3, 4,
5, 6, 7, 8, and 9), but such tools are more effective for rock
in thin layers and somewhat soft. When the rock is in thin
layers, these can be separated by the crow-bar and wedges,the vertical fracture following the jointing. If the piecesare too large, they are divided by drilling shallow holes
a few inches apart along the line of proposed division, andthen using the plug and feathers in each hole. The plugand feathers exert a tremendous pressure, and when properlyused the hardest granite is easily separated. Where granites
are in large masses (that is, the joints are widely separated),the bed joints are opened by means of wooden wedges.These are driven dry and then wet with water (Fig. 1).
This method was used by the Egyptians, and is now used
in some of the largest granite quarries in the United States.
Special steel wedges are also used for this work.
Quarrying by Machinery. Marble is cut out in blocks
of almost any desired size by the use of channeling machines
(Figs. 10 and 11),which cut a narrow channel, either vertically
or horizontally, for the full breadth of the face of the block
to be cut out. This method .saves a large waste and avoids
the forming of incipient cracks which sometimes result from
using other methods. In granite quarries of much magnitudeand where large blocks are wanted, a series of vertical and
horizontal holes are drilled a few inches apart along two
faces by machine drills (Fig. 12), and then the block is sepa-
rated from the rock mass by a"broach," a chisel used to
break the stone between the holes, or plugs and feathers.
The depth of the holes depends upon the nature of the rock
and the amount of waste which can be permitted. Spires
sixty feet long, and from four to five feet square in section,
have been quarried by drilling and broaching (Figs. 13
The channeling machines and the power drills are operated
by steam, electricity, or compressed air. Pneumatic and
electric hand drills are now extensively coming into use, and
are very handy and serviceable (Fig. 15).
The Use of Explosives in Quarrying. As stated above,
the use of explosives is not advisable, where dimension stone
is desired, on account of the waste which follows from the
irregularity of the pieces detached by explosives and the
danger of cracks. It is often economical, however, to use
explosives in separating large blocks of rock which are after-
ward broken into smaller pieces by means of a series of
plugs and feathers.
In using explosives, holes are drilled by hand or by powerdrills to the depth to which the rock is to be broken, and
NATURAL BUILDING STONES 15
FIG. 2. Crow Bars.
FIG. 3. Stone Pick.
FIG. 4. Common Drill.
FIG. 5. Flat Face Stone Sledge.
FIG. 6. Drilling or Striking Hammers, (a) Nevada Pattern. (6) OregonPattern.
FIG. 7. Spalling or Stone Hammers, (a) Single Face. (6) Double Face.
FIG. 8. Stone Wedge.
FIG. 9. Plug and Feathers.
FIG. 10. Channeling a 9-foot Key Block. Ingersoll-Sergeant Track
Channeler. (Ingersoll-Rand Co.)
NATURAL BUILDING STONES 17
FIG. 11. Swing Back Type of Ingersoll-Sergeant Track Channeler as Illus-
trated in a 5-inch "Marble" Channeler. (Ingersoll-Rand Co.)
FIG. 12. "Electric Air" Drill on a Quarry Bar Working in Barre Dark
Granite. (Ingersoll-Rand Co.)
FIG. 13. Spire of Granite Separated from Rock Mass on all Sides Except
One End. Horizontal Joints of Rock Mass Are Clearly Shown.
NATURAL BUILDING STONES 19
FIG. 14. A Spire of Barre (Vt.) Granite Over 60 Feet Long, Showing Marksof Drills, Also Showing Shallow Holes on End for Plug and Feathers.
FIG. 15. "Jack-hammer" at Work Drilling Horizontal Holes at the DiamondSlate Company's Quarries, Pen Argyl, Pa. (Ingersoll-Rand Company.)
then small charges of coarse black powder are put in the
holes and fired. Several repetitions of small charges, lightly
tamped, is better than the same amount of powder in one
blast. A heavy explosion is liable to break up the rock
and form incipient cracks. Quick-acting explosives like
dynamite (nitro-glycerine mixed with a granular absorbent)are not as satisfactory as black powder, since their action
shatters the rock.
Tools Used in Preparing Building Stones. The following
descriptions and names of tools were first published in the
Transactions of the American Society of Civil Engineers,
Vol. VI, pp. 297-304, and have been quoted in many pub-lications since then.
"The Double Face Hammer (Fig. 76) is a heavy tool weigh-
ing from 20 to 30 pounds, used for roughly shaping stones
as they come from the quarry, and knocking off projections.
This is used only for the roughest work.
"The Face Hammer (Fig. 7o) has one blunt and one cutting
end, and is used for the same purpose as the double face
hammer where less weight is required. The cutting end is
used for roughly squaring stones, preparatory to the use of
"The Cavil (Fig. 16) has one blunt and one pyramidal, or
FIG. 16. Cavil.
pointed, end, and weighs from 15 to 20 pounds. It is used
in quarries for roughly shaping stones for transportation.
"The Pick (Fig. 17) somewhat resembles the pick used in
digging, and is used for rough dressing, mostly on limestone
and sandstone. Its length varies from 15 to 24 inches, the
thickness at the eye being about two inches.
"The Axe or Pean Hammer (Fig. 186) has two opposite
cutting edges. It is used for making drafts around the arris,
NATURAL BUILDING STONES 21
or edge of stones, and in reducing faces, and, sometimes,
joints to a level. Its length is about 10 inches, and the
FIG. 17. Stone Pick.
FIG. 18. (a) Stone Axe with Teeth. (6) Stone Axe.
FIG. 19. Bush Hammers, (a) Solid. (6) With Leaves. " Patent Hammer."
cutting edges about 4 inches. It is used after the pointand before the patent hammer.
"The Tooth Axe (Fig. 18a) is like the axe, except that its
cutting edges are divided into teeth, the number of which
varies with the kind of work required. This tool is not used
on granite and gneiss cutting.
"The Bush Hammer (Fig. 19a) is a square prism of steel
whose ends are cut into a number of pyramidal points. The
length of the hammer is from 4 to 8 inches, and the cutting
face from 2 to 4 inches square. The points vary in number,and the size with the work to be done.
"The Patent Hammer (Fig. 196) is a double-headed tool
so formed as to hold at each end a set of wide thin chisels.
The tool is in two parts which are held together by the
bolts which hold the chisels. Lateral motion is prevented
by four guards on one of the pieces. The tool without teeth
is 5^4 X 2% x IJMz inches. The teeth are 2% inches wide.
Their thickness varies from % to Y of an inch. This tool
is used for giving a finish to the surface of stones.
"The Crandall (Fig. 20) is a malleable iron bar about two
feet long, slightly flattened at one end. In this end is a
slot 3 inches long and 3/s mcn wide. Through this slot are
passed ten double-headed points of J^-inch squared steel,
9 inches long, which are held in place by a key.
"The Hand Hammer (Fig. 21), weighing from 2 to 5
pounds, is used in drilling holes, and in pointing and chisel-
ing the harder rocks.
"The Mallet (Fig. 22) is used where the softer limestones
and sandstones are to be cut.
"The Pitching Chisel (Fig. 23) is usually of l^inch
octagonal steel, spread on the cutting edge to a rectangle
of 1 X 2 l/2 inches. It is used to make a well-defined edge
to the face of a stone, a line being marked on the joint
surface to which the chisel is applied, and the portion of
the stone outside of the line broken off by a blow with the
hand hammer on the head of the chisel.
"The Point (Fig. 24) is made of round or octagonal rods
of steel, from J^ to 1 inch in diameter. It is made about
12 inches long, with one end brought to a point. It is used
NATURAL BUILDING STONES 23
until its length is reduced to about 5 inches. It is employedfor dressing off the irregular surface of stones, either for
FIG. 20. CrandaU. FIG. 21. Stonecutter's Hammer.
FIG. 22. Stonecutters' Mallets, (a) Hickory Mallet, 5 to 7^ Inches in
Diameter. (6) Vulcanized Fiber-head Mallet, 2 to 3 Inch Face.
FIG. 23. Pitching Chisel.
FIG. 24. Stonecutters' Chisels, (a) Point. (6) Chisel, (c) Tooth Chisel.
(d) Hammer-head Point. Chisels With Large Heads Are Used with the
Wooden Mallet Shown in Fig. 22.
a permanent finish or preparatory to the use of the axe.
According to the hardness of the stone, either the hand
hammer or the mallet is used with it.
"The Chisel (Fig. 24) of round steel of % to % inch in
diameter and about 10 inches long, with one end broughtto a cutting edge from % inch to 2 inches wide, is used for
cutting drafts or margins on the face of stones.
"The Tooth Chisel (Fig. 24) is the same as the chisel,
except that the cutting edge is divided into teeth. It is
used only on marbles and sandstones.
"The Splitting Chisel (Fig. 25) is used chiefly on the softer
FIG. 25. Stonecutters' Chisels, (a) Splitter. (6) Drove.
stratified stones, and sometimes on fine architectural carvingsin granite.
"The Plug, a truncated wedge of steel, and the Feathers,
of half-round malleable iron (Fig. 9), are used in splitting
unstratified stone. A row of holes is made with the drill
(Fig. 26) on the line on which the fracture is to be made; in
each of these holes, two feathers are inserted and the plugsare driven in between them. The plugs are then graduallydriven home by light blows of the hand hammer on each
in succession until the stone splits."
All of the above-described tools are for hand use, and the
classification of masonry and kinds of finish are based upontheir use. At the present time, however, there are in use
a large number of machines for cutting, surfacing, polishing,
etc., and for accomplishing the same end as reached with
the use of hand tools.
Power Tools for Finishing Building Stone. In extensive
works, practically all of the work done on stone is accom-
plished with machinery. Large blocks are separated into
smaller blocks by means of the pneumatic plug driller (Fig.
26), and plugs and feathers. The tools shown in Fig. 27 are
NATURAL BUILDING STONES 25
also used with the plug driller. For finer work and carving,
the pneumatic hammers shown in Figs. 266 and 27 are used.
A pneumatic hammer is also used on a portable surfacing
FIG. 26. Pneumatic Hammers, (a) "Barre" Pneumatic Plug Drill. (6)
"Barre" Pneumatic Bushing Tool. (Trow and Holden.)
machine (Fig. 29), with the tools shown in Fig. 28. With the
above-mentioned tools, all of the work done by hand tools
can be accomplished better, in less time, and at a less cost.
There are numerous styles of pneumatic hammers and sur-
facing machines of which only one of each has been illus-
trated. The two machines shown are designed for workinggranite. The same devices are used in working limestoneand sandstone, but with cutting tools of different shape.While the above descriptions have been confined to tools
operated by compressed air, similar devices are in use which
are operated by electricity.
All of the rocks used for building stones can be sawed.
The saws are diamond saws, soft iron saws, and wire rope,
FIG. 27. Pneumatic Tool Chisels. (George Oldham & Sons Co.)
the particular type depending upon the character of the
stone. Thin slabs of marble and limestone are cut with the
soft iron saws and wire rope, and slate is cut into blocks
with the iron saws. The harder stones can be turned and
polished in lathes, and the softer stones planed, where mould-
ings and similar forms are wanted. In fact, practically
FIG. 28. Pneumatic Surfacer Tools, (a) Tooth Chisel. (6) Cross Chisel,
(c) Boltless Bush Chisel. (Trow and Holden.)
- Set Screw
Adjustable Brackets to keep'' '
'beam in alignment with column
Width of Wheelall 2 10,^*
Width of wheels 3%
Equipped with flange
FIG. 29. Portable Surfacing Machine Using Pneumatic Tools. (GeorgeOldham & Son Co.)
every form of stone and surface finish used in building can
be cut with power-operated tools.
Classification of Building Stones According to the Finish
of the Surface.
"All stones used in building are divided into three classes,
according to the finish of the surface, viz. :
"1. Rough stones that are used as they come from the
2. Stones roughly squared and dressed."
3. Stones accurately squared and finely dressed.
"In practice, the line of separation between them is not
very distinctly marked, but one class merges into the next.
"Unsquared Stones. This class covers all stones which
are used as they come from the quarry, without other
FIG. 30. Bridge at Ipswich, Mass. Built in 1764. Spandrel Wall Shows
Unsquared Stones Laid as Random Coursed Rubble. Parapet Shows
Coursed, Quarry-Faced Squared Stones.
preparation than the removal of very acute angles and ex-
cessive projections from the figure. The term backing, which
is frequently applied to this class of stone, is inappropriate,
as it properly designates material used in a certain relative
NATURAL BUILDING STONES 29
position in the wall, whereas stones of this kind may be
used in any position (see Fig. 30).
"Squared Stones. This class covers all stones that are
roughly squared and roughly dressed on beds and joints.
The dressing is usually done with the face hammer or axe,
or, in soft stones, with the tooth hammer. In gneiss, it maysometimes be necessary to use the point. The distinction
between this class and the third lies in the degree of close-
ness of joints. Where the dressing on the joints is such
that the distance between the general planes of the surfaces
of adjoining stones is one-half inch or more the stones
properly belong to this class (see Fig. 30)." Three subdivisions of this class may be made, depending
on the character of the face of the stones.
FIG. 31. Quarry-Faced SquaredStone.
FIG. 32. Pitched-Faced SquaredStone.
"Quarry-faced stones are those whose faces are left un-
touched as they come from the quarry (Fig. 31).
"Pitch-faced stones are those on which the arris is clearly
FIG. 33. Drafted Stone. FIG. 34. Rough-Pointed Face Finish.
defined by a line beyond which the rock is cut away by the
pitching chisel, so as to give edges that are approximatelytrue (Fig. 32).
"Drafted Stones are those on which the face is surrounded
by a chisel draft, the space within the draft being left rough.
Ordinarily, however, this is done only on stones in which
the cutting of the joints is such as to exclude them from
this class (Fig. 33).
"In ordering stones of this class, the specifications should
always state the width of the bed and end joints which are
expected, and also how far the surface of the face mayproject beyond the plane of the edge. In practice, the pro-
portion varies from 1 to 6 inches. It should also be specified
whether or not the faces are to be drafted.
"Cut Stones. This class covers all squared stones with
smoothly dressed beds and joints. As a rule, all the edges
of cut stones are drafted, and between the drafts the stone
is smoothly dressed. The face, however, is often left roughwhere the construction is massive.
"In architecture, there are a great many ways in which
the faces of cut stone may be dressed, but the following are
those which will usually be met with in engineering work.
"Rough-pointed. When it is necessary to remove an inch
or more from the face of a stone, it is done by the pick or
heavy point until the projections vary from J^ inch to 1
inch. The stone is then said to be rough-pointed (Fig. 34).
NATURAL BUILDING STONES 31
the effect being the same as fine-pointing, except that the
dots on the stone are more regular. The variations of level
are about M inch, and the rows are made parallel. Whenother rows at right angles to the first are introduced, the
stone is said to be cross-crandalled (Fig. 36).
"Axed or Pean-Hammered and Patent-Hammered. These
two vary only in the degree of smoothness of the surface
which is produced. The number of blades in a patenthammer varies from 6 to 12 to the inch; and, in precise
specifications, the number of cuts to the inch must be stated,
such as 6-cut, 8-cut, 10-cut, 12-cut. The effect of axing is
to cover the surface with chisel marks, which are made
parallel as far as practicable. Axing is a fine finish (Fig. 37).
"Tooth-axed. The tooth-axe is practically a number of
points, and leaves the surface of the stone in the same con-
FIG. 37. Axed or Pean-FJammered
FIG. 38. Bush-HammeredFace Finish.
dition as fine-pointing. It is usually, however, only a
preparation for bush-hammering, and the work is done with-
out regard to effect, as long as the surface of the stone is
"Bush-hammered. The roughness of the stone is poundedoff by the bush hammer, and the stone is then said to be
bushed. This kind of finish is dangerous on sandstone, as
experience has shown that sandstone thus treated is very
apt to scale. In dressing limestone which is to have a bush-
hammered finish, the usual sequence of operations is: (1)
rough-pointing, (2) tooth-axing, and (3) bush-hammering(Fig. 38).
"Rubbed. In dressing sandstone and marble, it is verycommon to give the stone a plane surface at once by the
use of the stone saw. Any roughnesses left by the saw are
removed by rubbing with grit or sandstone. Such stones,
therefore, have no margins. They are frequently used in
architecture for string courses, lintels, door-jambs, etc., and
they are also well adapted for use hi racing the walls of
lock-chambers and in other locations where a stone surface
is liable to be rubbed by vessels or other moving bodies.
"Diamond Panels. Sometimes the space between the
margins is sunk immediately adjoining them, and then
rises gradually until the four planes form an apex at the
FIG. 39. Sunk Diamond Panel. FIG. 40. Raised Diamond Panel.
middle of the panel. In general, such panels are called
diamond panels, and the one just described (Fig. 39) is called
a sunk diamond panel. When the surface of the stone rises
gradually from the inner lines of the margins to the middle
of the panel, it is called a raised diamond panel (Fig. 40).
Both kinds of finish are common on bridge-quoins and
similar work. The details of this method should be given
in the specifications.5 '
ARTIFICIAL BUILDING MATERIALS
Brick, LimCj and Cement
Building Brick is an artificial product manufactured from
clay, and, when properly made, is one of the most durable
and satisfactory of building materials. The use of brick is
not general in engineering structures, but it is universally
employed in buildings, and is a very valuable substitute for
stone. Since the advent of concrete, however, the use of
brick is being rapidly displaced, and, where employed, is
often used only for facing the concrete construction.
Manufacture of Building Brick. The manufacture of
brick consists in mixing clay and water to the proper con-
sistency, shaping the mixture by means of moulds or other
methods, drying, burning, and cooling. Each step in the
process has a bearing upon the quality of the product.
The clay used is of primary importance. Common build-
ing brick is made from the common clays, which consist
principally of silicate of alumina. If iron is present in the
form of oxide or carbonate, the bricks burn red, but if the
iron is in the state of silicate, the bricks do not burn red
In moulding brick, the clay and water are mixed to a
plastic state, and then the soft plastic material is pressedinto moulds. In early days (and even now, the same process
is used in small plants), the clay and water were broughtto a state of plasticity by a primitive pug-mill, and the
material placed hi the moulds by hand. At the present
time, the entire process can be performed by machinery.The machinery used, while of great variety, may be divided
into three classes, according to the plasticity of the claymixture when moulded.
Soft-mud machines handle the clay mixed with about one-
fourth of its volume of water. In the late machines, the
clay is constantly being worked in a pug-mill attached to
the machine, and is fed directly from the mill under the
plunger which presses it into moulds. The moulds are then
moved forward and struck off by hand with a special steel
tool made for the purpose.
Stiff-mud machines handle a stiff mud which is delivered
to the machine through a hopper (Fig. 41). A specially
designed screw forces the clay forward through a metal die
in the form of a continuous bar. This bar is pushed' along
to the table of a cutting machine, where it is separated bymoving wires (Fig. 42) into bricks, which are then ready to
be taken to the drying rooms or "dryers." If the bricks are
"side cut," the cross section of the clay bar is the largest
face of the brick; if "end cut," the cross section of the bar
is the end face of the brick. The cutting machine shown in
Fig. 42 'is operated by hand. In large plants, automatic
machines are used. The stiff-mud machine is used wherever
the character of the clay permits.
Dry-day machines use the clay with a very little moisture.
The moulds are holes in a metal plate in which plungers
move from below upward until flush with the top of the
plate. Sufficient clay is placed above the plungers to fill
the moulds, and then plungers from above move downward
and force the clay into the moulds. The lower plungers
move down to give the brick the proper thickness. The
upper plungers now move upward and the bricks are forced
up out of the moulds by the lower plungers and taken to the
drying-rooms or "dryers."
Drying Brick. Before the bricks are burned, they must
be dried either before being placed in the kiln for burning
or after they are in the kiln. In plants where little or no
machinery is employed, the hand-moulded bricks are placed
on the ground having a specially prepared smooth surface.
The bricks are deposited flatwise and left for about six hours,
or until the top surface is dry, and then they are turned on
ARTIFICIAL BUILDING MATERIALS 35
FIG. 41. Interior of Brick Machine. (The C. W. Raymond Co.)
FIG. 42. The Raymond Combination Cutting Table. "The Simplest Formof Cutter Made." (The C. W. Raymond Co.)
edge and left for several hours. When they are sufficiently
hard, they are loaded into barrows and taken to dryingracks which are under roof, where they remain from one
to four weeks, or until enough bricks are on hand to burn.
In plants where modern machinery is employed, the bricks
are set up on edge on racks which slip between uprights,
forming shelves, on cars, which are then run into "dryers."The time required for drying depends upon the method of
supplying heat and the character of the material used in
making the bricks. For the ordinary stiff-mud brick, about
twenty-four hours is sufficient to dry the brick when someof the modern "
dryers" are used.
Burning Brick. The operation of burning brick depends
upon the clay, the form and size of the kilns, and the
In brick-yards where the bricks are moulded by hand, andwhich do not have permanent kilns, the burning is done in
clamp kilns, which are constructed of the bricks to be burned.
The kiln is built up in sections called"arches." Fig. 43
shows a transverse section of three arches, and Fig. 44 a
longitudinal section of an "arch." Each arch is about
3J/2 feet wide, from 20 to 30 feet deep, and from 35 to 50
courses high. Each "arch" has an opening, called an "eye,"at the bottom, in the center of the width running entirely
through the kiln in which the fuel used in burning is placed.
(The fuel is usually wood.) After the arches have been built,
they are enclosed by a wall of green brick having all openings
between them stopped with mud. The top is covered with
bricks laid flatwise. In building the arches, there are cer-
tain arrangements of the bricks which must be followed in
order to distribute the heat as uniformly as possible throughthe mass. The brick is first subjected to a slow fire, pro-
ducing a moderate temperature, to expel the moisture, and
then the temperature is gradually increased until the bricks
next to the "eye" are at a white heat. This temperature is
kept up until the burning is complete, and then all open-
ings are closed and the mass allowed to cool. The process
ARTIFICIAL BUILDING MATERIALS 37
of drying and burning takes from 6 to 15 days. The drying
takes from 18 to 72 hours, depending upon the clay used.
This form of kiln is really a very simple up-draft kiln.
-Burned brick laid flatwise
u aFIG. 43. Cross-Section of Three "Arches" of a Clamp Kiln.
FIG. 44. Longitudinal Section of an "Arch" of a Clamp Kiln.
Occasionally, permanent walls are built as shown in Fig. 43,but generally they are dispensed with.
Modern Methods of Burning Brick. Modern methodsuse permanent kilns which are of various forms. They are
divided in three classes: the up-draft, the down-draft, andthe continuous.
The up-draft kiln may be either rectangular or circular
in plan, and has fires at the bottom so arranged that the
heat passes under and up through the floor of the kiln andthence up through the bricks to the top of the kiln, where it
escapes through openings in the roof. The bricks at the
bottom of the kiln receive too much heat and those at the
top too little. The bricks in the center are the only bricks
which receive the proper amount of heat. Under average
conditions, it is seldom that 50 per cent of the bric'ks are
No. 1 grade. As stated above, the clamp kiln, shown in
Figs. 43 and 44, is an example of an up-draft kiln.
In the down-draft kiln, which may be either circular or
rectangular in plan, the heat from the furnaces in the outside
wall is led through flues to the top of the kiln, and is then
drawn down through the brick and through the floor to
FIG. 45. Down-Draft Kiln, Circular in Plan, Built of Brick in a Steel Shell.
ducts which lead to a stack. This form of kiln gives more
brick of No. 1 grade than the up-draft kiln. Fig. 45 shows
the general arrangement of a circular down-draft kiln. It
is constructed of brick within a steel shell.
The up-and-down-draft kiln is so arranged that the heat
can be made to pass up through the brick and also down
through the brick. This requires two sets of furnaces, one
for the up-draft and one for the down-draft. This type
ARTIFICIAL BUILDING MATERIALS 39
of kiln burns a very uniform product. Fig. 46 shows a
section of a circular kiln through the furnaces which furnish
The continuous tunnel kiln, of the Raymond design (Figs.
47 and 48), consists of two parallel tunnels which are con-
FIG. 46. Section of a Circular Up-and-Down Draft Kiln. (Ohio Kiln Co.)
nected at the ends. Each tunnel is divided into sections by
drop arches, and each section is provided with a side en-
trance and necessary flues. The space between the tunnels
is utilized for draft and hot-air ducts. In filling a section,
the deflection wall V is made tight of green brick up to the
under side of the drop arch. Between this wall and the
drop arches, the bricks are set up to form flues which con-
nect with horizontal flues, built of the green brick, which
extend the length of the chamber. Immediately in front of
the drop arches a tight wall, W, of green brick is built, ex-
tending from the top of the horizontal flues just mentioned
to the top of the chamber. The fuel used is producer gas
admitted through the top of the kiln. The arrows, Fig. 48,
show the route taken by the hot gases. By using the proper
ARTIFICIAL BUILDING MATERIALS 41
number of sections, the process
of burning becomes continuous,as the bricks in different sections
will be in various stages of
the burning, from a section in
which green brick is being set
to one where the finished prod-uct is being taken out. Thesame result is obtained by prop-
erly connecting rectangular or
circular down-draft kilns. Fig. 49
is a sketch showing the Schaffer' '
kiln system,which is self-explanatory.
Fuel Used in Burning Brick
The fuel employed depends uponlocal conditions usually. Wood,coal, and gas may be used in anyof the up- or down-draft kilns bybuilding the proper furnaces.
Annealing or Cooling Brick
This is very important for all
kinds of clay products. After the
burning is completed, the fires in
the furnaces are stopped and all
cool currents of air excluded fromthe kiln. To obtain good results,
the cooling should be slow, other-
wise the brick will be brittle.
While brick-makers are well awareof this, they claim that they can-
hot profitably spend the time to
anneal the brick properly. Proper
annealing is especially importantin the manufacture of pavingbrick.
Classification of Brick. Ac-
cording to the method of mould-
FIG. 49. The Schaffer Semi-
Continuous Kiln System.
(The Schaffer Engineeringand Equipment Co.)
ing, brick is classified as soft-mud brick, stiff-mud brick,
pressed brick, repressed brick, slop brick, sanded brick, andmachine-made brick.
Soft-mud bricks are moulded by hand or machinery from
a soft mixture of clay and water.
Stiff-mud bricks are machine moulded from a stiff mixture
of clay and water.
Pressed bricks are machine moulded from dry or nearly
Re-pressed bricks are formed from soft-mud bricks and
stiff-mud bricks, which have been partially dried, by sub-
jecting them to great pressure in metal moulds. This makesthem more regular in form. Formerly, it was thought that
the density and strength were increased, but it is doubtful
if the strength is materially changed.
Slop bricks are those moulded by hand, where the
moulds are wet with water to prevent the clay from
Sanded bricks are soft-mud bricks moulded in moulds
sprinkled with sand.
Machine-made bricks are those made by machinery, and
now include all kinds of brick.
Brick is also classified according to its position in the
kiln. The following classification strictly refers to the old-
style clamp kiln, but where the quality is considered, it
refers to any kiln.
Arch or clinker bricks are those which are in immediate
contact with the fire. They are over-burned, hard, brittle,
and twisted in shape.
Body, cherry, or hard bricks are those taken from the
interior of the pile and are the best bricks in the kiln, or
No. 1 grade. Cherry refers to the color of the product. As
the color depends upon the kind of clay, cherry has no
meaning for clays which do not burn red.
Salmon, pale, or soft bricks are those forming the exterior
of the mass and, consequently, are under-burned. They are
usually regular in shape but quite soft, and are only suitable
ARTIFICIAL BUILDING MATERIALS 43
for the interior of walls. Soft bricks made from clay which
burns red are salmon in color.
Depending upon their form and use, bricks are designated
as compass bricks, feather-edge bricks, face bricks, sewer
bricks, fire bricks, paving bricks, etc.
Compass bricks have one edge shorter than the other, and
are used in walls with curved surfaces.
Feather-edge bricks have one edge thinner than the other,
and are used in arches.
Face bricks are usually pressed or re-pressed bricks, regular
in shape and size, and uniform in color, making them suit-
able for the outside of walls in buildings.
Fig. 50 shows a few of the many shapes in which brick
Sewer bricks are simply hard, common bricks used in the
construction of sewers.
Fire bricks are made of pure clay and sand, and are used
in places subjected to high temperatures. They are usually
yellow in color.
Paving bricks are generally made of hard clays or shale
and burned to a point a little below vitrification. For paving
purposes, they are regular in shape and size, uniform in
color, and tough. An inferior grade makes an excellent
material for walls, piers, etc., where strength and water
tightness are required.
Essential Requirements for Good Building Brick. Thebricks should be uniform in size, regular in form, with
parallel faces and sharp corners. The structure of the bricks
sjiould be uniform and so dense that not over 12 per cent
of their weight of water is absorbed.
The crushing strength of bricks is generally much greaterthan necessary, but a half-brick tested carefully between
steel plates should have an ultimate crushing strength of
at least 7,000 pounds per square inch (Baker).The modulus of rupture of brick in cross-breaking is a fair
measure of its quality, since it depends upon the toughnessof the brick. Its determination is easy and quick. The
modulus for building brick should be at least 1,000 poundsper square inch (Baker).
The absorption test of brick is made in the manner ex-
plained for building stones. Soft brick, of little use in build-
FIG. 50. A Few Shapes in Which Building Bricks Are Made.
ings, will absorb as high as 33 per cent of its weight of water,while the best grade of paving brick absorbs less than one
per cent of its weight.
ARTIFICIAL BUILDING MATERIALS 45
Ornamental Face Brick. Formerly, face bricks were
simply selected brick, uniform in color and true in shape.
Now, special face bricks are made with almost any color
desired. Some manufacturers produce the colors by selecting
the proper clay or shale and by proper burning. Others
enamel the exposed faces of the bricks, and, by so doing,
can obtain almost any shade wanted. Various textures are
also given to the exposed faces by numerous processes. The
sizes of the bricks are quite variable, and, therefore, it is
advisable to purchase all brick for a particular structure
from one maker. This difference in size is not always due
to the use of different sizes of moulds, but to the shrinkage
of the brick in drying and burning. Different clays and
different methods of handling lead to bricks which have
different coefficients of shrinkage.
Sizes of Brick. As stated above, the sizes of brick are
numerous. The following are the approximate standard
sizes, in inches.
Common brick %Y X 4 X 2^f 8^ X 4 X 2^
Paving brick \9 X4X3
I X5 X4Pressed brick Sy8 X 4 X 2^Roman brick 12 X 4 X 1 1ANorman brick 12 X 4 X 2%
Sand-Lime Brick consists of sand cemented together with
lime. The lime is in the form of carbonate or silicate. Whenin the form of carbonate, the brick is simply lime mortar
moulded, either with or without pressure, and dried in air
rich in carbon dioxide. The brick is weak and of little use.
When the lime is in the form of silicate, the bricks are
moulded under pressure, placed in a closed cylinder, and
dried under a steam pressure of from 100 to 150 pounds per
square inch. Such bricks are now made which equal in
quality and appearance the dry-clay bricks.
The crushing strength and the strength in cross-breaking
of sand-lime brick are not as great as for clay brick, but
they are sufficiently strong for all ordinary uses in buildings.
The absorption of water appears to be less than that of goodclay brick.
Cement Bricks. Bricks made of Portland cement andsand are quite extensively used in some localities. Thebricks are machine-moulded in the shape and size of the
common clay bricks. They can be made in various colors
by the proper selection of cement and sand or by intro-
ducing coloring matter. The bricks are"cured" in the
manner outlined for cement blocks.
Hollow Terra-Cotta or Tile is a clay product manu-factured in an almost innumerable number of shapes and
sizes, from the common rectangular blocks used in walls and
partitions to elaborately carved designs used for ornamental
purposes. For building purposes, the blocks have the desir-
able qualities of lightness and strength (see Fig. 51). For
partitions, the blocks are made porous by mixing sawdust
with the clay. This disappears during the burning, leavinga light and porous block having a crushing strength of a
little over one-half that of the blocks in which sawdust is
not used. There also is an under-burned terra-cotta which
has properties between the hard-burned and the porousterra-cotta.
The color of terra-cotta depends to a great extent uponthe clay used in its manufacture and the burning. Shades
of red and gray are the predominating colors, although a
glazed terra-cotta can be made with a surface of almost anycolor. Both glazed and unglazed products are used. For
face-work, the terra-cotta is burned hard and has a smooth,
impervious surface. Usually, this surface is not glazed. For
backing, walls to be plastered, partition walls, etc., the tile
blocks have corrugations to hold the plaster (Fig. 51), andboth the glazed and unglazed tiles are used.
The tile is manufactured by machinery, very much in the
manner employed in making wire-cut brick. The tempered
clay is forced through dies, and cut off in lengths of about
twelve inches by wires. The tile is burned in kilns of the
same construction as those for brick.
ARTIFICIAL BUILDING MATERIALS 47
STANDARD WALL BLOCKS
FIG. 51. A Few Shapes and Sizes of Hollow-Tile Blocks. (National Fire-
The crushing strength of dense terra-cotta ranges from
3,000 to 5,000 pounds per square inch, and its weight is about
120 pounds per cubic foot. The weight of hollow tile walls
is from 40 to 50 pounds per cubic foot.
Plaster Blocks. For partitions in buildings, a very light
and serviceable hollow block is made of plaster of Paris
FIG. 52. Hollow Fibered Plaster Partition Block.
combined with various materials such as cinders, asbestos,
wood-chips, etc. Such blocks are cheaper than terra-cotta
and are quite as good for ordinary partitions (Fig. 52).
Fat or Quick-lime. If ordinary limestone is heated to
a cherry red, the carbon dioxide is driven off, leaving the
oxide of calcium which is called quick-lime. Since pure car-
bonate of lime is composed of 44 parts, by weight, of carbon
dioxide and 56 parts, by weight, of oxide of calcium and with
the hydroscopic moisture variable, the amount of quick-
lime obtained in burning never exceeds one-half the original
stone by weight.
Quick-lime has a great affinity for water, and, when water
is added to it, it swells and breaks up into an impalpable
powder. As the water is added there is a rapid rise in tem-
perature and about a threefold increase in volume. Treat-
ing lime with water is called slacking, and the product is
called hydrated lime, fat-lime, or slacked lime, and, if more
water is added, it becomes lime paste or putty.
Since quick-lime will slack by absorbing moisture from
the air, it cannot be stored in bulk for any great length of
ARTIFICIAL BUILDING MATERIALS 49
time. It can, however, be kept for long periods in tightly
closed vessels. Hydrated lime is now made and shipped in
bags in the form of a dry powder which simply requires
Burning Lime. Practically all lime produced in the
United States is burned in some form of kiln. The usual
form is that known as the shaft kiln (Fig. 53). The limestone,
broken into small fragments, is dumped into the top of the
kiln, filling the hopper and shaft. The lime is burned in the
shaft, and is removed through a special opening at the
bottom. The stone in the hopper settles down into the
shaft as the burning proceeds. The fire boxes are made to
burn coal, wood, or gas, but the arrangement and dimensions
vary according to the fuel used. It is generally conceded
that wood fuel makes the best lime.
Rotary kilns, similar to those used in the manufacture of
Portland cement, have been used, but as they require fine
raw material the product cannot be sold as lump lime.
A very interesting and complete discussion of the" Manu-
facture of Lime" is given in "Technologic Papers of the
Bureau of Standards/' No. 16, by Warren E. Emley.Use of Lime. The principal use of lime is in making
mortar for laying masonry, plastering houses, etc., where
the mortar is exposed to the air. The mortar is made by
combining slacked lime and sand. The sand is added since
slacked lime or paste cannot be used neat because of its
great shrinkage in drying.
In hardening, the lime mortar exposed to the air slowly
unites with the carbon dioxide, and thereby changes a por-
tion of the hydrated lime back to its original form. The
process is slow, and takes place mostly on the exposed sur-
faces, the mortar inside a thick wall never becoming entirely
Natural Cement is a "finely pulverized product resulting
from the calcination of an argillaceous limestone at a tem-
perature only sufficient to drive off the carbonic acid gas."
This powder, mixed with about 25 per cent of its weight of
water, forms a combination which hardens quickly into an
artificial stone which increases in strength as it ages. The
powder is called natural cement because it is produced from
the natural rock. There are numerous trade names given
ARTIFICIAL BUILDING MATERIALS 51
to this product, usually being that of the locality in which
it is manufactured.
Natural cements are rapidly being superseded by artificial
mixtures, owing to their greater strength and uniformity.Natural cements vary in strength and uniformity, owing to
the variability of the constituents which make up the rock
from which they are manufactured.
According to the latest standard specifications, the finenessof natural cement shall be such that at least 90 per cent
by weight passes a No. 100 sieve, and at least 60 per cent
a No. 200 sieve.
The time of setting is important. The initial set should not
take place in less than 10 minutes, and a hard set in less
than 30 minutes or more than 3 hours.
The minimum permissible tensile strength of natural
cement, as found from standard briquettes, is as follows:
NEAT CEMENTAge Tensile Strength,
Lbs. per Sq. In.24 hours in moist air 757 days (1 day in moist air, 6 days in water) 150
28 days (1 day in moist air, 27 days in water) 250
ONE PART CEMENT, THREE PARTS STANDARD OTTAWA SAND7 days (1 day in moist air, 6 days in water) 50
28 days (1 day in moist air, 27 days in water) 125
Portland Cement is a "finely pulverized product resulting
from the calcination to incipient fusion of an intimate mix-
ture of properly proportioned argillaceous and calcareous
materials, and to which no addition greater than 3 per cent
has been made subsequent to calcination."
The principal constituents of Portland cement are 72 to 77
per cent of carbonate of lime, and 20 to 25 per cent of clay.Portland cement, when mixed with water, has the propertyof becoming very hard either in air or in water, and, conse-
quently, its uses are innumerable.
The specific gravity of Portland cement should be at least
3.1, and its fineness such that at least 92 per cent by weightpasses a No. 100 sieve, and at least 75 per cent the No. 200sieve.
The initial set should not develop in less than 30 minutes,
and a hard set in not less than 1 hour nor more than 10 hours.
The minimum permissible tensile strength of Portland
cement, as found from standard briquettes, is as follows:
NEAT CEMENTAge Tensile Strength,
Lbs. per Sq. In.
24 hours in moist air 175
7 days (1 day in moist air, 6 days in water) 50028 days (1 day in moist air, 27 days in water) 600
ONE PART CEMENT, THREE PARTS STANDARD OTTAWA SAND
7 days (1 day in moist air, 6 days in water) 20028 days (1 day in moist air, 27 days in water) 275
Standard specifications for cement, and methods for test-
ing, are given in the Year Book of the American Society for
Iron-Ore Cement is composed of limestone and iron ore,
and, when ground to the fineness of Portland cement, it is
slower in setting and attains greater strength. If iron-ore
cement is ground much finer than Portland cement its
setting is accelerated. It is claimed that mortar made with
this cement is uninjured by sea water. It is principally of
Magnesia Cement. "A mixture of magnesium oxide and
magnesium chloride makes the strongest hydraulic cement
known. This discovery was made in about 1853 by Sorel,
a French chemist, and the cement is known as Sorel, or
magnesia, cement. The magnesium oxide, or magnesia, is
prepared either by calcining magnesite, a comparatively rare
material, or from sea-salt. The cement is made by wetting
the pulverized magnesium oxide with bittern water, the
refuse of sea-side salt works, which contains magnesiumchloride.
"Magnesium cement was used about 1870 to a consider-
able extent in making emery wheels, and, in a small way, in
making artificial stone, Sorel stone; but at present it seems
not to be in use, owing to its great cost, quick setting, and
lack of durability" (Baker).
Puzzolan Cement as made in North America, or slag
ARTIFICIAL BUILDING MATERIALS 53
cement, is "an intimate mixture obtained by finely pul-
verizing together granulated basic blast-furnace slag and
slacked lime/' without previous calcination. This cement is
not safe for use in the open air, as it is likely to contain
sulphur in the form of sulphides, which, upon exposure,
change to sulphates and, in so doing, expand, and therefore
this cement is liable to injure the structure. When contact
with air is prevented, as in subaqueous structures or the
interiors of large masses, the cement is suitable. The cement
is light lilac in color, and, when rubbed between thumb and
finger, the absence of grit is very noticeable. The specific
gravity of slag cement ranges from 2.72 to 2.76.
Manufacture of Portland Cement. Modern methods used
in the manufacture of Portland cement (the general process
does not differ greatly for other hydraulic cements) have so
systematized the operations that the raw materials start at
one end of the plant and the finished product is delivered
to storage bins in a continuous process. From the storage
bins, the cement is run into bags or barrels and automatically
weighed.The raw materials, consisting of limestone and clay-shale,
are mixed in the proper proportions, and then ground to a
very fine powder. This powder is burned in a rotary cylinder
heated by a blast of air acting on oil as fuel (powdered coal
is also used), the material being introduced at one end of
the cylinder in a continuous stream and delivered at the
other end in the form of clinker. The clinker is now groundto an impalpable powder, which is the cement of commerce.
The method just outlined is called the dry process, and is
now almost universally employed in the United States. For
illustrations of the machinery used in the manufacture of
cements, the student is referred to Cements, Limes, and
Plasters, by Edwin C. Eckel.
Sand is an aggregation of small grains of hard rock used
with lime or cement in making mortar. The grains should,
in general, be composed of siliceous material. Sand is
usually obtained from beds of streams, or by screening bank
or river gravel. It is also obtained from the shores of lakes,
and, in some places, sea sand is used. The maximum size
of the grains depends upon the use of the mortar. In
masonry laid up with thin joints, fine sand is used in the
mortar, while for ordinary joints exceeding J^ inch the sand
grains all pass a J^-inch screen.
Coarse sands are preferable to fine sands, as they makea stronger mortar and require less cementing material. It
is generally conceded that a coarse sand having some fine
material, or sand having the sizes of the grains graded, re-
quire the minimum amount of cementing materials and,
consequently, are more economical than uniformly fine
Sand should be clean, but 5 to 10 per cent of clay or loam,
finely divided and uniformly distributed, appears to have
little detrimental effect. Formerly specifications for sand
called for sharp grains, but the present opinion is that the
rounded grains make fully as good mortar as the sand with
sharp grains. The rounded grains are much more easily
coated with the cementing material. Fig. 54 shows a tubu-
lar sand and gravel washer.
Testing Sand. There appears to be but one way of
determining the suitability of a sand for mortar, and that
is to compare the strengths of cement briquettes and blocks
made with the sand with that of briquettes and blocks madewith standard Ottawa sand, a natural bank sand obtained
at Ottawa, 111., and screened to size by means of a No. 20
and a No. 30 sieve. Sands which have grains of the propersize and are properly graded, and which appear to be ex-
cellent in every particular, sometimes fail to make goodmortar when mixed with cement. The reason for this is
not very clear, and, therefore, as stated above, a comparativetest is the only safe method of procedure to determine the
suitability of an untried sand.
Gravel is an aggregation of rock fragments worn by the
action of air and water or other natural forces. In general,
the fragments or pebbles will not pass a J^-inch screen, but
ARTIFICIAL BUILDING MATERIALS 55
will pass a 2j/-inch screen. These two limits, however, are
not fixed, and it is common practice to designate as gravel
any aggregation of coarse and fine pebbles. The rock should
be hard and, in most particulars, that which has been stated
concerning sand applies equally as well to gravel.
In building operations, the principal use of gravel is in the
making of concrete and "concrete blocks." The properties
and use of concrete are considered in Chapter V.
Voids in Sand and Gravel are independent of the sizes of
the grains, but dependent upon the gradation of the sizes.
A mass of perfect spheres of the same size has the same pro-
portion of voids regardless of the sizes of the spheres. The
proportion of voids varies from 26 per cent for tightly packed
spheres to about 48 per cent for those loosely packed.The best sands and gravels are those where several sizes
of grains are mixed. Sometimes this condition is found in
"pit gravels," but, as a rule, it is necessary to grade sand
and gravel to obtain the best results. This is especially true,
from an economical standpoint, where cement is expensive.
The proportion of voids in any sand or gravel is quicklydetermined by weighing a known volume of the material
thoroughly dried and shaken down. Taking the average
specific gravity of the rock comprising the sand or gravel
as 2.65, the percentage of voids equals 100 (1-
where W is the weight of a cubic foot of the sand or gravel.
This method is not rigidly exact, but is sufficiently so for
all practical purposes.
Shaking down and drying the material decreases the
percentage of voids for a given volume. A cubic foot of
sand or gravel weighing 100 pounds when dry has 39.4%voids, and when it contains 8% of moisture it has 44.2%voids (Taylor and Thompson).
Mortar. The quality of mortar depends upon that of its
constituents, their proportions, and the method used in mix-
ing them. Its principal use is to fill the spaces between the
pieces of stone, brick, etc., in masonry, and thoroughlycement the mass together so that it will act more or less as
ARTIFICIAL BUILDING MATERIALS 57
a monolithic structure. The Romans and Peruvians, in
early times, built stone masonry without mortar by very
carefully cutting the stones so that they fitted perfectly on
adjacent faces. This entailed an expenditure of an enormous
amount of time and labor. With the modern methods of
cutting stone this can be done now, but at a prohibitive cost,
in comparison with the cost of masonry laid up in mortar.
Lime Mortar is made by slacking lime, and mixing it with
sand. The amount of sand used is variable, depending uponthe size of the grains and the quality of the lime used.
Probably the best guide in determining the proper amount
of sand is to add sand until the mortar works well with a
trowel. For thin j oints, such as are required in pressed brick-
work, a fine sand is used, and, where the joints are to show
white, a natural or artificial white sand is employed. The
maximum amount of sand used in lime mortar is about
4 parts to 1 part of lime. Lime mortar should not be used
in freezing weather.
Natural Cement Mortar is made .by thoroughly mixingone part of cement with about two parts of sand until the
mass is uniform in color, and adding sufficient water to form
a mortar of the desired consistency. The mortar is mixed
in small batches as the cement is quick setting, and re-
tempering is not permissible. The sand used depends uponthe thickness of the mortar joints; thin joints requiring fine
Portland Cement Mortar is made in the manner explained
for natural cement mortar, using Portland cement. Theamount of sand varies from three to five parts for one part
of cement, the usual mixture being three parts sand to one
part of cement. The cement and sand used in practice are
quite variable, but probably a one-to-three mixture makesa mortar considerably stronger than is necessary in a great
many structures. The actual strength is determined bytesting standard briquettes and blocks.
Lime Paste Used with Cement Mortar. Pure cement
mortar is not easily handled on a trowel, and, to make it
more plastic and smooth, lime-paste is often used in the
mixture. The amount of lime-paste is variable, but should
not exceed one-half the volume of the mortar. The addition
of the lime-paste reduces the strength of the mortar unless
the amount is small; then it appears to have no appreciable
Water-Tight Mortar used for plastering cisterns and
similar structures is proportioned as follows, according to
Dykeshoff as quoted by Richey.
Portland cement 1 part, sand 1 part, lime parts.Portland cement 1 part, sand 2 parts, lime ^ part.Portland cement 1 part, sand 3 parts, lime 1 part.Portland cement 1 part, sand 5 parts, lime 1^ parts.
Colored Cement Mortars. Various substances are mixed
with mortars to give them certain colors. Colored mortars
are generally weaker than others, and, in the majority of
cases, the colors are not permanent. Richey gives the
following amounts of coloring matter for each barrel of
cement. To produce
Gray use 2 pounds of Germantown lampblack.Black use 45 pounds of manganese dioxide.
Blue use 19 pounds of ultramarine.
Green use 23 pounds of ultramarine.
Red use 22 pounds of iron oxide.
Bright Red use 22 pounds of Pompeian or English red.
Violet use 22 pounds of violet oxide of iron.
Yellow . . . use 22 pounds of yellow ochre.
Brown . . . use 22 pounds of brown ochre.
Pointing Mortar is a special mortar used for protecting
the joints in masonry. It is usually a very rich mixture of
Portland cement and sand. Some contend that no sand
should be used, but the cement be used neat.
PART II. MASONRY
Masonry may be designated as (1) stone masonry; (2)
brick masonry; (3) concrete masonry; (4) mixed masonry,
etc., according to the materials employed.Definitions. The following definitions of the parts of a
wall are, in general, those recommended by the Committee
of the American Society of Civil Engineers, referred to above,
FIG. 55. Range Masonry. Sketch Showing Arrangement and Names of
and conform to good practice, although they are not uni-
versally adopted (see Fig. 55). (Compare with definitions
given in Chapter VI.)
Back. The inside surface of a wall.
Backing. The stones or material forming the back of a
Batter. The inclination of the surface of a wall, and is
usually expressed as 1 : 12, 1 : 24, etc., the larger dimension
Bond. The arrangement of stones or other block materials
in adjacent courses.
Course. A horizontal layer of stones or other block
materials in a wall.
Coping. A course of heavy stones on the top of the wall
to protect it. Coping stones usually project a few inches
beyond the surface of the wall. Concrete is also used for
Cramps. Bars of metal, usually iron or steel, having their
ends turned at right angles to the body of the bar. The
turned ends enter holes in adjacent stones and keep them
from separating (see Fig. 70).
Dowels. Short bars of metal, usually iron or steel, which
enter holes in adjacent stones which are one above the other
(see Fig. 70).
Face. The outside surface of a wall.
Facing. The stones or other material which form the face,
or outside, of a wall.
Filling. The material between the backing and facing.
Header. A stone or block which has its greatest dimension
perpendicular to the face of the wall.
Joints. The mortar layers between the stones or other
block material. The horizontal joints are called bed joints,
or simply beds, and the vertical joints are designated as
joints or builds.
Pointing. A special grade of mortar used in the face of
joints to give better weathering qualities.
Stretcher. A stone or other block material which has its
greatest dimension parallel to the face of a wall.
Quoin. A corner stone or block. A quoin is a header
for one face of a wall and a stretcher for the other face.
Range masonry is the name given to masonry in which
STONE MASONRY 61
FIG. 56. Sketch Showing Arrangement of
Stone in Broken Range Masonry.
the courses are uniform in thickness throughout their ex-
tent. Different courses may have different thicknesses, the
thicker courses being at the bottom of the wall (Fig. 55).
Broken range masonry is that in which the courses
are not continuous
throughout the length
of the structure (Fig.
Random masonry is
that where no attemptis made to form courses
but the stones are
simply cut according to
the size and shape of the place they are to fit (Fig. 57).
Any of the above three terms can be used in connection
with ashlar masonry and squared-stone masonry.
Classification of Stone Masonry. There appears to be
no classification of stone masonry which can be considered as
standard. In general, the usual classifications depend uponthe structure in which the stone is to be used, the nature of
the finish of the stones,
the shape of the stones,
the thickness of the joints,
and the continuity of bed
joints. (See classification
in Chapter VI.)
The classification in gen-
eral use, but with slightly
different definitions, is :
ashlar masonry, squared-
stone masonry, and rubble
masonry.Ashlar Masonry, or cut-stone masonry, is composed of
stones which have their joint surfaces carefully dressed to
approximate planes so that the joints do not exceed one-halfof an inch in thickness; and which have their exposed faces
finished in one of the several ways described in Chapter II.
FIG. 57. Sketch Showing Arrangementof Stone in Random Masonry.
The stones are usually rectangular on the face, but for
architectural work and arches their shape depends upon their
position in the structure. In the best cut-stone work, the
joints do not exceed one-eighth of an inch in thickness.
Figs. 58, 59, and 60 show three styles of ashlar masonry.
FIG. 58. Regular Coursed Ashlar. All Stones of the Same Height.
Dressing Joint Surfaces for Ashlar. The joint surfaces
should be, practically, planes on the beds in order that the
joints shall be uniform in thickness throughout. This in-
FIG. 59. Coursed Ashlar, Using TwoSizes of Stone.
FIG. 60. Irregular Coursed Ashlar,
Courses Have Different Heights.
sures a uniform distribution of the pressure due to the load-
ing. A slight roughness of the surfaces, such as left by tool
marks, is desirable, as it increases the adhesion of the mortar.
If the bed surface of a stone is concave, the edges are liable
to be subjected to greater pressure than the central portion.
STONE MASONRY 63
This condition sometimes leads to spalling on the face when
the loading is heavy. If the bed surface is convex, the high
portion will press through the mortar to a bearing, leaving
the stone in an unstable condition until the mortar is hard.
This condition usually leads to open joints on the face. Thecarefulness with which the bed surfaces are dressed should
be governed by the nature of the structure and the position
of the stone in the structure.
In all structures, the bed surfaces are dressed for the full
depth of the stones. In thick walls, the vertical joint sur-
faces are dressed back for nine or more inches, the remainder
of the surfaces being roughly dressed and permitting thicker
joints. The distance back should always be stated in the
specifications. The backs of the stones are not dressed, but
no considerable overhang should be permitted, as it is
difficult to fill the space under the overhang with the filling
unless a sloppy concrete is employed.
Backing and Filling for Ashlar. Only in very exceptional
cases is ashlar masonry used throughout the body of a mass
of masonry. Generally it is used
only for the exposed faces, the back-
FIQ. 61. Ashlar Masonry with
Brick Backing and Filling.
FIG. 62. Ashlar Masonry with
Rubble Backing and Filling.
ing and filling being composed of a cheaper masonry. In
both architectural and engineering structures, concrete,
brick, and stone are in common use for backing and filling
(see Figs. 61, 62, and 63).
FlQ. 63. Ashlar Masonry with
Concrete Backing and Filling.
In comparatively thin walls,
the backing and filling are laid
up to form courses equal in thick-
ness to the face courses. This is
done to permit of thoroughly
bonding the face stones and the
backing and filling. In large
masses of masonry faced with
ashlar, such as masonry dams, no
attempt should be made to lay
up the backing and filling in
courses. In fact, it is preferable
to have no bed joints extending
through such structures (Fig. 64) .
If the backing of a damis of ashlar masonry, the
courses need not corre-
spond in thickness with
those in the face.
Bond. No two joints
in adjacent courses of
ashlar masonry (or anytype of block
but the stones
should overlap, or
FIG. 64. Ashlar Face Masonry and Rubble Filling without Horizontal or
Vertical Joints. (Muscoot Dam. Reports on the New Croton Aqueduct,
STONE MASONRY 65
breakpoints. The amount of the overlap is a function of the
depth of the course and the size of the stones. A common
specification makes the overlap from one to one and one-half
times the depth of the course. By this arrangement, each
stone is supported by portions of at least two stones immedi-
ately below and supports portions of at least two stones im-
FIG. 65. Ashlar Masonry with Few Headers.
mediately above. This statement applies only to stretchers,
as no joint is permitted immediately above or below a
header. The object of bonding is to bind the stones
thoroughly together and distribute the pressures (Fig. 65).
The strongest bond is obtained by using an equal number
FIG. 66. Ashlar Masonry with an Equal Number of Headers and Stretchers.
of headers and stretchers in the wall, each header in one
course being in the center of a stretcher (Fig. 66) of an ad-
jacent course. In thin walls, the headers should have a
length equal to the thickness of the wall (Fig. 67). In thick
walls, they should extend well into the filling (Figs. 61, 62,
and 63). Headers in the back of a wall should not be opposite
headers in the face (Figs. 68 and 69). Preferably headers
should be at least the size of the face for then: entire length.
In the usual run of masonry from one-third to one-fourth
the area of the face consists of headers.
Where masonry is subjected to heavy blows, as in the
case of sea walls, lighthouses, etc., the stones are carefully
cut with projections on one stone fitting depressions in ad-
jacent stones, and iron cramps, dowels, and bolts used to
tie the stone together thoroughly (see Fig. 70).
Relative Dimensions of Stones. The actual dimensions
of headers and stretchers are dependent upon the structure
in which they are used, the kind of stone, and the facilities
of the quarry from which the stone is obtained. In somestructures and localities, thin stones are necessarily em-
ployed, while in others large stones are used. As a matter
of strength and bond, custom and experience have specified
with some variations the bed of a stretcher as not less than
one and one-fourth times the depth of the course, and the
length as not less than four feet. For headers the width of
the face is specified as not less than the depth of the course
and its length not less than four feet for thick walls. These
specifications apply for heavy masonry.In architectural work, such as the walls of buildings faced
with ashlar, the relative sizes and bonding of the stones
seldom follow the- specifications given above. In buildings
the ashlar facing is, sometimes, merely a veneer of thin
stones set on edge. (This does not necessarily mean that the
stones are not set on natural beds.) These stones are
bonded to the body of the wall by metal ties unless a large
number of headers are employed. This masonry is not
expected to support very much load, as the body of the wall
carries the floors and their loading.
Setting Stone. In setting stone there are a number of
things which must constantly be kept in mind. Assumingthat the particular stone to be set is correctly cut for the
position it is to occupy, it must be transported to the wall
in a manner which does not injure it in any way. Stones
STONE MASONRY 67
FIG. 67. Section of Wall
Showing Headers Ex-
tending from Face to
FIG. 68. Sketch Showing Proper Arrange-ment of Headers.
FIG. 69. Sketch Showing Stretchers and Headers Dovetailed.
FIG. 70. Sketch Showing Construction When Structure Is Subjected to
Strong Wave Action.
FIG. 71. Forged Steel Grab Hooks and Chain. X Varies from 7 to 10 Inches.
Capacity Varies from 2% to 25 Tons. (American Hoist and Derrick
Lead-filled cushionsfor polished stone
Grip 24 inches
Capacity 2000 pounds
FIG. 72. Clamps for Lifting Cut Stone.
STONE MASONRY 69
may be lifted by derricks, the attachment to the stone being
made by grab-hooks, clamps, dowels, or lewis.
Grab-hooks (Fig. 71) are favored by contractors, as theyare quickly handled and can be used for very heavy stones.
Generally, it is necessary to drill holes
for the hooks which mar the face of
the stone, and hence the use of grab-
hooks is not permitted on good work.
For the usual size stone used, the clamp
(Fig. 72) is satisfactory. The wooden
blocks bearing against the stone do
not, in any way, mar the surface.
Dowels (Fig. 74) and the lewis (Fig. 73)
require holes in the top surface of the
stone. Both are satisfactory, and have
the advantage that by their use a
stone can be lowered between other
In setting a stone, a full bed of mor-
tar is prepared and the stone drenched
with water and lowered into place
without in any way disturbing the ad-
jacent masonry. It may be settled
FIG. 73. Lewis for
Lifting Cut Stone.
FIG. 74. Dowels for Lifting Cut Stone, (a) Pin Lewis; Capacity, 1,000 to
into place by light blows with a sledge or stick of
timber, but heavy blows should not be allowed. A goodstone-setter seldom fails to place the stone in its proper
position, as to line and elevation, as it is lowered by the
derrick. Stones for the filling or backing are laid with less
care. In ashlar masonry, where the joints do not exceed
one-half inch, the joints must be filled with care. This is
a tedious job when the stones are large, as the mortar must
be tamped into place if the joint is filled. In rubble masonry,the joints are usually so large that there is little difficulty
in filling them with mortar.
Pointing. Regardless of the kind of mortar employed,
that portion near the exposed face of the joint will be
deficient in density and water-resisting qualities. To pro-
FIG. 75. Joint Facings for Stone Masonry.
vide a complete protection of the joint, the mortar is raked
out for a depth of about one inch before it has become hard.
When the mortar in the joint is thoroughly set and hard,
the raked-out space is filled with a special pointing mortar.
This is usually composed of one part of Portland cement
and one part of rather fine sand mixed with water to a very
STONE MASONRY 71
stiff paste which can be put in place with a trowel, and
tamped in with a special metal caulking tool. The face of
the joint is finished to either a raised, flat, or sunken surface
with a metal tool. Fig. 75 shows several forms of joint
Joint Mortar. The kind of mortar employed usually de-
pends upon the character of the structure. If the masonryis subject to heavy loads and vibrations, Portland cement
mortar should be used, the mixture being about one part
of cement and from two to three parts of sand by measure.
In architectural work, care must be exercised to select a
cement which does not stain the particular kind of stone
employed.The amount of mortar required depends upon the size of
the stones and the thickness of the joints. Baker states
that for three-eighths to one-half inch joints and twelve to
twenty inch courses there will be about two cubic feet of
mortar for each cubic yard of masonry.
Pointing Mortar. According to Patton, pointing mortar"should be neat cement, or at any rate not more than one
sand to one cement, and before being applied should be
allowed to take a set, and tempered with a little water
when ready for use. Good pointing mortar of one sand
and one Louisville cement was used at Point Pleasant,
the mortar being mixed the night before and allowed to
remain overnight, and tempered with a little water whenused."
Most engineers and architects are very much opposed to
re-tempering mortar, but in the case of pointing mortar the
old custom of permitting a set and then re-tempering appearsto lead to good results. The re-tempering gives a consistencywhich permits of caulking and the working of a good finish
on the face of the joint. The mortar is dense and has good
weather-resisting properties. When fresh mortar is used,it is often put in place with a trowel, the only care beingtaken to form a good-looking face finish.
Squared-Stone Masonry. The essential difference be-
tween squared-stone and ashlar masonry is in the thickness
of the joints. In squared-stone masonry, the joints maybe from one-half of an inch to one inch in thickness. Thisdemands less care in dressing the joint surfaces of the stones.
The faces of the stones are usually quarry-faced. It is notuncommon to find squared-stone masonry which would beclassed as ashlar if the joints had been made less than one-
half of an inch in thickness.
Backing and Filling for Squared-Stone Masonry. Thebacking and filling are essentially the same as for ashlar
Bond, Mortar, Sizes of Stones, etc., for Squared-StoneMasonry are practically the same as for ashlar masonry. Of
course the thicker joints
require more mortar.
Baker states that one-
sixth to one-fourth the
mass of masonry is
Rubble Masonry is
composed of unsquaredstones. The joint surfaces are not dressed, and the faces left
as they were quarried. When no attempt is made to formcourses the masonry is
called uncoursed rubble
(Fig. 76), and when the
masonry is leveled at
specified heights it is
called coursed rubble (Fig.
77). Properly laid with
regard to breaking joints
and stability of bearing,
rubble masonry is verydurable either when laid in cement mortar or when laid dry.
When mortar is employed, all joint spaces should be thor-
oughly filled with mortar and spalls. This makes a strong and
durable wall at considerably less expense than ashlar or
FIG. 76. Sketch Showing Arrangement of
Stones in Uncoursed Rubble.
FIG. 77. Sketch Showing Arrangementof Stones in Coursed Rubble.
STONE MASONRY 73
squared-stone masonry. Dry rubble is generally used for
walls retaining earth.
Slope-Wall Masonry is a thin layer of stone, or an inclined
wall, placed on the slopes of embankments, excavations,
river banks, etc., to protect them from the action of wind
and water. (See Chapter VI.)
Stone Paving is used to protect the beds of streams from
erosion, and is used to floor culverts and at the ends of
culverts and similar structures.
Specifications for Stone Paving. "Stone paving shall be
made of flat stones from eight inches to fifteen inches in
depth, set on edge, closely laid and well bedded in the soil,
and shall present an even top surface"
Riprap is stone of any shape and size placed around
piers, abutments, and on the banks of streams to preventscour. It is often dumped into place, but it is much more
effective when arranged by hand.
Strength of Stone Masonry. The strength of stone
masonry depends upon the_kind of stone, the care with
which it is dressed and laid, the bond, the strength of the
mortar, the thickness of the joints, etc. In general, how-
ever, the mortar is the governing feature for strength of
good masonry.As far as known, there is no record of a failure of masonry
construction by crushing, but there are numerous exampleswhere the face stones are spalled on the beds, due to the
loads supported possibly, but more likely due to bad work-
manship or unequal settlement. Little or nothing is known
experimentally about the strength of stone masonry. Struc-
tures in existence, and which show no indications of
failure, carry loads as great as thirty tons per square foot.
(The granite columns of the Rookery Building, Chicago,
moThe following may be considered as safe loads (American
Civil Engineers' Pocket Book, Mansfield Merriman, Editor-
Rubble masonry j.-*v-^w
Squared-stone masonry 200-280Limestone Ashlar masonry 280-350Granite Ashlar masonry 250-400
140-200 pounds per sq. in.
200-280 " " " "
.350-400 " " " "
Measurement of Stone Masonry. There are numerousrules for measuring stone masonry which usually vary in
different localities. It is a safe precaution to state in the
specifications how the measurements shall be made. In
FIG. 78. Sketch Showing Method of Waterproofing a Basement Wall.
engineering work, the actual content in cubic yards is usually
taken, with an additional price per square foot of all surfaces
dressed. In architectural work, it is customary to fix prices
per square foot or per linear foot, according to the position
occupied by the stone.
STONE MASONRY 75
Waterproofing Stone Masonry. Most of the stone in
common use for masonry is practically impermeable, so that
the weak part of the masonry is the joints. If good mortar
is used, and all spaces between the stones are filled with
mortar, no water will pass through the masonry. To make
the surface of masonry impervious, all joints must be care-
fully pointed and all cracks carefully filled with pointing
mortar, then some of the soap and alum washes described
for brick masonry and concrete masonry may be used as a
wash on the face.
When the back of a masonry wall is in contact with water-
bearing soil it can be made impervious by the methods used
for the face. Usually, however, a thin layer of felt and
asphalt is used in the back, in the manner described for
concrete masonry, and this protected by a layer of brick
Cleaning Stone Masonry. After a piece of stone masonryhas been completed, the face is often marred in appearance
by little patches of mortar, dirt, etc. This is readily removed
with stiff brushes and by washing with water. It is quite
necessary that walls in buildings should be cleaned merelyfor general appearance.
In manufacturing cities, the stone-work in buildings,
bridges, etc., becomes soiled from the dirt in the air which
settles on the stone and is distributed in streaks by rains.
For hard stones with smooth faces, this dirt can be removed
with soap and water. For softer stones and irregular surfaces,
a wire brush is sometimes very effective when followed with
soap and water. The use of the sand blast is very efficient
but somewhat expensive. For that matter, all methods of
cleaning high walls are expensive, and, consequently, it is
seldom that they are cleaned after the first cleaning, at the
time the work is completed.
BRICK AND HOLLOW-TILE MASONRY
Brick Masonry includes all forms of masonry composed of
brick and mortar, such as walls of buildings, backing of
stone or concrete masonry, sewers, tunnels, etc., and some-
times bridges, piers, and abutments.
Ordinary building brick is used above ground in walls of
buildings; below ground a hard and nearly impervious brick,
FIG. 79. Finish of Joints in Brick Masonry, (a) Flush Joint. (&) Struck
Joint, (c) Weather Joint.
such as paving brick, should be used, and this class of brick
should also be employed for sewers, tunnels, bridge piers,
Brick may be used simply as a facing, and some other kind
of masonry used for the backing and filling, or an inferior
grade of brick may be used for this purpose.76
BRICK AND HOLLOW-TILE MASONRY 77
Ornamental brick-work in architectural structures is com-
posed of special moulded brick laid in mortar. Such bricks
are used only for facing (Fig. 50).
The terms header, stretcher, joint, bed, bond, etc., have
the same significance in brick-work as in stone masonry.
Joints for Brick-work. The joints in brick-work varyfrom one-eighth of an inch in thickness for pressed brick-
work to three-fourths of an inch in the face brick-work of
some modern buildings, the thick joint being used for archi-
tectural effect. If brick is used for the backing and filling,
the joints are made from three-eighths to one-half of an inch
in thickness. The thickness of the joints is adjusted so that
the filling can be brought level with the facing at intervals
to permit of bonding the two together (Fig. 84).
Mortar for Brick-work. Formerly all brick-work was laid
up in lime mortar, and even now it is extensively used in
small buildings. For large buildings, basement walls, sewers,
etc., cement mortar, or cement mortar containing lime paste,
is employed. While natural cement mortars are used, yetPortland cement mortar is preferable.
Unless the brick used is hard and absorbs but little water,
it must be thoroughly wet before it is laid, otherwise it will
rob the mortar of its water.
Brick-work, properly laid with all voids filled with cement
mortar, forms a monolithic mass which will break as readily
through the bricks as along the joints.
No special pointing mortar is employed for brick-work,but the faces of the joints are formed from the mortar used
in the joints as the work progresses. In some cases where
raised joints are used a special mortar is employed.
Pointing Joints of Brick-work. As just stated, the point-
ing usually comprehends shaping the mortar used in the
joints to form the desired shape on the face. When the joint
surface is a plane, flush with the surface of the wall, it is called
a flush joint (Fig. 79a) ;when the plane surface is inclined
backward and downward, forming a narrow shelf on the
lower course of brick, it is called a struck joint (Fig. 796) ;and
when the surface is inclined upward and backward it is called
a weatherjoint (Fig. 79c). The first and third are preferablewhen weathering alone is considered, and the second when
appearance is the governing quality.
Fig. 79 shows a number of styles more or less in commonuse.
Bond in Brick-work. In ordinary work the bonding is
done by making every fifth or sixth course a course of
headers, and for walls more than one brick thick, care
FIG. 80. Sketch Showing Direct FIG. 81. Sketch Showing Bonding of
Bonding of Facing and Back- Facing and Backing Through the
ing in Brick Masonry. Filling in Brick Masonry.
should be taken that the headers of the face and back bond
together either directly or through the filling, as shown in
Figs. 80 and 81.
For face work where it is not desirable to have headers
show, the secret bonds, shown in Figs. 82 and 83, are used.
When the sizes of the bricks in the filling and the face differ,
some form of metal bond is used, as shown in Fig. 84, or the
filling is brought up level with the face and a secret bond
employed, as shown in Fig. 85.
Fig. 86 shows the face of a wall where the ordinary
arrangement of headers is used.
The bond shown in Fig. 87 is called the Flemish bond,
where every alternate brick is a header.
BRICK AND HOLLOW-TILE MASONRY 79
FIG. 82. Diagonal Secret Bond in Brick Masonry.
FIG. 84. Sketch ShowingMetal Tie Used to BondFace Brick with Backing.
FIG. 83. Another Type of Secret Bond in Brick
FIG. 85. Sketch ShowingUse of Secret Bond in
FIG. 86. Sketch Showing Face of
Brick Wall and Usual Arrange-ment of Headers.
FIG. 87. Sketch Showing Brick Wall with an
Equal Number of Headers and Stretchers.
The English bond, where every alternate course is a header
course, is illustrated in Fig. 88.
In backing up and filling behind ashlar masonry and terra-
cotta it is important that there is a proper bond between
FIG. 88. Sketch Showing Arrangement of Headers and Stretchers in a Brick
Wall. English Bond.
the backing or filling brick and the face. The proper
arrangement is shown in Fig. 61.
Sometimes the facing is made of uniform thickness for the
full height of the wall, and metal ties used to form the bond.
Arches, in brick-work, which do not show are usually built
of a series of header courses with the bricks laid on edge.
FIG. 89. Sketch Showing Method of Arranging Common Brick in an Arch.
Such arches are called row-lock arches (Fig. 89). In face
work the brick should be either ground to shape or especially
moulded (Fig. 90).
BRICK AND HOLLOW-TILE MASONRY 81
Crushing Strength of Brick-work. As in the case of stone
masonry, the crushing strength of brick masonry depends
upon the materials and workmanship, the mortar usually
being the governing feature in good work. A number of
experiments on brick columns have been made on the United
FIG. 90. Sketch Showing the Use of Special Arch Brick.
States testing machine at Watertown, Mass., and publishedin the Reports of the Tests of Metals, etc., which show that
the mortar is the governing factor. The brick piers were
12 inches square and 8 feet high, and the crushing strengths
varied from a few hundred pounds per square inch for
common brick laid in lime mortar to nearly 5,000 pounds per
square inch for hard brick laid in neat cement.
The following safe compressive strengths for brick-work
are given in the American Civil Engineers' Pocket Book,Mansfield Merriman, Editor-in-Chief.
COMMON BRICK HAVING A COMPRESSIVE STRENGTH OF 1,800 POUNDSPER SQUARE INCH
When laid in Portland cement mortar 175 Ibs. per sq. in.
When laid in natural cement mortar 150 " " "
When laid in lime and cement mortar 125 " " "
When laid in lime mortar 100 " " "
SELECT HARD COMMON BRICK HAVING A COMPRESSIVE STRENGTHOF 2,500 POUNDS PER SQUARE INCH
When laid in 1 : 3 Portland cement mortar 200 Ibs. per sq. in.
When laid in 1 Portland cement, 1 lime paste, and3 of sand mortar 175 " " "
Paving brick laid in 1 : 3 Portland cement mortar. .350" " "
Lintels Supporting Brick Masonry. The actual load on
a lintel is very uncertain. If the masonry is considered to
act as a fluid, then the load is the weight of all of the masonryabove the lintel, including such loads as may be transmitted
to the wall from floors, etc. While this assumption is on the
side of safety, it undoubtedly leads to lintels very muchheavier than necessary. The more usual assumption is to
consider the weight of a triangle of masonry which has for
its base the span of the lintel and its side making an angle
of 45 to 60 with the base. This assumption may also be
questioned, but for ordinary openings it is usually safe.
Efflorescence. The white efflorescence often seen on the
face of brick walls is usually due to water which dissolves
the salts of soda, potash, magnesia, etc., contained in the
lime or cement mortar. Sometimes the efflorescence appearson brick which has been burned with coal containing sulphur,
or made from clay containing iron pyrites. When such bricks
get wet, the water dissolves the sulphates of lime and mag-
nesia, and, as the water evaporates, crystals of the salts are
left on the surface of the brick. The principal objection to
efflorescence is the appearance. It can be prevented bymaking the face of the wall water-proof. Sylvester's washes
have given good results. "The process consists in using
two washes or solutions for covering the surface of the walls
one composed of Castile soap and water, and one of alum
and water the proportions are three-fourths of a pound of
soap to one gallon of water, and one-half pound of alum to
four gallons of water; both solutions to be perfectly dis-
solved in water before using. The walls should be perfectly
dry, and the temperature of the air not below 50 F. whenthe compositions are used.
"The first soap wash should be laid on when fairly hot,
with a flat brush, taking care not to form a froth on the
brick-work. This wash should remain 24 hours so as to
become dry and hard before the second, or alum, wash is
applied, which should be done in the same manner as the
first. The temperature of this wash, when applied, may
BRICK AND HOLLOW-TILE MASONRY 83
be 60 or 70 F.; and this also should remain 24 hours before
a second coat of soap-wash is put on. Then coats are applied
alternately until the walls are made impervious to water.
The alum and soap thus combined form an insoluble com-
pound, filling the pores of the masonry, and entirely pre-
venting the water from entering the wall."
Since most of the efflorescence is due to the mortar, a
large portion of it may be prevented by using imperviousmortar.
The Sylvester washes have been successfully used for
water-proofing walls under ground and reservoir walls.
Measuring Brick Masonry. In figuring the cost of brick-
work, it is customary to base the estimate on the cost per
thousand brick in the wall. The cost of laying different
forms of masonry is provided for in the method of measure-
In plain walls, no deductions for openings of less than 80
square feet in area are made, and when deductions are madefor larger openings the width is taken as two feet less than
the actual width of the opening. Hollow walls are measured
as if solid. Footings are measured in the wall by adding the
width of the projections to the height of the wall. Flues in
chimneys are measured solid. Detached chimneys, etc., are
measured as a wall having a length equal to the sum of one
side and two ends, and a thickness equal to the width of the
Water-proofing Brick Masonry. All brick masonry which
is in a damp location should be built of impervious brick,
with good Portland cement mortar filling all voids. Such
masonry will be "water-tight." If impervious brick cannot
be used, then surface of the masonry may be treated with
some of the washes described for concrete masonry, or a
water-proof layer of asphalt and felt may be used in the
same manner as for concrete masonry. Basement walls are
often plastered with Portland cement mortar on the outside,
but unless this is well done it is not very satisfactory.
Cleaning Brick Masonry. As in the case of stone masonry,
all new work must be cleaned, and, for brick-work, stiff scrub
brushes and water do the work very well. This is assumingthat the face brick are hard. Mortar sometimes sticks to soft
brick and requires a metal tool to remove it.
Enameled brick can be cleaned with caustic soda or
sodium carbonate/which does not have any effect upon the
8 Natco Block .
Projecting Dove TailScored for Stuccoand Plaster.
DETAIL OF CORNEROF 8'WALLSCALE ONE FOOT
Projecting Dove TailScored for Stuccoand Plaster,
12"Blocks used for
Foundations, and for
Exterior Walls whereHeavy Loads are to
DETAIL OF CORNEROF 12*WALLSpecial Corner
Block for 10*Wallis4*xlO"xl2?
FIG. 91. Detail of Foundation and Exterior Wall Construction. Exterior
to be Finished with Stucco and Interior Plastered. (National Fire-
brick or cement and lime mortar. Sulphuric, nitric, and
hydrochloric acids do not affect enameled brick, but do,
even when diluted, affect both lime and cement
Hollow-Tile Masonry is composed of hollow blocks laid
BRICK AND HOLLOW-TILE MASONRY 85
in cement mortar. The masonry may be used for backing
only, or it may form the entire wall. The blocks are laid
Natco Tile X
Wire Screen L~
PLAN AT A-A
Wire Screeni__ IIUM,,,!,.,.. ,...,,M, .1 I, ....... .fl
SECTION THRU C-C PLAN AT B-B
FIG. 92. Section of Exterior Wall with Brick Facing and Hollow-Tile Backing.
Showing Method of Bonding and Sealing Vertical Holes. (National
with the openings horizontal, and also with the openingsvertical. When the openings are vertical, wire mesh is laid
in the horizontal joints to hold the mortar in place. The
mortar is composed of one part cement, and two parts sand.
Lime paste not exceeding ten per cent of the mass byvolume may be used in the mortar. Figs. 91, 92, and 93 show
a few details of hollow-block and terra-cotta construction.
FIG. 93. Details of Terra-Cotta Construction as Used in Steel Skeleton
Concrete used in masonry construction is "a compact
mass of broken stone, gravel, or other suitable material
assembled together with cement mortar, and allowed to
harden," thereby making an artificial stone. Concrete is
being substituted for brick and stone in all classes of struc-
tures. Sometimes it is cast in the shape required and laid
the same as stone masonry, and sometimes forms are built
and the structure cast as a whole. Both methods have their
advocates for many different classes of structures. At the
present time, the casting of concrete in the place it is to
occupy appears to be more in favor than the casting of
small units which are afterward assembled. In many cases,
the nature of the structure will govern the method used.
For example, concrete which is to be subjected to the action
of sea water must be allowed to harden before coming in
contact with the salt water. If it is not feasible to construct
a water-tight form in which to cast the concrete structure,
then it must be cast in parts in the open air and the parts
deposited in the sea water when they have become hard.
Balustrades composed of rails and balusters are more eco-
nomically cast in parts on account of the expensive moulds
Reinforced Concrete is concrete strengthened by the intro-
duction of metal, usually in the form of woven wire mesh,
expanded sheet metal, or metal rods. Reinforced concrete
construction and design are considered in special works uponthe subject, and, consequently, such constructions will not
be treated here, except in a very limited way.
Reinforcing Concrete for Shrinkage, etc. In order to
prevent cracks in long walls, which are due to the shrinkageof the concrete in hardening, changes of temperature, and
slight settlements, longitudinal reinforcement composed, usu-
ally, of iron or steel rods is introduced. This reinforcement
should be placed two or three inches from the exposed sur-
faces of the structure to resist cracks due to changes of
temperature, but for preventing cracks produced by shrink-
age it should be uniformly distributed over the cross-section
of the concrete. If no settlement occurs, there will be no
cracks due to settlement, and, consequently, no reinforce-
ment will be required. The above conditions make the
determination of the amount and the arrangement of the
reinforcement quite uncertain. Some contend that from
0.1 to 0.2 per cent of the area of the concrete section, in
steel, is sufficient to prevent cracks in long walls, while others
believe that from 0.2 to 0.4 per cent of steel is necessary to
prevent large cracks due to shrinkage and changes of tem-
perature. The reinforcement should be in small units and
placed near the surface of the concrete, with more reinforce-
ment near the exposed surfaces than near those protected.
When no reinforcement is used, vertical joints are made
every 25 or 30 feet to permit of slight changes of position
of the blocks between the joints. To prevent lateral move-
ments, the joints are usually made so that projections on
the blocks enter recesses in the adjacent blocks.
Constituents of Concrete. Concrete, as generally under-
stood in building, is composed of Portland cement, sand, and
broken stone. Gravel is often substituted for broken stone,
and, when bank gravel contains the proper amount of sand,
it is used as it comes from the bank.
In order to obtain the most economical concrete, the sand
and broken stone or gravel should be screened to various
sizes and then mixed so that the voids will be a minimum.
This insures a uniform mixture requiring a minimum amount
of cement and water. The coarse and fine aggregates should
be clean, and the water free from dirt or any impurities
which will have any deleterious action upon the cement or
Proportions of Materials for Concrete. The materials
CONCRETE MASONRY 89
are usually proportioned by measure, using the cubic foot
as a unit. That is, a 1 : 2 : 4 mixture means one part of
cement, two parts of fine aggregate (sand), and four parts
of coarse aggregate (broken stone or gravel) by measure.
One bag of Portland cement, weighing not less than 94
pounds, is considered as one cubic foot of cement. The
materials, including the water, should be measured separately
and then combined.
The proportions of constituents for concrete depend uponthe class of structure in which it is used. The following
proportions are approximately those in common use.
For structures where mass is of more importance than
strength, such as the interiors of abutments and piers for
arch bridges, the interiors of large piers for bridges, etc.,
1 : 3 : 6 to 1 : 4 : 8.
For piers, abutments, massive reinforced concrete work,
etc., 1 : 2.5 : 5 to 1 : 3 : 6.
For thin-walled structures and impermeable concrete,1 : 2 : 4 to 1 : 2.5 : 4.5.
For extra strong reinforced concrete, 1:1:2 to 1:1.5:3.In all cases, enough water is added to make the mixture
of the proper consistency.
Mixing Concrete. Concrete may be mixed by hand or
by machine. As far as quality is concerned, either methodis satisfactory when the work is properly done. The materials
must be thoroughly mixed so as to form a homogeneousmass. In hand mixing, the dry materials are mixed on awooden platform until the mass is uniform in color, andthen the water is added and the mass turned until, it is of
a uniform consistency. In machine mixing, the dry materials
are placed in the drum of the machine, and water added as
the drum revolves.
There is considerable difference of opinion as to the proper
consistency of concrete. Considering the practical side of
the question, a consistency of a fairly thin cream appearsto lead to the best results. This consistency permits of easy
handling, and the concrete readily flows into all parts of the
moulds or forms, and, if agitated near the surface of the
forms, the outside surface of the concrete will be free from
holes. For small pieces, and where the number of pieces of
the same pattern is large, a relatively dry mix is used, in
order that the moulds may be almost immediately removedand used over again.
Machines for Mixing Concrete. Machines for mixingconcrete are of many patterns and capacities, from the small
FIG. 94. Ransome Concrete Mixer. (Ransome Concrete Machinery Co.)
mixer turned by hand and fed with shovels to the mixers
operated by power which measure all of the materials and
deliver the finished product in a continuous stream. In
general, mixers may be divided into two classes, batch mixers,
and continuous mixers. Continuous mixers are not ap-
proved by most engineers, owing to the difficulty in obtain-
ing a homogeneous concrete by their use.
Batch mixers deliver a certain amount of concrete at
intervals, and all operations are under control at all times.
The modern forms consist of a movable skip, into which the
measured ingredients are dumped, the skip is then elevated
and the contents dumped into a drum which is kept con-
stantly revolving. The proper amount of water is intro-
CONCRETE MASONRY 91
duced into the drum, and, when the mixing has progressed
to the proper point, the drum is tilted and the concrete dis-
charged into wheel-barrows, skips on cars, or other devices
for transporting the concrete to its final destination. Themovable skip and the revolving drum are operated by either
FIG. 95. No. 104 Smith "Mascot" Mixer on Truck with Gasoline Engine,Power Charger, and Water-Tank. Skip in Discharging Position. (TheT. L. Smith Co.)
a steam, gasoline, or oil engine. In case the drum of the
machine does not tilt, a gate is opened for the discharge of
the batch. Fig. 94 shows a non-tilting type, and Fig. 95
one where the drum tilts.
Concrete Building Blocks are moulded pieces of concrete,
usually of the hollow-block type, having rectangular faces
and walls from two to three inches thick. The size is suchthat they can be handled by one man. The finish of the
face is made to imitate any of the cut finishes on natural
stone, but, as ordinarily executed, the imitation is quite
evident, and therefore not pleasing. In exceptional cases,
the faces are so well finished by hand that a close examination
is necessary to detect the counterfeit, but such finishes are
expensive and are seldom employed.
Practically all concrete building blocks are moulded by
machines, and, in order that the block may be removed
FIG. 96. Concrete Block 8 x 8 x 24 Inch Granite Faced. Zagelmeyer Process.
(Zagelmeyer Cast Stone Block Machine Co.)
from the machine as soon as formed, a minimum amount
of water is used, often less than necessary for the complete
setting of the cement; consequently, the blocks are quite
porous and absorb moisture readily. Sometimes the face is
formed from a thin layer of rich mortar which is backed
with a lean mixture. This decreases the porosity of the
face and makes a more durable block.
Dry casting can be employed, and excellent blocks made,
if, after the blocks are removed from the moulds, they are
CONCRETE MASONRY 93
kept in a saturated atmosphere for 24 hours or longer, and
then kept wet with water for a few days.
To secure good results, good materials properly propor-
tioned must be used. There are thousands of concrete blocks
being made and used which should be condemned owing to
FIG. 97. Showing a Number of Different Face Patterns for Concrete Blocks.
the use of poor aggregates and not enough cement. Such
blocks are very porous and absorb large amounts of water,
making damp walls. The blocks are also lacking in strength
Various natural stones are imitated in color and structure
by embedding in the face small clean chips of the stone to be
imitated. The best results are obtained when the face is
a plane surface. While quarry-face appears to be the uni-
versal finish for concrete blocks, it is almost impossible to
get a satisfactory appearance from moulding. Figs. 93, 96,
and 97 show a common shape for concrete blocks, and Fig.
98 shows another form in a wall.
Architectural Concrete. By using the proper materials
and moulds, and exercising care and judgment in their use,ustone concrete" can be cast in any form desired, from blocks
to be laid as ashlar masonry to columns and their capitals.
In fact, entire buildings of classic design have been con-
structed entirely of concrete, and, unless examined closely,
they have all characteristics and appearance of buildings
constructed of cut stone. Such buildings, however, are
exceptions. The usual construction is so poorly finished
FIG. 98. Showing Wall Constructed of Concrete Blocks. (American
Hydraulic Stone Co. Barren and Harridge.)
that it has none of the characteristics of natural stone work.
It is much better practice not to attempt the imitation of
cut stone, unless well done, and simply let the structure
show that it is made of concrete. This is accomplished by
CONCRETE MASONRY 95
having all surfaces planes, whether the walls are made of
blocks or cast in place.
The moulds used in casting architectural concrete are
made of wood, plaster of Paris, sand, or metal. Sand and
metal moulds give very good results where a large number
of pieces of simple patterns are to be cast.
Surface Finish for Concrete Blocks. If the face of the
block is made of 1 : 2 mixture of cement and limestone
screenings, and it is finished by placing the block face down on
a revolving metal disk covered with wet lake sand (or anyclean hard and fine sand) ,
the result will be a plane surface,
smooth and uniform in appearance. This is not an expensive
operation, and the excellent appearance of the blocks whenlaid in a wall is ample return for the expense. Of course, anyrock other than limestone can be used.
A rock-face finish of natural stone can be made by first
placing about a half-inch of sand over the bottom of a mould
and then arranging spalls of natural stone on the sand,
pressing each piece to a firm bed; then enough mortar (mixedwr
et) consisting of equal parts of sand and cement is pouredover the spalls until they are covered, and then the body of
the block is poured of the usual concrete mixture. The blocks
are left in the moulds 24 hours. When properly done, the
spall-face blocks are a great improvement over the usual
The Zagelmeyer block (Fig. 96) is faced with very small
pieces of natural rock (a coarse sand made by crushing the
rock) . This sand is bedded in glue on the face plate of the
machine and then backed up with mortar and concrete. Themoisture in the mortar softens the glue so that the block,
when removed from the machine, carries the natural stone
sand embedded in the mortar.
Monolithic and Mass Concrete. When an entire structure
is composed of concrete cast in place without joints it maybe called monolithic concrete. If there are occasional joints
to provide for contraction, expansion, etc., it may be called
mass concrete. Nearly every structure which can be built
of stone or brick can be made of mass concrete. This in-
cludes buildings, footings for walls, bridge piers and abut-
FIG. 99. Ransome Steel Tray Barrow. Capacity, 3 Cubic Feet.
ments, water towers, reservoirs, dams, tunnel linings, sewers,
arch bridges, etc.
Forms are so constructed that the concrete is cast in the
exact shape desired.
FIG. 100. Ransome 6 Cubic Feet Capacity Concrete Cart.
Depositing Concrete in Mass Construction. Concrete is
deposited in a great many different ways, depending uponthe magnitude of the work and the plant available. In
small work, it is usually taken in wheel-barrows or special
CONCRETE MASONRY 97
carts (see Figs. 99 and 100) from the place of mixing to
the forms where it is to be deposited, and dumped into the
forms. Care must be taken to see that the coarse aggregatedoes not separate from the mortar. This is a function of
the consistency and height of fall. If wheel-barrows are not
FIG. 101. "Ransome" Plant for Mixing and
used, the mixing platform or the machine is moved as thework progresses, the concrete being shoveled directly into
the forms from the mixing platform or as discharged fromthe machine.
For large buildings, walls, bridges, etc., the mixing plant
is usually stationary, and the concrete is taken to its destina-
tion by first elevating it in a bucket in a tower (Figs. 101
and 102), and then dumping it into carts or troughs or chutes
FIG. 102. Floating Mixer Plant Delivering Concrete Through Chutes. Gun-
powder River Bridge. (Engineering Record, May 2, 1914.)
of wood or metal leading to the place where it is to be de-
posited. The troughs are changed as the work progresses.
Here, again, the question of consistency is important. The
usual consistency is too thin in order that the concrete will
flow readily in the troughs. Unless the consistency is right,
and the inclinations of the troughs are carefully considered,
the mortar and coarse aggregate are quite likely to separate,
and must be re-mixed in the forms by"spading."
For bridge piers, the concrete is often mixed on land and
transported in buckets on small cars running on rails sup-
ported by a light trestle, to the pier being built, where the
bucket is lifted by a derrick and swung and lowered to the
place where the concrete is to be deposited
Mixing and Depositing Concrete by Compressed Air.
This method has many advantages over the usual methods,
especially when the concrete is to be transported long dis-
tances and the place where it is to be deposited is not easily
accessible with buckets or chutes. The apparatus consists
CONCRETE MASONRY 99
of a pneumatic mixer (Fig. 103) and pipe for transportation.
The mixer is a conical drum with a feeding hopper on top
and a delivery elbow at the bottom. Pipes for compressed
air are provided, one at the top of the machine and one at
the heel of the delivery elbow. The concrete aggregates,
FIG. 103. The Pneumatic Concrete Mixer. (Concrete Mixing & Placing Co.)
cement, and water are passed into the machine through the
hopper at the top, which is then closed by a door operated
by compressed air (the closing air cylinder is shown in Fig.
103). Air is admitted above the charge, which forces it
downward into the elbow at the bottom where air, admitted
at the heel of the elbow, assists in forcing the concrete
through the delivery pipe. The mixing of the materials
takes place during the time it is moving forward under the
action of air at not less than 80 pounds pressure. For the
usual size broken stone or gravel used in mass concrete, an
eight-inch delivery pipe is used. The mixers are made in
Blow-off when Mixing
Grout Dischargeto Place
FIG. 104. Ransome-Cannif Grout Mixer. (Ransome Concrete MachineryCo.)
one-quarter and one-half yard sizes and will deliver about30 and 60 yards of concrete per hour.
Mixing and Depositing Grout by Compressed Air. Small
spaces back of tunnel linings, fissures in rock, etc., can be
completely filled with grout composed of one part cementand one part sand by the Ransome-Cannif grout mixer. Theconstruction of this mixer is shown in Fig. 104. The cementand sand are delivered to the mixer through the charging
door, with the proper amount of water. The materials are
mixed by permitting compressed air to enter at the bottom
CONCRETE MASONRY ', i^
of the mixer and blow through the mass, the blow-off valve
at the top being open. When the grout is thoroughly mixed,
the blow-off valve is closed and the air supply diverted to
the top of the machine. This forces the grout into the dis-
tributing pipe and to its destination. When two or more
mixers are used in a battery, it is possible to keep up a con-
tinuous flow of grout through a two-inch pipe. A battery
of three mixers, working under an air pressure of 300 pounds,
has delivered a batch of grout every 30 seconds for 24 hours
a day for several months, without a stop.
Mixing and Depositing Concrete in Freezing Weather.
Unless it is absolutely necessary, it is better not to mix and
deposit concrete in freezing weather. If the work must be
executed in such weather, then the aggregates and the water
must be heated before being mixed. Since the chemical
action of the setting of cement-paste produces a rise in
temperature, if the warm concrete is deposited in forms it
will become sufficiently hard before its temperature falls to
that of freezing, to prevent any injury from freezing,
especially if the top surface is protected with straw or other
means after concreting has been stopped.
Sometimes salt is dissolved in the mixing water, the per-
centage depending upon the temperature. (See Chap-ter VI.)
The water is usually heated by turning steam into the
water barrel or tank. The sand and broken stone may be
heated by piling it over an old boiler shell in which a fire
is kept burning, or steam may be turned into the pile throughseveral pipes.
The following instructions should be carefully adhered to
in doing work in freezing weather.
Do not use too much salt, as it affects the ultimate strengthof the concrete.
See that the aggregates are uniformly heated and that
they contain no lumps.See that the forms are absolutely free from ice.
Deposit each batch of concrete as soon as it is mixed, and
do not let its temperature be less than 50 F. when it reaches
Do not remove the forms until the concrete has been
In the case of building construction, the work may be
enclosed with canvas on the sides and top, and salamanders
placed beneath the new work.
Depositing Concrete Under Water. While it is possible
to place concrete in running water, yet the results are far
from certain. Unless a coffer-dam is very expensive, it is
FIG. 105. Bottom Dump Bucket. Capacity, in Cubic Feet, 15 to 75. (Insley
better to construct such a dam and place the concrete in
still water. In case a metal or wooden dam cannot be built,
a wall of concrete in sacks may be employed as a substitute.*
The concrete is made rich and not too wet, and is placed in
gunny sacks, filling the sack about two-thirds full. Thesacks are then lowered and placed by a diver who arranges
* For methods employed in constructing coffer-dams, see Foundations : AShort Text-book on Ordinary Foundations, including a Brief Description of
the Methods Used for Difficult Foundations. By Malverd A. Howe. John
Wiley & Sons, Inc., New York.
CONCRETE MASONRY 103
them so as to form a well-bonded wall. Each sack is firmly
pressed into place. The sacks are sufficiently loose in struc-
ture so that considerable mortar oozes through them, thereby
cementing the units into one mass. Paper sacks have been
used, but the gunny sacks are very much to be preferred.
When the wall has reached a sufficient height to insure still
rFlangeConnection Water Level
FIG. 106. Tremie Empty, Sealed, and Ready to be Raised. (Engineering
Record, August 15, 1914.)
water within its perimeter the concrete is deposited either
by means of a drop-bottom bucket or a tremie. When a
drop-bottom bucket (Fig. 105) is used, it should be lowered
as far as possible and permit the opening of the bottom so
that the concrete will be washed as little as possible.
Atremie (Fig. 106) is preferable to the drop-bottom bucket.
This is simply a tube of wood or metal with a hopper at the
top through which the concrete is passed. The tremie is
usually suspended by a cable so that it can be raised and
lowered and also moved horizontally. To use the tremie, it
is first lowered until the bottom is sealed, and then the water
inside the tremie is displaced by concrete. When the tremie
is full of concrete, it is raised a little to permit the concrete
to run out at the bottom, displacing the water, and not pass-
ing through it. Concrete is placed in the hopper as fast as
it runs out of the bottom. When the concrete stops flowing
FIG. 107. Tools for Finishing Concrete Surfaces, (a) Ransome Concrete
Axe. (*>) Bush Hammer with Four Points.
the tremie is moved a little horizontally, permitting the con-
crete to flow again. In this way layers of constant elevation
are put in place. The thickness of a layer which can be suc-
cessfully deposited depends upon the consistency of the con-
crete and the rate at which concrete can be supplied to the
tremie. Thin layers are easier to manage than thick layers.
The concrete should be quite wet so that it will spread lat-
erally after leaving the bottom of the tremie. The top sur-
face of each layer should be horizontal and free from holes.
Properly managed, concrete deposited in still water througha tremie is as good as that deposited in the dry.
Finishing the Surface of Concrete. In mass construction
and, sometimes, in block work, the surface of the concrete
is given an additional finish from that left by the forms.
The marks left by the forms can be fairly well and easily
removed by rubbing the surface with a brick of carborundum,
CONCRETE MASONRY 105
emery, concrete, or soft natural stone, if the forms are re-
moved before the concrete becomes too hard. The surface
may be given a similar finish by rubbing it with a wooden
float, and using sand and water to cut the concrete.
Bush-Hammer Surface Finish. The surfaces of mass
concrete, walls of buildings, concrete blocks, etc., can be
finished with the bush hammer operated by hand or by a
pneumatic hammer. Fig. 107 shows two hand tools which
have been successfully used. When the bush hammer is to
be used, the concrete should stand at least three weeks after
being deposited and several weeks longer if possible, as the
harder the concrete becomes the better will be the surface
produced. Various styles and weights of hammers are used.
The hammer with four points, shown in Fig. 107, weighsthree pounds, and the points are two-thirds of an inch apart.
Any of the pneumatic tools used for dressing natural stone
can be used on concrete, judgment
being exercised in selecting the tool
suitable for the age and texture of
There are no objections to the
use of bush hammers on concrete,
provided the concrete is fairly rich.
The hammer removes the mortar
on the surface which decreases the
imperviousness of lean mixtures.
Spaded Finish for Concrete Sur-
faces. In mass concrete, if the
forms are carefully built so as to
have a smooth and even surface,
the concrete can be "spaded"
against them so as to give a finished surface requiring nofurther treatment. Fig. 108 shows two tools used in"spading."
Brushed Concrete Surfaces. To obtain a brushed finish,
the forms must be removed as soon as can be done safelyand the surface brushed with a wire brush or an ordinary
FIG. 108. Ransome Tampers,
scrubbing brush, using water freely. The wire brush which
gives satisfactory results is about four inches wide and is
made by clamping together a sufficient number of sheets of
wire cloth. After the surface has been brushed, the appear-ance can be greatly improved by washing it with a diluted
FIG. 109. Brushed Concrete Surface. Foundation Indiana Tuberculosis
Hospital. (Concrete Surfaces, Universal Portland Cement Co.)
solution of acid applied with a brush. While the surface
is wet with the acid wash, it should be immediately scrubbed
with a brush, and then the acid removed with water freely
applied. The acid cleans the aggregate (Fig. 109).
"A solution of one part commercial muriatic acid to two
or three parts of clean water should be used on surfaces in
which standard Portland cement is used and a sulphuric-acid
solution of the same strength when white Portland cement
and white aggregates are used in the facing mixture." (Uni-
versal Portland Cement Company.)Plaster Coats are not as a rule very satisfactory, as they
almost invariably crack unless in a locality where there is
little change in temperature and moisture. The surface of
the concrete, in all cases, must be thoroughly cleaned before
CONCRETE MASONRY 107
the plaster coat of mortar is applied, and the coat should be
given only enough troweling to give an even surface.
Sand-Blasted Surfaces. "A finish very much the same
texture and appearance as that obtained by brushing while
green may be obtained by sand-blasting a thoroughlyhardened concrete surface. Any pronounced ridges or ir-
regularities in surface, formed by cracks or open joints in
the forms, should be removed by tooling, and any pointing
that may be necessary should be done several days before
the surface is sand-blasted.
"Upon a smooth, dense, thoroughly hardened concrete
surface a three-eighth inch nozzle may be used, but under
ordinary conditions one-quarter-inch or even one-eighth-inch
nozzles have been found to give the best results. A clean,
sharp, thoroughly dried silica sand or crushed quartz is most
effective for sand-blasting, and for use with a one-quarter-
inch nozzle the sand should be screened through a No. 8
screen, and through a No. 12 when a one-eighth-inch nozzle
is used. The best results are apparently obtained on a
thoroughly hardened concrete surface at least a month old,
and for such work a nozzle pressure of from 50 to 80 poundswill be required." (Universal Portland Cement Company.)With a special attachment, the cement-gun, described later,
can be used for sand-blasting.
Pebble Finish. A pebble finish is obtained by usingrounded pebbles in the face concrete, and "
against the forms. If the forms are removed before the con-
crete is too hard, the mortar between the pebbles can be
brushed out until about half the surface of the pebbles is
exposed. This finish is successfully accomplished when the
mortar is about one day old, except in cold weather, whenthe age should be greater. The same results can be obtained
by plastering the forms with clay and sticking the pebblesin the clay just before the concrete is deposited. In this
case, the clay is washed out and this can be done any timeafter the forms are removed.
Special Surface Finish for Concrete. "A method of
finishing exposed concrete surfaces has been developed bythe engineers of the South Park Commissioners of Chicago,and successfully used by them in the erection of large mono-lithic concrete buildings. By using a comparatively lean,
dry mixture for the entire thickness of their walls and as a
facing for heavy walls, a concrete surface is obtained which
FIG. 110. Sectional Views of Type G. L. Cement-Gun. Air Pressure, 100
Pounds. (Cement-Gun Company, Inc.)
does not take the imprint of the form imperfections, and
which requires no further treatment after the removal of
the forms. For this work, they use a mixture composed of
about one part cement, one and one-half parts sand, and
four and one-half parts crushed limestone screenings passing
a one-half-inch screen, and from which the fine material has
CONCRETE MASONRY 109
been removed by re-screening through a quarter-inch screen.
. . . The concrete is thoroughly mixed so dry that no
mortar flushes to the surface when it is rammed into the
forms which are constructed in the usual manner.
"The resulting surface has a rough, porous texture of a
uniform, soft cement-gray color. Contrary to what mightbe expected of a surface which absorbs considerable moisture,
work that is six years old shows no evidence of injury from
frost. It is also possible to obtain sharp, clean-cut lines for
architectural details and mouldings, and a surface which
remains remarkably free from discolorations due to efflores-
cence." (Universal Portland Cement Company.)Cement-Gun Surface Finish. A very dense, impervious,
and satisfactory surface finish can be given mass concrete
or architectural concrete by the use of the cement-gun (Figs.
110 and 111). This machine forms a cement mortar coating
l" Sand and Cement
FIG. 111. Details of Hose Connections and Nozzles Used with the Cement-Gun. (Cement-Gun Company, Inc.)
by blowing the materials through a nozzle against the surface
to be covered. In operating the machine (Fig. 110), the sand
and cement are passed into the chambers A and B throughthe cone valves C and D, which are opened by means of levers
on the outside. After the chambers A and B are filled, the
cone valve C is closed and compressed air admitted throughthe valve N, which holds the valve C closed in the positionshown in Fig. 110. The air valve P is then opened, whichmakes the feed wheel K revolve. This wheel has pocketsaround the circumference which are filled with the dry
materials. As the wheel revolves, each pocket in turn passes
through the goose-neck R, where its contents are blown into
the hose leading to the nozzle (Fig. 111). The material re-
mains in a dry state until it reaches the base of the nozzle,where water is admitted from the side. When the mixture
reaches the surface to be covered, it immediately forms a
dense coating of mortar. The final surface may be that
left by the gun, or it may be brushed with a whisk broom.In case the concrete to be coated is old, it should be sand-
blasted before the mortar is deposited. This can be donewith the cement-gun by using the proper nozzle.
The cement-gun has been used to coat steel in buildingsand bridges, to cover wooden piles, and to fill cracks in massconcrete.
Forms for Mass Concrete are usually constructed of wood,
although there are a number of patented portable metal
form in use. Wooden forms are made of vertical studs to
which boards are nailed. The studs are usually two by four
FIG. 112. Sketch Showing Wire Ties in Concrete Forms.
inches or two by six inches spaced about two feet apart for
inch boards. The inch boards are dressed on one side to a
uniform thickness and with both edges straight and parallel.
The boards are nailed to the studs so as to make as smooth
and even a surface as possible without cracks. Matchedlumber and boards beveled on one edge are sometimes used.
CONCRETE MASONRY 111
The walls of the forms are kept in position either by bracing
on the outside or by ties running from the back to the front
wall. For ordinary work, No. 8 wire is used for ties, and
for very heavy work No. 7 or No. 6 wire is employed. Fig.
112 shows the arrangement of the wires, and Fig. 113 shows
Cross Section Forms
FIG. 113. Ratchet Form Clamp, (a) Anchor for One End of Wire. (6)
Ratchet Tightener at Other End of Wire, (c) Lever for OperatingRatchet. (Peerless Form Clamp Co.).
one mechanical device for tightening the wires. Where the
surface of the concrete is exposed, the use of wires makes it
difficult to produce a good surface appearance, as the wires
extend through the surface and must be cut off, leaving ends
more or less exposed. This difficulty is avoided by usingthe device shown in Fig. 114.
The lumber used in wooden forms can be used a second,
and sometimes a third time, for unexposed surfaces, but
for exposed surfaces it is better to use new lumber in order
that it may be true to line and shape.
Wetting and Oiling Forms. If the form boards are dry,
they should be wet before the concrete is deposited to pre-
vent the absorption of water from the surface concrete. If
the forms are to be quickly removed, the boards may be
oiled with crude oil to fill the pores and thereby prevent the
concrete from sticking to the wood. For the same purpose,and also to make a smooth surface, oiled paper and sheet
metal have been used for mass work. Where the forms are
not removed for several days, a thorough wetting is all that is
necessary. Even if the planks are dry, the concrete will
FIG. 114. Universal Form Clamp Used with Round Rods with Nut on OneEnd. (a) Clamp on Free End of Rod. (6) Device for Pulling Rod whenForms are Removed. (Universal Form Clamp Co.)
not stick to them, as its cohesion is greater than the adhesion
to wood. The faces will show the marks of the forms.
Rubble Concrete is concrete in which are placed large
and small stones. Where stone is plentiful, this makes a
more economical structure than if composed entirely of con-
The stones should be far enough apart to insure that all
spaces can be readily filled with concrete. The stones should
be washed free of dirt, and be wet when placed in the con-
crete. They are usually dropped into the concrete, and the
77to remove entrained air. From 50 to
70 per cent of the structure may be stone. This kind of
CONCRETE MASONRY 113
construction is used for heavv piers, abutments, large walls,
dams, etc. (Fig. 115).
Waterproofing Concrete. Concrete structures may be
waterproofed in two ways: (a) by making the concrete im-
FIG. 115. Cross-Section of Shirawata Dam, Showing Large Stones Em-bedded in Concrete. (For Description see Engineering Record, Novem-ber 8, 1913.)
permeable, and (6) by making the surface of the concrete
In mass concrete, such as dams and large piers and walls,
concrete with graded aggregates deposited very wet, that is,
having a consistency of very thin cream, and well"spaded
to remove air bubbles, will usually be impermeable. If not
absolutely impermeable at first, it will become so after a
short lapse of time. If, however, there is carelessness in the
workmanship at any point, the concrete at that point will
not be impermeable, and, if cracks occur, the structure, while
composed of impermeable concrete, will not be impervious,as water will follow the cracks through the mass. To prevent
shrinkage cracks and those due to changes of temperature,the concrete is generally reinforced longitudinally, unless
special joints are made at intervals.
There are numerous compounds on the market which are
designed to be mixed with the cement in making the con-
crete. These compounds are claimed to make the concrete
impermeable. Such compounds are not necessary, and
should be used with caution.
. The following simple means are claimed to produce im-
(a) In mixing the concrete, use, in equal parts, "a five-
per-cent solution of alum and water and a seven-per-cent
solution of soap and water." (Hatt.)
(6) Baker states that an impervious mortar can be made
by the following formula: "One per cent, by weight, of
powdered alum is added to the dry cement and sand, and
one per cent of potash soap (ordinary soft soap is good) is
dissolved in the water used in mixing. The chemical action
set up makes an insoluble compound which practically fills
all pores, making an impervious concrete."
Tests of the Absorptive and Permeable Properties of
Portland Cement Mortars and Concretes. Following is a
summary of the conclusions drawn from a series of experi-
ments made on mortars and concretes given in Technologic
Papers of the Bureau of Standards, No. 3, Tests of the
Absorptive and Permeable Properties of Portland Cement
Mortars and Concretes, Together with Tests of Damp-proofing and Waterproofing Compounds and Materials, by
Rudolph J. Wig and P. H. Bates:
"Portland cement mortar and concrete can be made prac-
tically water-tight or impermeable (as defined below) to any
CONCRETE MASONRY 115
hydrostatic head up to 40 feet, without the use of any of the
integral' waterproofing materials; but, in order
to obtain such impermeable mortar or concrete, considerable
care should be exercised in selecting good materials as ag-
gregate and proportioning them in such a manner as to
obtain a dense mixture. The consistency of the mixture
should be wet enough so that it can be puddled, the particles
flowing into position without tamping. The mixture should
be well spaded against the forms when placed, so as to avoid
the formation of pockets on the surface.
"The addition of so-called 'integral' waterproofing com-
pounds will not compensate for lean mixtures, nor for poor
materials, nor for poor workmanship in the fabrication of
the concrete. Since, in practice, the inert integral com-
pounds (acting simply as void-filling material) are added in
such small quantities, they have very little or no effect on
the permeability of the concrete. If the same care be taken
in making the concrete impermeable without the addition
of waterproofing materials as is ordinarily taken when
waterproofing materials are added, an impermeable concrete
can be obtained.
"The terms '
should not be confused. A mortar or concrete is impermeable
(not necessarily damp-proof), as defined and used throughoutthis report, when it does not permit the passage or flow of
water through its pores or voids. The absorption of a
mortar or concrete is the property of drawing in or engross-
ing water into its pores or voids by capillary action or other-
wise. If the pores or voids between the grains or particles,
or in the individual grains, are sufficiently large and con-
nected from surface to surface of the wall, the concrete will
be permeable to water. If the pores or voids are very minute,but connected one with another, theoretically they may act
as capillary tubes, absorbing or drawing in and filling them-
selves with water; but the capillary forces will tend to hold
the water in the pores and will prevent the passage or flow
of water, even though one surface of the wall may be exposed
116 . MASONRY
to a considerable hydrostatic pressure. For all practical
purposes, a wall under such conditions would be considered
perfectly water-tight and impermeable, although it may be
highly absorptive. If these minute pores do act as capillary
tubes, and are never minute enough to prevent capillary
action, the moisture either as water or water vapor would,in time, penetrate entirely through and fill a concrete wall,
no matter what the thickness or composition. In such a
case, the capillary forces would not permit an actual flow
of water, but these forces may carry moisture, entirely filling
the wall, and, unless evaporation is retarded, the opposite
face of the wall would appear dry. In such a case, the con-
crete would be considered impermeable, but not damp-proof."The damp-proofing tests, as conducted, would indicate
that Portland cement mortars can be made not only im-
permeable but damp-proof as well, as defined above, with-
out the use of any damp-proofing or waterproofing com-
pound. However, these tests should be interpreted with
caution, as the evaporation may have been sufficient to care
for the slight amount of moisture coming through the test
pieces without indicating on the filter paper. Thus it cannot
be stated that if a material were used which was damp-proof
according to this test, if used as a basement wall, one surface
being constantly exposed to moisture and the other surface
in an inclosed room where there would be little or no circu-
lation of air, the interior surface would not appear damp,and the atmosphere become saturated with moisture. Thetests of coating materials as damp-proofing mediums can
be considered as only preliminary, but the results, considered
along with chemical discussion, throw some light on their
comparative merits. The mortar used in these tests, per-
haps, was too coarse and too absorptive for a fair test. The
purpose of the rough surface was to test the flowing qualities
of the coating, and it would seem that many of the failures
may be due to the poor or imperfect spreading and adhesive
quality. Several of the compounds deteriorated, and provedtheir unfitness for the purpose intended.
CONCRETE MASONRY 117
"Well-graded sands containing considerable graded fine
material are preferable for making impermeable concrete,
but if such is not to be had, fine material in the form of
hydrated lime, finely ground clay, or an additional quantity
of cement will be found of value." Where Portland cement mortar is used as a plaster coat,
if sufficient cement be used and the sand contains sufficient
fine material (or a fine material be added) and the mortar
be placed without joints and well troweled (care being taken
not to overtrowel, which may cause crazing), the coating
will be effective as an impermeable medium without the use
of any waterproofing compound."As a precaution, under certain conditions, it is un-
doubtedly desirable to use bituminous or similar coatings,
even on new work, as a protection where cracks may occur,
due to settling of foundation or expansion and contraction
caused by temperature changes. In large or exposed work,it is practically impossible to prevent some cracks, but where
cracks can be prevented no coating whatever is required to
make the structure impermeable."The permeability of Portland cement mortars and con-
cretes rapidly decreases with age.
"None of the integral compounds tested materially re-
duced the absorption of the mortars before they were dried
by heating at 212 F. Thus they would have little or no
practical value. But some of the so-called integral water-
proofing compounds did decrease the absorption obtained
after drying the mortars at 212 F., and the rate of absorption
was much slower in these cases. The addition of hydratedlime and clays seemed to have little or no effect on the
"The addition of any of the compounds tested to a mortar
in the quantities as used in these tests does not seriously
affect the compressive or tensile strength. The addition of
the inert void fillers to mortars, as used in these tests, upto 20 per cent of the volume of cement increases the com-
pressive strength." (Washington, D. C., Aug. 24, 1911.)
Surface Coating of Mortar. A coating of rich cement
mortar, made of one part Portland cement and one or two
parts of fine sand, from 0.25 to 1 inch thick, is applied
with a trowel to the concrete when it is still green. This
makes an impermeable medium, and is successful under still
water, but when exposed to the weather is liable to crack.
To be successful, plaster coats require very careful treat-
ment, and especially must the concrete to be plastered be
perfectly clean. Coatings applied with the cement-gun are
Surface Washes. A wash composed of alum, lye, cement,
and water has been successfully used to make concrete sur-
"Dissolve one pound of concentrated
lye and five pounds of alum in two gallons of water, care
being taken to have every particle dissolved. Heating to
near the boiling-point will quickly insure this without injury
to the mixture. This constitutes the stock mixture, and maybe used in any quantity. To one pint of stock, add ten
pounds of cement, thinning it with water until the mixture
spreads easily and well on the surface to be treated, with
a calcimine or whitewash brush, filling all the pores. The
mixture will be found to be satisfactory when it lathers
freely under the brush." This mixture should be applied
within three or four days after the concrete has been de-
The Sylvester process can be applied to concrete in the
same manner as explained for brick-work.
Waterproofing with Asphalt and Coal Tar. One of the
materials in general use for waterproofing concrete is asphalt,
which is used alone or in conjunction with burlap, paper,
felt, etc. This is supposed to form a barrier against water,
and to be sufficiently flexible not to break when small cracks
occur in the concrete. Coal tar is used in a similar
Hot asphalt will not adhere to the surface of cold concrete,
and, therefore, it must be heated with hot sand or some other
means, and then cleaned. Usually, the asphalt is cut with
CONCRETE MASONRY 119
naphtha and applied as a paint with a swab to the cleaned
The ordinary method of procedure in waterproofing with
asphalt and paper is, first, to paint the concrete surface with
hot asphalt, and then spread a layer of paper or felt, lapping
all joints. The layer of paper or felt is then thoroughly
painted with the hot asphalt, and another layer of paper or
felt spread. This process is continued until the requisite
number of thicknesses of paper and asphalt has been laid.
From two to six or seven layers are generally used, depending
upon the structure and the amount of water expected.
There are a number of special compounds and felts on the
market which are used very much in the manner outlined
Asphalt and coal tar are not permanent. The asphaltdeteriorates rapidly when exposed to illuminating gas.
Joining Old and New Concrete. In many cases it is
necessary to join new concrete with concrete which has been
deposited one or more days. As in the case of waterproofing,there is a large number of proprietary ^compounds which are
claimed to make more or less perfect bond between new andold concrete. The use of such compounds is not advisable
or necessary, as satisfactory results can be obtained bysimply roughening and cleaning the surface of the old con-
crete and then coating it with a rich Portland cement mortarbefore the new concrete is deposited. This applies to vertical
surfaces which are to receive a plaster coat applied by handor by the cement-gun and to horizontal surfaces upon whichconcrete is to be placed. Vertical joints extending from topto bottom of a wall or similar structure should be reinforced
with metal rods or dowels.
Effect of Alkali and Sea-water on Concrete. If concrete
is properly proportioned, carefully mixed, and deposited in
moulds, and allowed to harden before it comes in contact
with water containing alkali or sea-water, it will not be in-
jured by such waters. An impermeable concrete with asmooth surface is practically uninjured by either the salts
in alkali water or sea-water. Of course the aggregates should
be selected from materials which are inert to the action of
the salts in alkali water and sea-water.
Physical Properties of Concrete. The physical propertiesof concretes, necessarily, vary for concretes of different pro-
portions of cement and aggregates, and with the quality of
The crushing strength of good 1:3:6 concrete at the endof one month is about 2,000 pounds per square inch, and at
the end of six months about 2,600 pounds per square inch.
For 1:2:4 concrete, these values become 2,400 and 3,300
respectively. The safe compressive strength is taken at
about 400 pounds per square inch, and in some cases a com-
pressive strength of 650 pounds per square inch is assumed.
Young's modulus of elasticity for a compressive load be-
tween 100 and 600 pounds per square inch is, for 1 : 3 : 6
concrete one month old, about 2,400,000 pounds per square
inch, and for 1 : 2 : 4 concrete, 2,700,000 pounds per squareinch.
The weight of gravel and broken-stone concrete varies
from 145 to 155 pounds per cubic foot.
Fire-Resisting Property of Concrete. While there is con-
siderable difference of opinion concerning the ability of con-
crete to resist a hot fire successfully, its behavior in several
large conflagrations indicates that it is superior to any of
the natural building stones, and equal to if not superior to
terra-cotta and hollow tile. The exposed surfaces and corners
of concrete are injured by fire, but the injury apparently
does not extend to any great depth below the surfaces.
PART III. SPECIFICATIONS
RAILROAD MASONRY, BRICK CEMENT, ETC.
Railroad Masonry. The following abstracts (published
by permission) are taken from the Manual of the American
Railway Engineering Association. The classification of
masonry definitions and specifications were recommended
by a special committee on masonry, and adopted by the
The specifications apply particularly to bridge and retain-
ing-wall masonry, but they can be easily modified to applyto masonry in buildings
CLASSIFICATION OF MASONRY
Masonry, Bridge and Retaining Wall. Masonry of stone
or concrete designed to carry the end of a bridge span, or to
retain the abutting earth, or both.
Masonry, Arch. That portion of the masonry in the arch
ring only, or between the intrados and the extrados.
Masonry, Culvert. Flat-top masonry structure of stone
or concrete designed to sustain the fill above, and to permitof the free passage of water.
Masonry, Dry. Masonry in which stones are built upwithout the use of mortar.
Concrete. A compact mass of broken stone, gravel, or
other suitable material assembled together with cement
mortar and allowed to harden.
Reinforced Concrete. Concrete which has been reinforced
by means of metal in some form, so as to develop the com-
pressive strength of the concrete.
Rubble Concrete. Concrete in which rubble stone are
Brick, No. i. Hard-burned brick, absorption not exceed-
ing two per cent by weight.
Cement. A material of one of the three classes, Portland,
Natural, or Puzzolan, possessing the property of hardening
into a solid mass when mixed with water.
Portland Cement. This term shall be applied to the
finely pulverized product resulting from the calcination to
incipient fusion of an intimate mixture of properly propor-
tioned argillaceous and calcareous materials, and to which
no addition greater than three per cent has been made subse-
quent to calcination.
Natural Cement. This term shall be applied to the finely
pulverized product resulting from the calcination of an
argillaceous limestone at a temperature only sufficient to
drive off the carbonic acid gas.
Puzzolan Cement as Made in North America. An in-
timate mixture obtained by finely pulverizing together
granulated basic blast furnace slag and slacked lime.
COURSES AND BOND
Coursed. Laid with continuous bed joints.
Broken Coursed. Laid with parallel, but not continuous,
Uncoursed. Laid without regard to courses.
English Bond. That disposition of bricks in a structure
in which each course is composed entirely of headers or of
Flemish Bond. That disposition of bricks in a structure
in which the headers and stretchers alternate in each course,
the header being so placed that the outer end lies on the
middle of a stretcher in the course below.
Dressing. The finish given to the surface of stones or to
Smooth. Having surface the variations of which do not
exceed one-sixteenth inch from the pitch line.
Fine Pointed. Having irregular surface the variations of
which do not exceed one-quarter inch from the pitch line.
Rough Pointed. Having irregular surface the variations
of which do not exceed one-half inch from the pitch line.
Scabbled. Having irregular surface the variations of
which do not exceed three-quarters inch from the pitch line.
Rock-Faced. Presenting irregular projecting face, with-
out indications of tool mark.
Abutment. A supporting wall carrying the end of a bridge
or span and sustaining the pressure of the abutting earth.
The abutment of an arch is commonly called a bench wall
Arris. The external edge formed by two surfaces, whether
plain or curved, meeting each other.
Ashlar. A squared or cut block of stone with rectangular
Backing. That portion of a masonry wall or structure
built in the rear of the face. It must be attached to the
face and bonded with it. It is usually of a cheaper gradeof work than the face.
Batter. The slope or inclination of the face or back of a
wall from a vertical line.
Bed. The top and bottom of a stone. (See Course Bed,
Natural Bed, Foundation Bed.)
Bed Joint. A horizontal joint, or one perpendicular to the
line of pressure.
Bench Wall. The abutment from which an arch
Bond. The mechanical disposition of stone, brick, or other
building blocks by overlapping to break joints.
Build. A vertical joint.
Centering. A temporary support used in arch construc-
tion. (Also called centers.)
Clamp. An instrument for lifting stone so designed that
its grip on the surface of the stone is increased as the load
is applied. That portion engaging the stone is of wood
attached to a steel shoe, which in turn is hinged to the shank
of the clamp in such a manner as to, adjust itself to the
surface of the body lifted.
Coping. A top course of stone or concrete, generally
slightly projecting, to shelter the masonry from the weather,
or to distribute the pressure from exterior loading.
Course. Each separate layer of stone, concrete, or brick
masonry.Course Bed. Stone, brick, or other building material in
position, upon which other material is to be laid.
Cramps. Bars of iron having the ends turned at right
angles to the body of the bar which enter holes in the upper
side of adjacent stones.
Culvert. A small covered passage for water under a road-
way or embankment.
Dimension Stone. (1) A block of stone cut to specified
dimensions. (2) Large blocks of stone quarried to be cut
to specified dimensions.
Dowels. (a) Straight bars of iron which enter a hole in
the upper side of one stone and also a hole in the lower side
of the stone next above. (b) A two-piece steel instrument
used in lifting stone. The dowel engages the stone by means
of two holes drilled into the stone at an angle of about 45
pointing toward each other. The dowel is not keyed in
Draft. A line on the surface of a stone cut to the breadth
of the chisel.
Expansion Joint. A vertical joint or space to allow for
Extrados. The upper or convex surface of an arch.
Intrados. The inner or narrow concave surface of an
Face. The exposed surface in elevation.
Facing. In concrete: (1) A rich mortar placed on the
exposed surface to make a smooth finish. (2) Shovel facing
by working the mortar of concrete to the face.
Final Set. A stage of the process of setting marked bycertain hardness. (See Cement Specifications.)
Flush. (Adj.) Having the surface even or level with an
adjacent surface. (Verb) (I) To fill. (2) To bring to a level.
(3) To force water to the surface of mortar or concrete bycompacting or ramming.
Footing. A projecting bottom course.
Form. A temporary structure for giving concrete a de-
Foundation. (1) That portion of a structure, usuallybelow the surface of the ground, which distributes the
pressure upon its support. (2) Also applied to the natural
support itself; rock, clay, etc.
Foundation Bed. The surface on which a structure rests.
Grout. A mortar of liquid consistency which can be
easily poured.Header. A stone which has its greatest length at right
angles to the face of the wall, and which bonds the face
stones to the backing.
Initial Set. An early stage of the process of setting,
marked by certain hardness, (See Cement Specifications.)
Joint. The narrow space between adjacent stones, bricks,
or other building blocks, usually rilled with mortar.
Lagging. Strips used to carry and distribute the weightof an arch to the ribs or centering during its construction.
Lewis. A four-piece steel instrument used in lifting stone.
(The lewis engages the stone by means of a triangular-shapedhole into which it is keyed.)
Lock. Any special device or method of construction used
to secure a bond in the work.
Mortar. A mixture of fine aggregate, cement, or lime andwater used to bind together the materials of concrete, stone,
or brick in masonry, or to cover the surface of same.
Natural Bed. The surfaces of a stone parallel to its
Parapet. A wall or barrier on the edge of an elevated
structure for protection or ornament.
Paving. Regularly placed stone or brick forming a floor.
Pier. An intermediate support for arches or other
Pitch. (Verb) To square a stone.
Pitched. Having the arris clearly defined by a line be-
yond which the rock is cut away by the pitching chisel so as
to make approximately true edges.
Pointing. Filling joints or defects in the face of a masonrystructure.
Retaining Wall. A wall for sustaining the pressure of
earth or filling deposited behind it.
Voussoirs. The individual stones forming an arch. Theyare always of truncated wedge form.
Ring Stones. The end voussoirs of an arch.
Riprap. Rough stones of various sizes placed compactlyor irregularly to prevent scour by water.
Rubble. Field stone or rough stone as it comes from the
quarry. When it is of a large or massive size, it is termed
Rubbed. A fine finish made by rubbing with grit or
Set. (Noun) The change from a plastic to a solid or
Slope Wall. A wall to protect the slope of an embank-
ment or cut.
Soffit. The under side of a projection.
Spall. (Noun) A chip or small piece of stone broken
from a large block
Spandrel Wall. The wall at the end of an arch above
the springing line and extrados of the arch, and below the
coping or the string course.
Stretcher. A stone which has its greatest length parallel
to the face of the wall.
Wing Wall. An extension of an abutment wall to retain
the adjacent earth.
SPECIFICATIONS FOR STONE MASONRY
3. Stone shall be of the kinds designated, and shall be
hard and durable, of approved quality and shape, free from
seams or other imperfections. Unseasoned stone shall not
be used where liable to injury by frost.
4. Dressing shall be the best of the kind specified.
5. Beds and joints, or builds, shall be square with each
other, and dressed true and out of wind. Hollow beds shall
not be permitted.
6. Stone shall be dressed for laying on the natural bed.
In all cases, the bed shall not be less than the rise.
7. Marginal drafts shall be neat and accurate.
8. Pitching shall be done to true lines and exact batter.
9. Mortar shall be mixed in a suitable box, or in a machine
mixer, preferably of the batch type, and shall be kept free
from foreign matter. The size of the batch and the pro-
portions and the consistency shall be as directed by the
engineer. When mixed by hand, the sand and cement shall
be mixed dry, the requisite amount of water then added,and the mixing continued until the cement is uniformly dis-
tributed and the mass is uniform in color and homogeneous.10. The arrangement of courses and bond shall be as
indicated on the drawings, or as directed by the engineer.
Stone shall be laid to exact lines and levels to give the re-
quired bond and thickness of mortar in beds and joints.
11. Stone shall be cleansed and dampened before laying.
12. Stone shall be well bonded, laid on its natural bed,
and solidly settled into place in a full bed of mortar.
13. Stone shall not be dropped or slid over the wall, but
shall be placed without jarring stone already laid.
14. Heavy hammering shall not be allowed on the wall
after a course is laid.
15. Stone becoming loose after the mortar is set shall be
re-laid with fresh mortar.
16. Stone shall not be laid in freezing weather, unless
directed by the engineer. If laid, it shall be freed from ice,
snow, or frost by warming; and the sand and water used in
the mortar shall be heated.
17. With precaution, a brine may be substituted for the
heating of the mortar. The brine shall consist of one poundof salt to eighteen gallons of water, when the temperatureis 32 F. For every degree of temperature below 32 F., one
ounce of salt shall be added.
18. Before the mortar has set in beds and joints, it shall
be removed to a depth of not less than one inch. Pointing
shall not be done until the wall is complete and mortar set,
nor when frost is in the stone.
19. Mortar for pointing shall consist of equal parts of
sand, sieved to meet the requirements, and Portland cement.
In pointing, the joints shall be wet, and filled with mortar,
pounded in with a"set-in" or caulking tool, and finished
with a beading tool the width of the joint, used with a
BRIDGE AND RETAINING WALL MASONRY
20. The stone shall be large and well proportioned.
Courses shall not be less than 14 inches or more than 30
inches thick; thickness of courses to diminish regularly from
the bottom to the top.
21. Beds and joints, or builds, of face stone shall be fine-
pointed, so that the mortar layer should not be more than
one-half inch thick when the stone is laid.
22. Joints in face stone shall be full to the square for a
depth equal to at least one-half the height of the course,
but in no case less than 12 inches.
23. Exposed surfaces of the face stone shall be rock-faced,
and edges pitched to the true lines and exact batter; the
face shall not project more than three inches beyond the
24. Chisel drafts one and one-half inches wide shall be
cut at exterior corners.
25. Holes for stone hooks shall not be permitted to showin exposed surfaces. Stone shall be handled with clamps,
keys, lewis, or dowels.
26. Stretchers shall not be less than four feet long, andhave at least one and a quarter times as much bed as thick-
ness of course.
27. Headers shall not be less than four feet long, shall
occupy one-fifth of face of wall, shall not be less than 18
inches wide in face, and, where the course is more than
18 inches high, width of face shall not be less than height of
28. Headers shall hold in heart of wall the same size
shown in face, so arranged that a header in a superior course
shall not be laid over a joint, and a joint shall not occur overa header; the same disposition shall occur in back of wall.
29. Headers in face and back of wall shall interlock whenthickness of wall will admit.
30. When the wall is three feet thick or less, the face stone
shall pass entirely through. Backing shall not be permitted.31. (a) Backing shall be large, well-shaped stone, roughly
bedded and jointed; bed joints shall not exceed one inch.
At least one-half of the backing stone shall be of the samesize and character as the face stone and with parallel ends.
The vertical joints in back of wall shall not exceed twoinches. The interior vertical joints shall not exceed six
inches. Voids shall be thoroughly filled with concrete (or)
spalls, fully bedded in cement mortar. (6) Backing shall be
of concrete (or) headers and stretchers, as specified in para-
graphs 26 and 27, and heart of wall filled with concrete.
32. Where the wall will not admit of such arrangement,stone not less than four feet long shall be placed transverselyin heart of wall to bond the opposite sides.
33. Where stone is backed with two courses, neither course
shall be less than eight inches thick.
34. Bond of stone in face, back, and heart of wall shall
not be less than 12 inches. Backing shall be laid to break
joints with the face stone and with one another.
35. Coping stone shall be full size throughout, of dimen-
sions indicated on drawings.
36. Beds, joints, and top shall be fine-pointed.
37. Location of joints shall be determined by the positionof the bed plates, and be indicated on the drawings.
38. Where required, coping stone, stone in wings of abut-
ments, and stone on piers, shall be secured together with
iron cramps or dowels, to the position indicated on the
BRIDGE AND RETAINING WALL MASONRY
39. The stone shall be roughly squared, and laid in ir-
regular courses. Beds shall be parallel, roughly dressed, and
the stone laid horizontal to the wall. Face joints shall not
be more than one inch thick. Bottom stone shall be large,
selected flat stone.
40. The wall shall be compactly laid, having at least one-
fifth the surface of back and face headers arranged to inter-
lock, having all voids in the heart of the wall thoroughly
filled with concrete (or) suitable stones and spalls , fully bedded
in cement mortar.
41. Voussoirs shall be full size throughout and dressed
true to templet, and shall have bond not less than thickness
42. Joints of voussoirs and intrados shall be fine-pointed.
Mortar joints shall not exceed three-eighths of an inch.
43. Exposed surface of ring stone shall be smooth (or)
rock faced with a marginal draft.
44. Number of courses and depth of voussoirs shall be
indicated on the drawings.
45. Voussoirs shall be placed in the order indicated on
46. Backing shall consist of concrete (or) large stone, shapedto fit the arch, bonded to the spandrel, and laid in a full bed of
47. Where waterproofing is required, a thin coat of mortar
or grout shall be applied evenly for a finishing coat, uponwhich shall be placed a covering of approved waterproofingmaterial.
48. Centers shall not be struck until directed by the
49. Bench walls, piers, spandrels, parapets, wing walls,
and copings shall be built under specifications for Bridgeand Retaining Wall Masonry, Ashlar Work
50. Voussoirs shall be full size throughout, and shall have
bond not less than thickness of voussoirs.
51. Beds shall be roughly dressed to bring them to radial
52. Mortar joints shall not exceed one inch.
53. Exposed surfaces of the ring stone shall be rock-faced,
and edges pitched to true lines.
54. Voussoirs shall be placed in the order indicated on the
55. Backing shall consist of concrete (or) large stone, shapedto fit the arch, bonded to the spandrel, and laid in full bed of
56 and 57. (See 47 and 48.)
58. Bench walls, piers, spandrels, parapets, wing walls,
and copings shall be built under the specifications for Bridgeand Retaining Wall Masonry, Rubble Stone.
59. Culvert masonry shall be laid in cement mortar.
Character of stone and quality of work shall be the same
as specified for Bridge and Retaining Wall Masonry, Rubble
60. One-half the top stone of the side walls shall extend
entirely across the wall.
61. Covering stone shall be sound and strong, at least
12 inches thick, or as indicated on the drawings. They shall
be roughly dressed to make close joints with each other,
and lap their entire width at least 12 inches over the side
walls. They shall be doubled under high embankments, as
indicated on the drawings.
62. End walls shall be covered with suitable coping, as
indicated on the drawings.
63. Dry masonry shall include dry retaining walls and
64. Retaining walls and dry masonry shall include all
walls in which rubble stone laid without mortar is used for
retaining embankments or for similar purposes.
65. Flat stones at least twice as wide as thick shall be
used. Beds and joints shall be roughly dressed square to
each other and to face of stone.
66. Joints shall not exceed three-quarters of an inch.
67. Stone of different sizes shall be evenly distributed
over entire face of wall, generally keeping the larger stone
in lower part of wall.
68. The work shall be well bonded, and present a reason-
ably true and smooth surface, free from holes or projections.
69. Slope walls shall be built of such thickness and slope
as directed by the engineer. Stone shall not be used in this
construction which does not reach entirely through the wall.
Stone shall be placed at right angles to the slopes. The wall
shall be built simultaneously with the embankment which
it is to protect.
SPECIFICATIONS FOR PLAIN CONCRETE
1. The cement shall be Portland, and shall meet the
requirements of the standard specifications.
2. Fine aggregate shall consist of sand, crushed stone, or
gravel screenings, graded from fine to coarse, and passing
when dry a screen having one-quarter inch diameter holes;
it shall preferably be of hard siliceous material, clean, free
from dust, soft particles, vegetable loam or other deleterious
matter, and not more than six per cent shall pass a sieve
having 100 meshes per linear inch.
3. The fine aggregate shall be of such quality that mortar
composed of one part Portland cement and three parts fine
aggregate by weight when made into briquettes shall showa tensile strength at least equal to the strength of 1 : 3
mortar of the same consistency made with the same cement
and standard Ottawa sand.
4. Coarse aggregate shall consist of material such as
crushed stone or gravel which is retained on a screen having
one-quarter inch diameter holes and having gradations of
sizes from the smallest to the largest particles. Aggregates
containing dust, soft, or elongated particles shall not be
5. The water used in mixing concrete shall be free from
oil, acid, and injurious amounts of alkalies or vegetable
22. The unit of measure shall be the cubic foot. A bag
containing not less than 94 pounds of cement shall be
assumed as one cubic foot of cement. Fine and coarse
aggregates shall be measured separately as loosely thrown
into the measuring receptacle.
23. The fine and coarse aggregates shall be used in such
relative proportions as will insure maximum density.
25. For plain concrete, a proportion of 1 : 9 (unless other-
wise specified) shall be used; i.e., one part of cement to a
total of nine parts of fine and coarse aggregates measured
separately; for example, one part cement, three parts fine
aggregate, and six parts coarse aggregate.
27. The ingredients of concrete shall be thoroughly mixed
to the desired consistency, and the mixing shall continue
until the cement is uniformly distributed and the mass is
uniform in color and homogeneous.28. The various ingredients, including the water, shall be
measured separately, and the methods of measurement shall
be such as to secure the proper proportions at all times.
29. A machine mixer, preferably of the batch type, shall
be used, wherever the volume of the work will justify the
expense of installing the plant. The requirements demandedare that the product delivered shall be of the specified pro-
portions and consistency, and thoroughly mixed.
30. When it is necessary to mix by hand, the mixing shall
be on a water-tight platform of sufficient size to accommodatemen and materials for the progressive and rapid mixing of
at least two batches of concrete at the same time. Batches
shall not exceed one-half cubic yard each. The mixing shall
be done as follows: The fine aggregate shall be spread evenly
upon the platform, then the cement upon the fine aggregate,and these mixed thoroughly until of an even color. Thewater necessary to mix a thin mortar shall then be added,and the mortar spread again. The coarse aggregates, which,if dry, shall first be thoroughly wetted down, shall then be
added to the mortar. The mass shall then be turned with
shovels or hoes until thoroughly mixed and all aggregatecovered with mortar. Or, at the option of the engineer, the
coarse aggregate may be added before, instead of after,
adding the water.
31. The materials shall be mixed wet enough to producea concrete of such consistency that it will flow into the
forms and about the metal reinforcement, and which, onthe other hand, can be conveyed from the place of mixingto the forms without separation of the coarse aggregate fromthe mortar.
32. Re-tempering mortar or concrete, i.e., remixing with
water after it has partially set, will not be permitted.33. Concrete after the completion of the mixing shall be
handled rapidly to the place of final deposit, and under no
circumstances shall concrete be used that has partially set
before final placing.
34. The concrete shall be deposited in such a manner as
will prevent the separation of the ingredients and permitthe most thorough compacting. It shall be compacted byworking with a straight shovel or slicing tool kept movingup and down until all the ingredients have settled in their
proper place and the surplus water is forced to the surface.
In general, except in arch work, all concrete must be de-
posited in horizontal layers of uniform thickness throughout.35. In depositing concrete under water, special care shall
be exercised to prevent the cement from floating away and
to prevent the formation of laitance.
36. Before depositing concrete, the forms shall be thor-
oughly wetted (except in freezing weather) or oiled, and the
space to be occupied by the concrete cleared of debris.
37. Before placing new concrete on or against concrete
which has set, the surface of the latter shall be roughened,
thoroughly cleansed of foreign material and laitance,
drenched and slushed with a mortar consisting of one part
Portland cement and not more than two parts fine
38. The faces of concrete exposed to premature drying
shall be kept wet for a period of at least three days.
39. Concrete shall not be mixed or deposited at a freezing
temperature, unless special precautions, approved by the
engineer, are taken to avoid the use of materials covered
with ice crystals or containing frost and to provide means
to prevent the concrete from freezing.
40. Where the concrete is to be deposited in massive work,
clean, large stones, evenly distributed, thoroughly bedded,
and entirely surrounded by concrete, may be used, at the
option of the engineer.
41. Forms shall be substantial and unyielding, and built
so that the concrete shall conform to the designed dimen-
sions and contours, and so constructed as to prevent the
leakage of mortar.
42. The forms shall not be removed until authorized bythe engineer.
43. For all important work, lumber used for face work
shall be dressed to a uniform thickness and width, shall be
sound and free from loose knots, and secured to the stud-
ding or uprights in horizontal lines.
44. For backing and other rough work, undressed lumber
may be used.
45. Where corners of masonry and other projections liable
to injury occur, suitable mouldings shall be placed in the
angles of the forms to round or bevel them off.
46. Lumber once used in forms shall be cleaned before
being used again.
49. Concrete structures, wherever possible, shall be cast
at one operation, but when this is not possible, the resulting
joint shall be formed where it will least impair the strength
and appearance of the structure.
50. Girders and slabs shall not be constructed over freshly
formed walls or columns without permitting a period of at
least four hours to elapse to provide for settlement or shrink-
age in the supports. Before resuming work, the tops of such
walls or columns shall be cleaned of foreign matter and
51. A triangular-shaped groove shall be formed at the
surface of the concrete at vertical joints in walls and abut-
52. Except where a special surface finish is required, a
spade or special tool shall always be worked between the
concrete and the form, to force back the coarse aggregatesand produce a mortar face.
53. Top surfaces shall generally be "struck
" with a
straight-edge or"floated" after the coarse aggregates have
been forced below the surface.
54. When a"sidewalk finish" is called for on the plans,
it shall be made by spreading a layer of 1 : 2 mortar at
least three-quarters of an inch thick, troweling the same to
a smooth surface. This finishing coat shall be put on before
the concrete has taken its initial set.
Monolith of Concrete. A single mass of concrete madewithout joints by a continuous operation of construction.
Monolithic Concrete Construction. Monolithic concrete
construction is the building of a single mass of concrete
without joints by a continuous operation.
Principles of Practice
These conclusions are based upon the supposition that the
structure is well designed, and that the foundation is good.1. Monolithic concrete construction may be used without
danger of cracking for abutments of any length that the
working conditions will permit, provided the length does
not exceed about three times the height.
2. Where abutments with wing walls are not of mono-lithic construction, joints should be provided at the inter-
sections of the wing walls and the body of the abutments.
3. Reinforced concrete abutments may be built in units
of any length that economic conditions will permit.4. Monolithic concrete construction may be used for
arches where the conditions will permit, otherwise the arch
ring should be constructed with radial joints.
PROPOSED STANDARD SPECIFICATIONS FORBUILDING BRICK*
Sampling. For the purpose of tests, brick shall be selected
to represent the commercial product by an experienced
*Proceedings of American Society for Testing Materials, Vol. XIII, 1913,
person agreed upon by the parties to the contract. All
brick shall be carefully examined and their condition noted
before being subjected to any kind of test.
For the purpose of the tests, ten bricks will be required,
which shall be thoroughly dried to constant weight in a
suitable oven at a temperature of from 225 F. (107 C.) to
250 F. (121 C.).
Compression Test. Compression tests shall be made on
at least five half-bricks, each taken from a different brick.
The half-brick shall be prepared either by sawing or bybreaking upon a yielding bed with a sharp mason's chisel,
which shall be the full width of the brick. To secure a uni-
form bearing in the testing machine, they shall be bedded
in a thin coat of plaster of Paris, spread upon a plate glass
surface coated with a thin layer of oil. The brick shall be
pressed firmly upon the surface, making the layer as thin
as possible, and remain undisturbed until set. Before apply-
ing the plaster of Paris, the bearing surface of the brick shall
receive a coat of shellac.
Recessed or panel brick should be brought to a full bearing
surface by filling the depression with neat Portland cement
mortar, which shall stand at least 24 hours before the plaster
of Paris is applied.
The machine used for the compression test shall be
equipped with a spherical bearing block kept thoroughlylubricated to insure accurate adjustment, and the adjust-
ment should be made by hand under a small initial load.
During the test, the beam of the testing machine shall be
kept constantly in a floating position. The breaking load
shall be divided by the area in compression and the results
reported in pounds per square inch.
Absorption. At least five dry bricks shall be weighed and
completely submerged in water at a temperature between
60 and 80 F., the water heated to boiling within one hour,boiled continuously for four hours, then allowed to cool in
the water to temperature between 60 and 80 F.
They should then be removed, the surface water wiped off
with a cloth and the brick quickly weighed. The percentageof absorption shall be computed on the dry weight.
Class A. Vitrified Brick
Average compressive strength not less than 5,000 pounds
per square inch.
Minimum compressive strength, of any specimen in test,
not less than 4,500 pounds per square inch.
Average absorption, not more than five per cent.
Class B. Hard-Burned Brick
Average compressive strength not less than 3,500 pounds
per square inch.
Minimum compressive strength, of any specimen in the
test, not less than 3,000 pounds per square inch.
Average absorption not more than 12 per cent.
If subjected to the freezing test, they shall not show
cracking or serious spalling in any of the bricks tested, or
serious disintegration of the material.
Class C. Common Brick, First
Average compressive strength not less than 2,000 pounds
per square inch.
Minimum compressive strength of any specimen in the
test, not less than 1,800 pounds per square inch.
Average absorption not more than 18 per cent.
(Freezing test same as for Class B.)
Class D. Common Brick, Second
(These bricks to be used only for backing-up and for
interior walls involving small loads.)
Average compressive strength not less than 1,500 pounds
per square inch.
Minimum compressive strength of any specimen in the
test not less than 1,200 pounds per square inch.
Any brick other than clay brick may be included in
Classes A, B, and C, provided they meet the specified re-
quirements; and when the freezing test is required, it shall
not show cracking or serious spalling in any of the bricks
tested, or serious disintegration of material.
PROPOSED STANDARD SPECIFICATIONSFOR LIME*
1. Lime is a product resulting from the calcination, at
a temperature below the cintering point, of a material con-
taining carbonates of calcium or calcium and magnesium,which may be or has been converted to a paste or a dryflocculent powder, by slaking.
2. Limes may be divided into two commercial forms:
(a) Quicklime. A product coming from the kiln, without
subsequent treatment other than sorting, crushing, or pul-
verization, which slakes on the addition of water. Quick-
lime may be shipped either as lump lime or pulverized lime.
Lump lime shall be kiln size. Pulverized lime is lump lime
reduced in size by mechanical means.
(6) Hydrate. A dry flocculent powder resulting from the
hydration of quicklime.
3. (a) Quicklimes are divided into two grades:
Selected. A. well-burned lime, picked free from ashes, core,
clinker, or other foreign material.
Run-of-kiln. A well-burned lime without selection.
(6) Hydrates are divided into two classes.
Building and Chemical. A lime hydrated to definite
*Proceedings of American Society for Testing Materials, Vol. XIII, 1913,
chemical proportions, and reduced to a fineness suitable
for building purposes.
Agricultural. . . . .
8. (a) Selected quicklime shall contain not under 90 percent of calcium and magnesium oxides, and not over three
per cent of carbon dioxide. (6) Run-of-kiln quicklime shall
contain not under 85 per cent of calcium and magnesiumoxides, and not over five per cent of carbon dioxide.
9. Building and chemical hydrates shall contain not over
five per cent of carbon dioxide, and not under one per cent
of water in excess of that required to hydrate fully the cal-
cium oxide present.
PHYSICAL PROPERTIES AND TESTS
11. An average five-pound sample of selected or run-of-
kiln quicklime shall be put in a box and slaked with sufficient
water to produce a lime putty, which shall be allowed to
stand 24 hours, then washed through a standard 10-mesh
sieve. Not over three per cent of the weight of selected
quicklime, nor over five per cent of the weight of run-of-kiln
quicklime, shall be retained on the sieve. The sample taken
for this test shall not be crushed finer than will pass a one-inch
ring, either before being sent to the laboratory or at the
(B) Hydrated Lime
12. (a) Building and chemical hydrates shall leave byweight a residue of not over five per cent on a standard
PACKING AND MARKING
(A) Lump Lime
13. When not shipped in bulk, lump lime shall be packedin barrels, which may weigh either 200 pounds gross and
contain approximately 185 pounds of lime, or 300 pounds
gross and contain approximately 280 pounds of lime.
14. The name of the manufacturer, grade, and gross weightshall be legibly marked on each barrel. Marking shall be
blue for selected and red for run-of-kiln quicklime.
(B) Pulverized Lime
15. Pulverized lime shall be packed either in cloth bags
containing 167 pounds, or in paper sacks containing 80
(C) Hydrated Lime
17. Hydrated lime may be packed either in cloth bags
containing 100 pounds, or in paper sacks containing 40
A SPECIFICATION FOR SAND*
The material shall be of such fineness that all shall passa No. 4 sieve.
The material shall contain at least 95 per cent of silica.
Before acceptance of the sand, the contractor shall forward
to the engineer an average sample, taken from the proposedsource of supply, which sample shall be subject to analysisand comparative physical tests with standard Ottawa sand.
*Proceedings of American Society for Testing Materials, Vol. X, 1910,
Requirement 1. The sand under examination, when
tested, with a normal Portland cement as mortar in the
proportion of one part cement to three parts sand, accordingto standard methods, shall develop at least 75 per cent of
the strength developed in similarly proportional mortar of
the same cement and Ottawa sand. But in no case shall
such sample mortar under investigation, in a 1 : 3 mixture
briquette, when tested in tension, fail at less than 150 poundsat 7 days or 200 pounds at 28 days.
Requirement 2. The sand under examination, whentested as mortar in the proportion of one part cement to
three parts sand, gauged by hand with 50 per cent excess
of the normal quantity of water, shall develop at least 50
per cent of its strength at identical periods, when normally
gauged. But in no case shall such sample mortar under
investigation, in a 1 : 3 mixture briquette, 50 per cent excess
gauge, when tested in tension, fail at less than 100 poundsat 7 days or 150 pounds at 28 days.
Requirement 3. After complete tests have been madeto determine the character of the representative sample,
each carload of sand to be used shall be subjected to the
above-described analysis and tests, and shall develop at
seven days, under similar methods of testing and gauging,
at least 80 per cent of the strength of the original sand
sample shown by the preliminary tests under which the sand
may have been accepted.
STANDARD SPECIFICATIONS FOR CEMENT*
ADOPTED AUGUST 16, 1909
1. These remarks have been prepared with a view of
pointing out the pertinent features of the various require-
ments and the precautions to be observed in the interpreta-
tion of the results of the tests.
* Year Book, 1914, American Society for Testing Materials.
2. The Committee would suggest that the acceptance or
rejection under these specifications be based on tests made
by an experienced person having the proper means for
making the tests.
3. Specific gravity is useful in detecting adulteration.
The results of tests of specific gravity are not necessarily
conclusive as an indication of the quality of a cement, but
when in combination with the results of other tests mayafford valuable indications.
4. The sieves should be kept thoroughly dry.
Time of Setting
5. Great care should be exercised to maintain the test
pieces under as uniform conditions as possible. A sudden
change or wide range of temperature in the room in which
the tests are made, a very dry or humid atmosphere, and
other irregularities vitally affect the rate of setting.
Constancy of Volume
6. The tests for constancy of volume are divided into two
classes, the first normal, the second accelerated. The latter
should be regarded as a precautionary test only, and not
infallible. So many conditions enter into the making and
interpreting of it that it should be used with extreme care.
7. In making the pats, the greatest care should be exer-
cised to avoid initial strains due to moulding or to too rapid
drying-out during the first 24 hours. The pats should be
preserved under the most uniform conditions possible, and
rapid changes of temperature should be avoided.
8. The failure to meet the requirements of the accelerated
tests need not be sufficient cause for rejection. The cement
may, however, be held for 28 days, and a re-test made at
the end of that period, using a new sample. Failure to meetthe requirements at this time should be considered sufficient
cause for rejection, although in the present state of our
knowledge it cannot be said that such failure necessarilyindicates unsoundness, nor can the cement be considered
entirely satisfactory simply because it passes the tests.
1. All cement shall be inspected.
2. Cement may be inspected either at the place of manu-facture or on the work.
3. In order to allow ample time for inspecting and test-
ing, the cement should be stored in a suitable weather-tight
building having the floor properly blocked or raised from
the ground.4. The cement shall be stored in such a manner as to per-
mit easy access for proper inspection and identification of
each shipment.5. Every facility shall be provided by the contractor, and
a period of at least 12 days allowed for the inspection and
6. Cement shall be delivered in suitable packages with
the brand and name of manufacturer plainly marked thereon.
7. A bag of cement shall contain 94 pounds of cement net.
Each barrel of Portland cement shall contain four bags, and
each barrel of natural cement shall contain three bags of the
above net weight.
8. Cement failing to meet the 7-day requirements maybe held awaiting the results of the 28-day tests before
9. All tests shall be made in accordance with the methods
proposed by the Committee on Uniform Tests of Cement
of the American Society of Civil Engineers, presented to
the Society January 21, 1903, and amended January 20,
1904, and January 15, 1908, with all subsequent amendmentsthereto.
10. The acceptance or rejection shall be based on the
11. Definition. This term shall be applied to the finely
pulverized product resulting from the calcination of an ar-
gillaceous limestone at a temperature only sufficient to drive
off the carbonic acid gas.
12. It shall leave by weight a residue of not more than
10 per cent on the No. 100 and 30 per cent on the No. 200
Time of Setting
13. It shall not develop initial set in less than 10 minutes;and shall not develop hard set in less than 30 minutes, or in
more than 3 hours.
14. The minimum requirements for tensile strength for
briquettes one square inch in cross section shall be as follows,
and the cement shall show no retrogression in strength within
the periods specified:
Age StrengthNEAT CEMENT
24 hours in moist air 75 Ibs.
7 days (1 day in moist air, 6 days in water) 150 "
28 days (1 day in moist air, 27 days in water) 250 "
ONE PART CEMENT, THREE PARTS STANDARD OTTAWA SAND7 days (1 day in moist air, 6 days in water) 50 "
28 days (1 day in moist air, 27 days in water) 125 "
Constancy of Volume
15. Pats of neat cement about three inches in diameter,one-half inch thick at center, tapering to a thin edge, shall
be kept in moist air for a period of 24 hours.
(a) A pat is then kept in air at normal temperature.
(6) Another is kept in water maintained as near 70 F. as
16. These pats are observed at intervals for at least 28
days, and, to pass the tests satisfactorily, shall remain firm
and hard and show no signs of distortion, checking, crack-
ing, or disintegrating.
17. Definition. This term is applied to the finely pul-
verized product resulting from the calcination to incipient
fusion of an intimate mixture of properly proportioned ar-
gillaceous and calcareous materials, and to which no addition
greater than three per cent has been made subsequent to
18. The specific gravity of cement shall not be less than
3.10. Should the test of cement as received fall below this
requirement, a second test may be made upon a sample
ignited at a low red heat. The loss in weight of the ignited
cement shall not exceed four per cent.
19. It shall leave by weight a residue of not more than
8 per cent on the No. 100 and not more than 25 per cent
on the No. 200 sieve.
Time of Setting
20. It shall not develop initial set in less than 30 minutes;
and must develop hard set in not less than one hour, nor
more than ten hours.
21. The minimum requirements for tensile strength for
briquettes one square inch in cross-section shall be as follows,
and the cement shall show no retrogression in strength within
the periods specified :
Age StrengthNEAT CEMENT
24 hours in moist air 175 Ibs.
7 days (1 day in moist air, 6 days in water) 500 '
28 days (1 day in moist air, 27 days in water) 600 "
ONE PART CEMENT, THREE PARTS STANDARD OTTAWA SAND
7 days (1 day in moist air, 6 days in water) 200 "
28 days (1 day in moist air, 27 days in water) 275 '
Constancy of Volume
22. Pats of neat cement about three inches in diameter,
one-half inch thick at the center, and tapering to a thin edge,
shall be kept in moist air for a period of 24 hours.
(a) A pat is then kept in air at normal temperature and
observed at intervals for at least 28 days.
(6) Another pat is kept in water maintained as near
70 F. as practicable, and observed at intervals for at least
(c) A third pat is exposed in any convenient way in an
atmosphere of steam, above boiling water, in a loosely closed
vessel for five hours.
23. These pats, to pass the requirements satisfactorily,
shall remain firm and hard, and show no signs of distortion,
checking, cracking, or disintegrating.
Sulphuric Acid and Magnesia
24. The cement shall not contain more than 1.75 percent of anhydrous sulphuric acid (S03) nor more than 4 percent of magnesia (MgO).
Nomenclature of Building Stones and Stone Masonry. Committee Report,T. A. S. C. E., Vol. VI, 1877.
Dimension Stone Quarrying: The Blasting Process. T. A. S. C. E., Vol.
Notes upon Testing Building Stones, with Bibliography. T. A. S. C. E.,
Vol. XXXII, 1894.
Relative Effects of Frost and Sulphate of Soda Efflorescence Tests on
Building Stones. T. A. S. C. E., Vol. XXXIII, 1895.
The Strength of Stone as Affected by Different Methods of Quarrying.E. N., Nov. 1, 1906.
The Characteristics of Good Building Stones. Ores and Metals, March 20,
The Two Carraras. Description of Quarries in Italy and Vermont, U. S. A.
Architectural Record, May, 1907.
Marbles: Their Ancient Application. The Modern Aspect of Marble-Workin Architecture. Journal, Royal Institute of British Architects, Jan. 26, 1907.
Sand Lime Brick Manufacture and Use. Municipal Engineering, Jan., 1907.
Sand Lime Brick, Historical. Scientific American Supplement, May 25, 1907.
Standard Specifications for Paving and Building Brick. Report of Com-
mittee, P. A. S. T. M., Vols. IX, X, and XIII, 1909, 1910, and 1913.
Tests of Brick Columns and Terra-Cotta Block Columns. University of
Illinois, Bulletin No. 27, Sept., 1908.
Working Loads on Brick-Work. Builder, March 14, 1908.
Strength of Brick and Brick Piers. E. R., Feb. 23, 1907.
Tests and Theories in Their Relation to Specifications for Bricks. Proceed-
ings of Engineers' Society of Western Pennsylvania, Nov., 1906.
Modern Methods of Brick Making. Journal of Society of Arts, Aug. 12,
Story of the Brick. Scientific American, April 6, 1907.
Brick Manufacture and Brick Pavements. T. A. S. C. E., Vols. XXVI(1892), XXIX, and XXX.Terra Cotta: Its Character and Construction. Brick Builder, Oct., 1909.
Architectural Terra-Cotta Construction. American Architect, Nov. 15, 1911.
Proposed Specifications for Hollow Clay Tile Building Blocks. E. N.,
Feb. 8, 1912.
Manufacture of Plaster of Paris. Engineering and Mining Journal, Dec. 8,
Manufacture of Lime. Technological Papers of the Bureau of Standards,
U. S. A., No. 12.
* E. N. refers to Engineering News. E. R. refers to Engineering Record. E. C. refers to
Engineering-Contracting. T. A. S. C. E. refers to Transactions of American Society of Engi-
neers. P. A. S. T. M. refers to Proceedings of American Society for Testing Materials.
P. A. R. E. A. refers to Proceedings of the American Railway Engineers' Association.
Standard Sand for Cement Work. E. R., July 20, 1907.
Sands: Their Relation to Mortar and Concrete. Cement Age, July, 1908.
A Sand Specification and Its Specific Application. P. A. S. T. M., Vol. X,1910.
A Proposed Study of Concrete Sands. E. N., May 30, 1912.
Testing Sand for Use in Concrete and Cement Mortar. Cement and En-
gineering News, Sept., 1912.; E. R., April 27, 1912.
Sand and Gravel Washing Plants. Cement and Engineering News, July,
A Portable Sand and Gravel Washer for Contractors' Use. E. C., June 17,
Prevention of Freezing in Concrete by Calcium Chloride. E. R., April 20,
Winter Construction of a Reinforced Concrete Building. E. N., Sept. 24,
The Concrete Block and Its Advance to the Position of a First-Class Build-
ing Material. Journal Association Engineering Societies, March, 1907.
Standard Rules and Regulations Governing Concrete Hollow Blocks
Adopted by National Association of Cement Users. E. R., March 7, 1908;
Cement Age, Feb., 1908.
Proportioning Gravel Concrete. Cement and Engineering News, Aug., 1912.
Effect of Oil on Cement Mortar. E. N., July 4, 1907.
Simple Tests of Portland Cement. E. C:, July 17, 1907; Cement Age, Aug.,1907.
Standard Specifications for Cement and Methods for Testing Cement.
Year Book, American Society for Testing Materials.
Efficiency of Cement Joints in Joining Old Concrete to New. E. N., Dec. 12,
Strength of Concrete Joints. Results of Tests. Proceedings of Engineers'
Society of Western Pennsylvania, Dec., 1908.
Tests on Bonding New Concrete to Old. E. N., Aug. 13, 1908.
The Bonding of New and Old Concrete. T. A. S. C. E., Vol. LXIV, 1909.
Methods of Patching and Repairing Plain and Reinforced Concrete.
P. A. R. E. A., Vol. XIII, 1913.
Some Representative Concrete Mixing Plants with Records of OperatingCosts. E. C., April 10, 1907.
Proportions of Concrete and Methods of Mixing. E. R., Feb. 15, 1908.
Pneumatic Rammers for Concrete. E. R., May 2, 1914.
Lining Rondout Pressure Tunnel, New York. (Compressed Air Method.)E. R., Dec. 30, 1911, Sept. 17, 1910; E. N., June 1, 1911.
Grouting Big Savage Tunnel, Using Air. E. R., Dec. 23, 1911.
Olive Bridge Dam. (Grout and Compressed Air) . E. R., April 8, 1911.
Grouting Arches, Hamburg, Germany. (Air Method.) E. R., Sept. 3, 1910.
French Methods and Machines. (Air Methods.) E. R., Oct. 30, 1909.
Grouting a Water-Bearing Rock Seam on Catskill Aqueduct. (Air Method.)E. N., Feb. 8, 1912.
Mixing and Conveying Concrete by Compressed Air. E. N., Aug. 10, 1911.
Lining and Grouting a French Railway Tunnel in Water-Bearing Material.
E. N., Nov. 25, 1909.
Pneumatic Concreting, Stockton Street Tunnel. E. R., July 4, 1914.
Use of Gunite in Protection of Face of Levee. E. N., Oct. 8, 1914.
A Compressed Air Concrete Mixer and Conveyer. E. N., Aug. 8, 1912.
Mixing and Distributing Concrete by Compressed Air. Railway AgeGazette, March 18, 1914.
A Concrete Tunnel-Lining Car with Pneumatic Mixer and Placer. E. N.,
March 26, 1914.
Pneumatic Placer of Concrete. Internal Wear on Pipe Lines and Methodsof Efficient Air Propulsion. E. R., May 23, 1914.
Cement for Sea-Water Construction. Cement Age, Jan., 1907.
Action of Sea-Water on Mortar. Cement Age, March, 1907.
The Action of Sea-Water on Concrete. Railway Age Gazette, Nov. 8, 1907.
The Effect of Alkali Soils on Concrete. E. N., July 23, 1908.
The Effect of Alkali on Portland Cement. E. R., July 25, 1908.
Destruction of Cement Mortar and Concrete by Alkali at Great Falls,
Montana. E. C., June 24, 1908.
Effect of Alkali on Concrete. T. A. S. C. E., Vols. LXV, LXVI, LXVII,and LXVIII.
The Effect of Sea-Water, Alkali Water, and Sewage on Portland Cement,and Methods Used for Counteracting Same. E. C., July 20, 1910.
What Are the Facts Respecting the Disintegration of Concrete by Sea-
Water, Alkali Sewage, etc. E. C., June, 1910.
Concrete Subjected to the Action of Water Containing Alkalies. P. A. R.
E. A., Vol. XIV, 1914.
Action of Sea-Water on Concrete. Results of Six-Year Tests of Twenty-three Moulded Piles of Various Mixtures, Submerged in Boston Harbor, and
Withdrawn Periodically for Examination. E. R., March 21, 1914; E. C.,
May 6, 1914.
Action of the Salts in Alkali Water and Sea Water on Cements. Technologic
Papers of the Bureau of Standards, U. S. A., No. 12.
Tests on the Permeability of Concrete. Bulletin of the University of
Wisconsin, Vol. VI, No. 1.
Permeability of Concrete Under High-Water Pressures. E. N., June 26,
Impervious Concrete: An Informal Discussion. T. A. S. C. E., Vol. LI,
Notes on Concrete Construction in Government Fortifications, with Water-
proofing Data. E. N., April 2, 1903.
The Permeability of Concrete and Methods of Waterproofing. E. N.,
Sept. 26, 1907.
Permeability Tests of Concrete with the Addition of Hydrated Lime.
E. R., June 27, 1908.
Investigation of Impermeable Concrete by the Laboratory of the Board
of Water Supply, New York City. E. C., Feb. 26, 1908.
Tests of Alum and Soap Waterproofing. E. R., Oct. 9, 1909.
Making Concrete Waterproof: Alum and Soap Mixture. Tecknograph,
Oil-Mixed Concrete as a Waterproofing Material. E. N., Dec. 15, 1910.
Tests on the Permeability of Concrete. Commercial Compounds. Wis-
consin Engineer, Feb., 1910.
Tests of the Absorptive and Permeable Properties of Portland Cement
Mortars and Concretes, and Waterproofing Compounds and Methods. Tech-
nological Papers of the Bureau of Standards, U. S. A., No. 3, Aug. 22, 1911.
Waterproofing Concrete Structures on the C. B. & Q. Track Elevation,
Chicago. Railway Age Gazette, Feb. 16, 1912.
Waterproofing Materials. Committee Report. P. A. S. T. M., Vols. IX, X,and XIII.
Waterproofing of Masonry. P. A. R. E. A., Vols. XI, XII, XIII, and XIV.
Bibliography in Vol. XII, pp. 564-578.
Manufacture, Test, and Use of Waterproofing Fabric. E. N., Sept. 24,
Methods of Depositing Concrete Under Water. Committee Report,
P. A. R. E. A., Vol. XIII.
Deep-Water Concreting Through a Tremie. E. R., Aug. 15, 1914.
Cement Surfaces (Pamphlet). Universal Portland Cement Company.Concrete Surface Finish. The Concrete Review, Vol. IV, No. 1.
The Method of Finishing the Concrete Surfaces of Philadelphia Bridges.
E. N., Feb. 4, 1904.
Concrete Surface: Various Methods of Finishing. Cement, Jan., 1907.
Painting Cement Surfaces. Municipal Engineering, Oct., 1908.
Specifications for Scrubbed Concrete Surface. E. N., Dec. 22, 1910.
Exterior Treatment of Concrete Surfaces. Committee Report to National
Association of Cement Users. E. N., Sept. 15, 1910.
Ornamental Treatment of Concrete Surfaces. American Architect, Jan. 24,
BOOKS FOR REFERENCEMarble and Marble Working. A Handbook for Architects, Sculptors, etc.
By W. G. Renwick. 226 pp.
Building Stones and Clays. Their Origin, Character, and Examination. ByEdwin C. Eckel. 264 pp.
Building Stones. Stone Formation, Quarrying, and Blasting, etc. ByPaul N. Hasluck. 96 pp.
Building Stones and Clay Products. A Handbook for Architects. ByHeinrich Ries. 415 pp.
Stones for Building and Decoration. By George P. Merrill. 557 pp.
Report on the Compressive Strength, Specific Gravity, and Ratio of Ab-
sorption of Building Stones. By Q. A. Gilmore.
Modern Brick-Making. By Alfred B. Searle. 441 pp.Vitrified Paving Brick. A Review of the Practice in Manufacture and
Testing and Uses of Vitrified Paving Brick. By H. A. Wheeler. 121 pp.
Bricklaying System. By Frank B. Gilbreth. 321 pp.
Practical Brick-work. By Paul N. Hasluck. 160 pp.Practical Bricklaying Self-Taught. Especially Designed for Home Study.
By Fred. T. Hodgson. 281 pp.
Twentieth-Century Bricklayer's and Mason's Assistant. By Fred. T.
Hodgson. 311 pp.
Bricklaying. Illustrated by over 200 engravings. By Owen B. Maginnis.
Bricklaying and Brick Cutting. By H. W. Richards. 139 pp.
Clays: Their Occurrence, Properties, and Uses, etc. By Heinrich Ries.
History of the Clay-Working Industry in the United States. By Heinrich
Ries and Henry Leighton. 270 pp.
Practical Cement Testing. By W. Purves Taylor. 320 pp.
Experimental Research Upon the Construction of Hydraulic Mortar. ByH. Le Chatelier, translated by J. L. Mack. 128 pp.
A Practical Treatise on Limes, Hydraulic Cements, and Mortars. By Q. A.
Mortars, Plasters, Stuccos, Artificial Marbles, etc. By Fred. T. Hodgson.520 pp.
Building Mechanic's Ready Reference-Book. Cement workers and plasterers'
edition. By H. G. Richey. 458 pp.
Hydraulic Cement. Its Properties, Testing, and Use. By Frederick P.
Spalding. 300 pp.
Portland Cement. Its Manufacture, etc. By D. B. Butler. 458 pp.
Cements, Limes, and Plasters: Their Materials,Manufacture, and Properties.
By Edwin C. Eckel. 712 pp.
Portland Cement. Its Composition, Raw Materials, Manufacture, and
Properties. By Richard K. Meade. 512 pp.
Calcareous Cements: Their Nature, Manufacture, and Uses, etc. ByGilbert R. Redgrave. 310 pp.
Modern Manufacture of Portland Cement. By Percy C. H. West. 262 pp.
Manual of Cement Testing, for the Use of Engineers, Chemists, etc. ByWm. A. Richards and Henry B. North. 137 pp.
Popular Handbook for Cement and Concrete Users. By Myron H. Lewis
and Albert H. Chandler. 430 pp.
Treatise on the Inspection of Concrete Construction. By Jerome Cochran.
Concrete System. By Frank B. Gilbreth. 182 pp.
Concrete Construction, Methods, and Cost. By Halbert P. Gillette and
Charles H. Hill. 690pp.Practical Concrete Block Making. By Charles Palliser. 74 pp.
Cement and How to Use It. By William A. Radford. 369 pp.
Cement Houses and How to Build Them. By William A. Radford. 171 pp.
Concrete and Reinforced Concrete Construction. By Homer A. Reid.
Concrete Block Manufacture, Processes, and Machines. By Harmon H.
Rice. 152 pp.
Cement and Concrete. By Louis T. Sabin. 572 pp.
Concrete Costs. By F. W. Taylor and Sanford E. Thompson. 700 pp.
Treatise on Concrete, Plain and Reinforced. By F. W. Taylor and Sanford
E. Thompson. 807 pp.
Concrete from Sand Moulds. By A. A. Houghton. 145 pp.
Ornamental Concrete Without Moulds. By A. A. Houghton. 132 pp.
Concrete Floors and Sidewalks. By A. A. Houghton. 63 pp.
Modern Cement Sidewalk Construction. By Charles Pallister. 64 pp.
Concrete Blocks. Their Manufacture and Use in Building Construction.
By H. H. Rice and Wm. M. Torrance. 125 pp.
Concrete. Its Use in Building from Foundation to Finish. By T. Potter.
Modern Methods of Waterproofing. By Myron H. Lewis. 44 pp.
Prevention of Dampness in Buildings. (Translated from second edition,
revised.) By A. W. Keim. 115 pp.
Treatise on Masonry Construction. By Ira O. Baker. 745 pp.
Practical Stone Masonry Self-Taught. By Fred. T. Hodgson. 305 pp.
Masonry Construction. By Alfred E. Phillips and Austin T. Byrne. 128 pp.
Building Mechanic's Ready Reference. (Stone and brick masons' edition.)
By H. G. Richey. 255 pp.
Modern Stone Cutting and Masonry. By John S. Siebert and Frederic C.
Biggin. 47 pp.
Masonry and Reinforced Concrete. By Walter A. Webb and W. Herbert
Gibson. 444 pp.
Materials of Construction. Part I. By Adelbert P. Mills.
Practical Masonry. By W. R. Purchase, 226 pp.
Engineering Geology. By Heinrich Ries and Thomas L. Watson.
Building Superintendence. By T. M. Clark.
American Civil Engineer's Pocket-Book. Mansfield Merriman, Editor-in-
Civil Engineer's Pocket-book. By Albert I. Frye.The Civil Engineer's Pocket-Book. By John C. Trautwine.
Architect's and Builder's Pocket-Book. By Frank E. Kidder.
Absorption, see Granite, Limestone,
Absorption tests, 3
Alkali, effect of, 119
Arches, brick, 80
Ashlar masonry, 61, 62, 63
Bond, 60, 64
in brickwork, 78
Brick, absorption, 44
arch or clinker, 42
body or cherry, 42
continuous, kiln, 39
crushing strength, 43
down-draft kiln, 38
dry-clay machines, 34
machine made, 42
modern methods of mfg., 37
modulus of rupture, 43
Brick, ornamental, 45
requirements for good, 43
salmon or pale, 42
sand lime, 45
soft-mud, 34, 42
stiff-mud, 34, 42
up-and-down-draft kiln, 38
up-draft kiln, 38
Brick-work, cleaning, 83
crushing strength, 81
safe compressive strength, 81
Bucket, drop bottom, 102
Building blocks of concrete, 91
Building stones, absorption, 3
axed or pean-hammered, 31
chemical tests, 6
crushing strength, 4
diamond panels, 32
fire-resisting properties, 12
freezing tests, 5
microscopic tests, 6
physical properties, 11
power tools, 24
Building stones, rocks used for, 2
specific gravity, 6
tools used, 20
Bush hammer, 22
Cement, fineness, 51
manufacture of, 53
specific gravity, 51
tensile strength, 51, 52
time of setting, 51, 52
Channeling machines, 14
Chemical tests, 6
Coefficient of expansion, see Granite,
alkali effect, 119
crushing strength, 120
depositing under water, 102
fire-resisting properties, 120
joining old and new, 119
machines for mixing, 90
mixing and depositing by com-
mixing in freezing weather, 101
Concrete, modulus of elasticity, 120
pebble surface, 107
physical properties, 120
plaster surface, 106
proportion of materials, 88
sand-blasted surface, 107
spaded surface, 105, 107
surface finish, 95, 104, 105, 106,
tests of permeable properties, 114
water-proofing, 113, 118
Concrete blocks, surface finish, 95
Concrete building blocks, 91
Crushing strength, see Granite, Lime-
Double-face hammer, 20
Dowels, 60, 69
Drill hammer, 13
Drills, machine, 14
Durability of rocks, 2
Explosives, see Quarrying
Face hammer, 20
Fire-resisting properties of building
Forms, for concrete, 110
wetting and oiling, 111
Freezing tests, 5
Glass seams, 7
Grab hooks, 69
coefficient of expansion, 8
Granite, crushing strength, 8
modulus of elasticity, 8
modulus of rupture, 8
specific gravity, 8
Hand hammer, 22
Hollow terra-cotta, 46
Hollow tile masonry, 84
Joints, 60, see Quarrying
stone masonry, 70
Kilns, see Brick and Lime
paste in cement mortar, 57
paste or putty, 48
shaft kiln, 50
coefficient of expansion, 9
crushing strength, 9
modulus of elasticity, 9
modulus of rupture, 9
specific gravity, 9
Masonry, Ashlar, 61
definitions, 59, 122
Masonry, broken range, 61
Microscopic tests, 6
Modulus of elasticity, see Granite,
Modulus of rupture, see Granite,
Monolithic or mass concrete, 95
lime paste and cement, 57
natural cement, 57
pointing, 58, 71
Patent hammer, 22
Pean hammer, 20
Pick, 13, 20
Pitching chisel, 22
Plaster blocks, 48
Plug and feathers, 13, 24
Pneumatic hammer, 25
Pneumatic plug driller, 24
Pointing, 60, 70, 77
hand tools, 13
References to books, 153
to periodicals, 150
Rocks, argillaceous, 2
Rocks, durability, 2, 3
Rubble concrete, 112
coefficient of expansion, 10
crushing strength, 10
modulus of elasticity, 10
modulus of rupture, 10
specific gravity, 10
Sea water, effect on concrete, 119
coefficient of expansion, 11
crushing strength, 11
modulus of elasticity, 11
modulus of rupture, 11
specific gravity, 11
Slope-wall masonry, 73
Soft-mud, stiff-mud, etc., see Brick
Specifications, arch masonry, 131
bridge and retaining wall-ma-
building brick, 138
Specifications, cement, 144
culvert masonry, 132
dry masonry, 133
plain concrete, 133
stone masonry, 127
Specific gravity of building stones, 6
Splitting chisel, 24
Stone masonry, cleaning, 75
strength of, 73
Stones, dimensions of, 66
Strength of building stones, 4
of stone masonry, 73
Surface finish, concrete blocks, 95
concrete, 95, 104, 105, 106, 107,
Surfacing machines, 25
Sylvester's washes, 82
Terra-cotta or tile, 46
crushing strength, 48
Ties for forms, 111
Tools, see QuarryingTooth axe, 22
Water-proofing, 75, 83, 113, 118
UNIVERSITY OF CALIFORNIA LIBRARY